This book is a practical guide to electron diffraction in the transmission electron microscope (TEM). Case studies and e

*534*
*106*
*21MB*

*English*
*Pages (184 pages) : illustrations
[185]*
*Year 2020*

*Table of contents : Cover......Page 1Half Title......Page 2Title Page......Page 4Copyright Page......Page 5Table of Contents......Page 6Abbreviations......Page 10List of symbols......Page 12Preface......Page 14 How a lens forms a diffraction pattern......Page 16 Introduction to diffraction in the TEM......Page 19 SAD in the TEM......Page 22 Limitations to the accuracy of selected-area diffraction......Page 23 Diffraction using small probes......Page 26 Spatial resolution......Page 29 Problems with specimens......Page 31 Beam damage......Page 32 Obtaining and recording a SAD pattern in the TEM......Page 34 STEM mode......Page 36 Alignments that are important for diffraction......Page 37 Electrons as waves......Page 40 Interference of waves......Page 41 Bragg's Law......Page 43 The reciprocal lattice......Page 46 The 180° ambiguity in indexing the diffraction pattern......Page 50 Diffraction patterns from amorphous materials......Page 52 Systematic absences......Page 53 Cubic patterns......Page 55 Hexagonal close-packed patterns......Page 57 Input data......Page 60 Measuring the pattern and indexing it – an example......Page 63 Calibration of the camera constant......Page 64 Calibration of the rotation between the image and the diffraction pattern......Page 65 Using electron diffraction to identify unknown phases......Page 67 Exercises......Page 68 The reflecting sphere......Page 70 Second-phase particles or precipitates......Page 75 Twinned crystals......Page 76 Determining habit and composition planes......Page 77 The importance of crystal orientation......Page 79 Dark-field imaging......Page 80 Exercises......Page 81 How Kikuchi lines form......Page 84 Kikuchi maps and their uses......Page 89 Exercises......Page 93 The structure factor, Fhkl......Page 96 Systematic absences due to lattice type......Page 98 Systematic absences due to translational symmetry elements......Page 99 The kinematic and dynamical theories of electron diffraction......Page 103 Measuring the structure factor, Fhkl, and the extinction distance, ξ......Page 104 Exercises......Page 105 Determination of the crystal system from conventional electron diffraction patterns......Page 106 Zonal repeats parallel to the electron beam......Page 107 Geometry of CBED patterns from HOLZs......Page 109 The symmetry of CBED patterns......Page 111 The Tanaka method......Page 121 Exercises......Page 124 Double diffraction......Page 128 Double diffraction of 'forbidden' reflections......Page 130 Detection of double diffraction in the microscope......Page 131 Diffraction from small particles......Page 134 The distribution of streaks in the diffraction pattern......Page 135 The effects of elastic strain......Page 136 Long-range order......Page 137 Short-range order......Page 138 Spinodal decomposition and other compositional modulations......Page 140 Periodic antiphase domain boundaries......Page 141 Regular dislocation arrays......Page 142 Planar and linear defects......Page 143 Exercises......Page 146 Appendix A: Some basic crystallography......Page 148 Appendix B: An introduction to space groups......Page 156 Appendix C: Some useful crystallographic relationships......Page 162 Appendix D: Relativistic electron wavelengths......Page 166 Appendix E: Mathematical definition of the reciprocal lattice......Page 168 Appendix F: Computer programs concerning electron diffraction......Page 170 Appendix G: Answers to exercises......Page 172 Appendix H: References......Page 178Index......Page 182*

MICROSCOPY HANDBOOKS 47

Electron Diffraction in the Transmission Electron Microscope

Royal Microscopical Society MICROSCOPY HANDBOOKS Series Advisors Angela Kohler (Life Sciences), Alfred Wegener Institut, Notke-Strasse 85, 22607 Hamburg, Germany Mark Rainforth (Materials Sciences), Department of Engineering Materials, University of Sheffield, Sheffield Si 3JD, UK 08 09 20 21 25 26 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47

Maintaining and Monitoring the Transmission Electron Microscope Qualitative Polarized Light Microscopy The Operation of Transmission and Scanning Electron Microscopes Cryopreparation of Thin Biological Specimens for Electron Microscopy The Role of Microscopy in Semiconductor Failure Analysis Enzyme Histochemistry Food Microscopy: a Manual of Practical Methods, Using Optical Microscopy Scientific PhotoMACROgraphy Microscopy of Textile Fibres Modern PhotoMICROgraphy Contrast Techniques in Light Microscopy Negative Staining and Cryoelectron Microscopy: the Thin Film Techniques Lectin Histochemistry Introduction to Immunocytochemistry (2nd Edn) Confocal Laser Scanning Microscopy Introduction to Scanning Transmission Electron Microscopy Fluorescence Microscopy (2nd Edn) Unbiased Stereology: Three-Dimensional Measurement in Microscopy Introduction to Light Microscopy Electron Microscopy in Microbiology Flow Cytometry (2nd Edn) Immunoenzyme Multiple Staining Methods Image Cytometry Electron Diffraction in the Transmission Electron Microscope

Electron Diffraction in the Transmission Electron Microscope

P. E. Champness Department of Earth Sciences, University of Manchester, Manchester M13 9PL, UK

@ ....,

Taylor & Francis Taylor & Francis Group

LONDON AND NEW YORK

© Taylor & Francis 2001 First published by Taylor & Francis 2 Park Square, Milton Park, Abingdon, Oxon, OX14 4RN 52 Vanderbilt Avenue, New York, NY 10017 Transferred to Digital Printing 2008 All rights reserved. No part of this book may be reproduced or transmitted, in any form or by any means, without permission. A CIP catalogue record for this book is available from the British Library. ISBN 1 85996 1479

Production Editor: Paul Barlass. Typeset by Marksbury Multimedia Ltd, Midsomer Norton, Bath, UK.

Front cover: [001] Tanaka CBED pattern of the 24R polysome of the AI, Sn oxide mineral nigerite (see Figure 6.1) and [111] schematic Kikuchi map for diamond cubic crystals (see Figure 4.7). Publisher's Note The publisher has gone to great lengths to ensure the quality of this reprint but points out that some imperfections in the original may be apparent.

Contents

Abbreviations

IX

List of symbols

Xl

Preface 1.

2.

XUI

Diffraction and the electron microscope

1

How a lens forms a diffraction pattern Introduction to diffraction in the TEM SAD in the TEM Low- (or small-) angle diffraction Limitations to the accuracy of selected-area diffraction Diffraction using small probes Spatial resolution Problems with specimens Specimen preparation Beam damage Obtaining and recording a SAD pattern in the TEM Obtaining a CBED pattern TEM mode STEM mode Alignments that are important for diffraction

21

21

21

22

The reciprocal lattice and Bragg's Law

25

Electrons as waves Interference of waves Bragg's Law The reciprocal lattice The 180 ambiguity in indexing the diffraction pattern Diffraction patterns from polycrystalline materials Diffraction patterns from amorphous materials Systematic absences Standard patterns Cubic patterns Hexagonal close-packed patterns Patterns from the diamond structure

25

26

28

31

35

37

37

38

40

40

42

45

0

1

4

7

8

8

11

14

16

16

17

19

v

vi

Electron Diffraction in the TEM

Computer indexing of electron diffraction patterns Input data Measuring the pattern and indexing it - an example Calibration of the camera constant Calibration of the rotation between the image and the

diffraction pattern Using electron diffraction to identify unknown phases Exercises

3. The reflecting sphere The reflecting sphere Obtaining orientation relationships Second-phase particles or precipitates Twinned crystals Determining habit and composition planes The importance of crystal orientation Dark-field imaging Exercises

4. Finding your way around reciprocal space:

45

45

48

49

50

52

53

55

55

60

60

61

62

64

65

66

Kikuchi diffraction

69

How Kikuchi lines form The determination of the deviation parameter s Kikuchi maps and their uses Finding the exact orientation of the crystal Exercises

69

74

74

78

78

5. The intensities of reflections The atomic scattering amplitude, f The structure factor, F hkl Systematic absences due to lattice type Crystal with a simple structure Systematic absences due to translational symmetry elements The kinematic and dynamical theories of electron diffraction Measuring the structure factor, F hkl , and the extinction

distance, ~ Exercises

81

81

81

83

84

84

88

89

90

6. Determination of the Bravais lattice, point group and

space group

91

Determination of the crystal system from conventional

electron diffraction patterns Convergent-beam methods Zonal repeats parallel to the electron beam

91

92

92

Contents

7.

vii

Geometry of CBED patterns from HOLZs The symmetry of CBED patterns The Tanaka method Exercises

94

96

106

109

The fine structure in electron diffraction patterns

113

Double diffraction Double diffraction of 'forbidden' reflections Double diffraction of spots from precipitates and twins Detection of double diffraction in the microscope Diffraction from small particles The distribution of streaks in the diffraction pattern The effects of elastic strain Diffraction from ordered structures Long-range order Short-range order Periodic and modulated structures Spinodal decomposition and other compositional modulations Periodic antiphase domain boundaries Regular dislocation arrays Incommensurate structures Planar and linear defects Thermal diffuse scattering Exercises

113

115

116

116

119

120

121

122

122

123

125

125

126

127

128

128

131

131

Appendices

133

Appendix Appendix Appendix Appendix Appendix Appendix Appendix Appendix

Index

A: Some basic crystallography B: An introduction to space groups C: Some useful crystallographic relationships D: Relativistic electron wavelengths E: Mathematical definition of the reciprocal lattice F: Computer programs concerning electron diffraction G: Answers to exercises H: References

133

141

147

151

153

155

157

163

167

Abbreviations

APB CBED CCD FEG FOLZ FWHM FWTM HOLZ K-M relp relrod

SAD

SOLZ STEM TEM ZAP ZOLZ

antiphase domain boundary convergent-beam electron diffraction charge-coupled detector field-emission gun first-order Laue zone full width at half maximum full width at 10th maximum higher-order Laue zone Kossel-Mollenstedt reciprocal lattice point reciprocal lattice rod selected-area diffraction second-order Laue zone scanning transmission electron microscope transmission electron microscope zone-axis pattern zero-order Laue zone

ix

List of symbols

a, b, c a*, b*, c* A Cs d d hkl D E

f f Fhk l ghkl

G hkl (hkl) lhkll H';'

I

ko k L M m n N N N nm pm R s s'

t t u

lattice parameters reciprocal lattice parameters amplitude spherical aberration coefficient spacing of periodic object spacing of lattice planes (hkl) diameter of diffraction aperture energy atomic scattering factor focal length of lens structure factor reciprocal lattice vector radius of HOLZ rings indices of reflection from (hkl) planes Miller indices of a plane form or set of planes related by symmetry spacing of reciprocal layers intensity vector of the incident beam vector of the diffracted wave camera length magnification pitch of screw axis integer h 2 +k 2 +z2 total number of atoms in unit cell order of screw axis nanometre (10- 9 metres) picometre (10 - 12 metres) distance in the diffraction pattern as measured on the film or screen deviation parameter effective deviation parameter thickness of specimen lattice repeat fourth crystallographic axis used in hexagonal and trigonal systems xi

xii

Electron Diffraction in the TEM

[UVW]

v V Vc

x y

x,y,z x", y", zn x*, y*, z*

zone direction family of zones related by symmetry velocity voltage volume of unit cell distance displacement direction of crystallographic axes fractional coordinates of nth atom in unit cell direction of reciprocal crystallographic axes

Greek symbols

a a

2a a, {3, y a*, {3*, y* {3 ,1

Af

AB

4Y 4Y 4Yhkl

S A

Phkl Po

e

primary tilt angle scattering angle convergence angle angles between crystallographic axes angles between reciprocal crystallographic axes secondary tilt angle path difference defocus displacement of Kikuchi line from diffraction spot on film or screen angle between g vectors/normal to planes phase difference phase angle for reflection hkl extinction distance wavelength amplitude of diffracted beam amplitude of undeviated beam Bragg angle

Preface

This text is the result of many years' experience of teaching the elements of electron diffraction to postgraduate students in the University of Manchester and UMIST, and to students attending the annual Royal Microscopical Society School in Electron Microscopy. I have tried to minimize the use of mathematics, but where I considered mathematics unavoidable, I have made the derivations as full as possible. I have also tried to illustrate physical concepts with suitable diagrams, wherever appropriate. My examples have been taken from a range of metals, minerals and ceramics, and I have tried to make the coverage as broad as possible in terms of crystal symmetry. My experience has been that students who are only familiar with the cubic and hexagonal systems come unstuck when confronted with a system of lower symmetry! I also hope that biologists will find the book accessible. The appendices cover material that is not dealt with in the main text. They include a summary of essential crystallography and an introduction to space groups. Other appendices and parts of the text provide tables of data and crystallographic formulae that I hope will provide the reader with a useful source of reference. P.E. Champness

Acknowledgements I am extremely grateful to the following people who have made helpful comments on various parts of the text: Alwyn Eades, Chris Hammond, Peter Kenway, Gordon Lorimer and Jian-Guo Zheng. I am also grateful to Sue Maher, Robin Hadley and Margaret Banton, who printed the photographs, and to Richard Hartley who produced the line drawings from my, often rough, originals. Feridoon Azough, Chris Hammond, Peter Kenway, Gordon Lorimer and Phil Prangnell kindly supplied photographs. A number of copyright holders have permitted me to reproduce figures, the acknowledgement of which is made in the figure captions.

xiii

xiv

Electron Diffraction in the TEM

Safety Attention to safety aspects is an integral part of all laboratory procedures and both the Health and Safety at Work Act and the COSHH regulations impose legal requirements on those persons planning or carrying out such procedures. In this and other Handbooks every effort has been made to ensure that the recipes, formulae and practical procedures are accurate and safe. However, it remains the responsibility of the reader to ensure that the procedures which are followed are carried out in a safe manner and that all necessary COSHH requirements have been looked-up and implemen ted. Any specific safety instructions relating to items of laboratory equipment must also be followed.

1

Diffraction and the electron . microscope

When we look at a distant street light through a finely woven net curtain or an umbrella we see a pattern of bright spots. This pattern is not an image, it is a diffraction pattern. We see a regular array of spots because the fabric of the curtain or the umbrella also has a regular, periodic weave. The pattern that we see is telling us about the periodicity of the weave and its orientation; if you rotate the fabric about a direction perpendicular to its surface, the pattern of spots will also rotate. We will look at this phenomenon in more detail at the end of the next section.

1.1 How a lens forms a diffraction pattern We are most familiar with the use oflenses to form a (usually) magnified image of an object; for instance, with a magnifying glass or an optical microscope. However, any converging lens used in this way is also forming a diffraction pattern. What happens can be understood by reference to Figure 1.1. Here we have a periodic object (it could be a piece of net curtaining) placed in front of a converging lens which is illuminated by a parallel beam of monochromatic (single wavelength) light. Some of the light is transmitted undeviated through the object and some is 'scattered' (some will also be absorbed). The undeviated light travels parallel to the optic axis of the lens and is focused by the lens so that it passes through the principal focal point F 0 at a distance from the lens equal to the focal length, f A plane drawn through F 0 perpendicular to the axis is the back focal-plane of the lens (note that there is a conjugate, i.e. optically equivalent, front focal-plane at a distance f from the lens on the object side of the lens). Light scattered at angles ± IX by the object will form parallel beams which are focused to points F 1 and F l ' in the back focal-plane, at a distance from the axis proportional to the angle IX. This pattern of spots formed when the transmitted and scattered beams are focused into the back focal-plane is the diffraction pattern. In fact, for an infinite, periodic object such as our net curtain the spots are only formed for rays that are scattered in specific directions (we will learn 1

2

Electron Diffraction in the TEM

Figure 1.1. Formation of an image and diffraction pattern by a lens from an infinite periodic object. For parallel, monochromatic illumination, the transmitted and diffracted beams are focused into spots, Fo, F" F, ' etc., which form the diffraction pattern in the back focal-plane of the lens at a distance f, the focal length, from the lens. Only three diffraction spots are shown for clarity. The diffracted beams recombine to form a magnified image in the image plane. Note that the image is inverted with respect to the object, but the diffraction pattern is not. In effect, the screen of the electron microscope is in the plane 1, - 13 in the imaging mode and in the plane F, - F, in the diffraction mode.

the rule that governs these directions later). The rays that form the diffraction spots in the back focal-plane go on to form an inverted image in the image plane. If you follow the three rays shown in Figure 1.1 that are emerging from any of the three apertures Ob O2 or 0 3 of the object, you will find that they end up at the same point in the image (rays from 0 1 end up at 11 for example, as you would expect), each having passed through a different diffraction spot. In other words, information about the object is contained in each diffraction spot. A direct consequence of this effect is that, in order for the lens to form an image of the object (i.e. in order to resolve the weave of the curtain material), at least two diffracted beams should enter the objective lens and be allowed to recombine in the image plane. This principle was first described by Ernst Abbe in the 19th century and is known as the Abbe criterion. If we explore a little further, we find that there is a definite relationship between the periodicity and orientation of the object and the spacing and orientation of the spots in a diffraction pattern. You can easily see what this relationship is if you hold a set of meshes, net-curtain materials or diffraction gratings of varying periodicity in front of a laser pointer (do NOT look directly into the laser beam) or other small torch and view the diffraction pattern produced on the wall on the opposite side of the room. You will find that the spacing of the diffraction spots is inversely proportional to the object's periodicity (for instance, if you halve the spacing of the grating or mesh, the spacing of the diffraction spots doubles) and that the separation of the spots produced by the grating or by the weave of the net is perpendicular to the lines ofthe grating (Figure 1.2). (If you do not have a set of such objects, you can see the size effect by rotating a mesh about the direction of one of the threads, thus effectively shortening the mesh periodicity perpendicular to the direction of rotation.

Diffraction and the electron microscope

3

Figure 1 .2 . Optical diffraction patterns taken with a laser and recorded under the same conditions. (a) Pattern from a diffraction grating with spacing 0.126 mm. The lines of the grating were parallel to the length of the page; notice that the row of diffraction spots is perpendicular to this direction. (b) Pattern from a 100-mesh electron-microscope grid, grid spacing 0 .25 mm. (c) Pattern from a 200-mesh electron-microscope grid, grid spacing 0.125 mm. (d) Pattern from a 400-mesh electron-microscope grid, grid spacing 0 .0625 mm . (e) Diffraction pattern from the rectangular two-dimensional 'crystal' shown in (I) . Note the reciprocal relationship between the spacings in the objects and the spacing of the corresponding row of diffraction spots. Note also that the row of spots is perpendicular to the grating from which it is diffracted.

4

Electron Diffraction in the TEM

The spacing of the corresponding diffraction spots will increase). What we have been looking at in the diffraction pattern is also known as the reciprocal lattice because of the inverse (reciprocal) relationship it bears to the direct lattice - the object.

1.2 Introduction to diffraction in the TEM A transmission electron microscope (TEM) consists of a source of electrons (the electron gun) and a series of electromagnetic lenses, as shown in Figure 1.3 (see also Table 1.1). The most critical components of a magnetic lens are the soft-iron pole-pieces which produce an axially symmetric magnetic field for focusing the electrons. The rest of the lens is a magnetic yoke containing the windings for energizing the lens with a d.c. current. By varying this current, the magnetic field, and hence the

Figure 1.3. Schematic diagram of the lenses and apertures in a modern TEM. The nomenclature shown for the imaging lenses follows that adopted for FEI/Philips instruments. The nomenclature used by other manufacturers is given in Table 1.1. Note: the scan coils will only be present if the instrument is designed for scanning transmission electron microscopy.

Table 1.1. Nomenclature used by different manufacturers for the imaging lenses in a TEM FEI / Philips

JEOL

Hitachi

Objective Diffraction Intermed iate Projector 1 Projector 2

Objective First intermediate Second intermediate Third intermediate Projector

Objective First intermediate Second intermediate First projector Second projector

Diffraction and the electron microscope

5

focal length of the lens, is changed. This ability to change the focal length is one ofthe most important ways in which magnetic lenses differ from glass ones. Another difference is that, unlike the glass lenses in a light microscope, magnetic lenses in an electron microscope, because oftheir construction, size and weight, cannot be moved physically with respect to one another in order to focus the image, although the specimen can be moved up or down in the holder to achieve a certain amount of focusing. We will see some other differences between the two types of microscope later. The specimen is placed in a holder in the front focal-plane of the objective lens (Figure 1.3), i.e. at a distance f in front of the lens. Figure 1.4 shows schematically the ray paths for the imaging system of a TEM that employs three stages of magnification. The magnified image produced by the objective in its image plane serves as an object for the diffraction lens, which produces a second intermediate image, which is further magnified by the projector lens to produce the final image on the fluorescent viewing screen (or on the photographic film which is just

Figure 1_4_ Schematjc diagram showing the imaging system of a TEM. A three-stage magnification system is shown . (a) The ray paths for the imaging mode in which the image formed by the objective lens forms the object for the diffraction lens. Note: in this mode there is an objective aperture in the back focal-plane of the objective lens which restricts the number of diffracted beams that recombine in the image plane. This arrangement improves contrast in the image. (b) The ray paths for the diffraction mode. Here the objective aperture is withdrawn and a diffraction aperture is inserted in the image plane of the objective lens (the first intermediate image). The diffraction lens is weakened (its focal length is changed from fl to fo) so that its object plane is the back focal-plane of the objective lens. Hence, the diffraction pattern is magnified by the projector lens and the diffraction pattern appears on the screen of the instrument. Note that the top part of the diagrams (from the specimen to the first image plane) is identical to Figure 2.1 .

6

Electron Diffraction in the TEM

below the screen). This is the imaging mode (Figure l.4a); the action of the objective lens and the diffraction/projector lenses parallels that of the objective and eyepiece, respectively, in the optical microscope. However, the diffraction lens can be reduced in strength (its focal length is increased from fr to fD) by decreasing the current in the windings so that an image of the diffraction pattern in the back focal-plane of the objective lens is focused on the final screen (Figure l.4b); in other words the 'object' for the diffraction lens in the diffraction mode is the diffraction pattern produced by the objective lens. Referring back to the diagram of a simple lens in Figure 1.1, the screen of the electron microscope is effectively in the plane I 1-Ia in the imaging mode and in the plane F I-FI' in the diffraction mode. The weakening of the current in the diffraction lens is simply achieved by selecting the diffraction mode on the microscope's console. If an aperture of diameter D (called the selected-area or diffraction aperture) is placed in the first image plane (Figure l.4b), and if the objective lens behaves as a 'perfect' lens (i.e. one without aberrations; see Section 1.5), only those electrons passing through an area of diameter DIM in the specimen will reach the final screen, where M is the magnification of the objective lens. This can be seen in Figure 1.5 which shows the virtual aperture produced in the object plane. In practice, D may be about 50 /lm and since M is about 50, the diameter of the area selected is about 1 /lm. The diffraction pattern from this area only is therefore observed. This technique is known as selected-area

Figure 1 . 5 . Ray diagram showing the formation of a selected-area (SAD) pattern . The insertion of a (diffraction) aperture in the image plane of the objective lens results in the creation of a 'virtual' aperture in the object plane. Only electrons falling inside the virtual aperture will pass through into the imaging system; all other electrons (for instance the dashed rays) will hit the diffraction aperture and will not contribute to the image or the diffraction pattern seen on the screen . If the diameter of the diffraction aperture is D and the magnification of the lens is M, then the area selected in the object has diameter D I M . Diagram courtesy of P. B . Kenway.

Diffraction and the electron microscope

7

diffraction or SAD. It allows observation of diffraction patterns from small areas of the specimen so that, among other things, a correlation between features seen in the image and the crystallography of the specimen can be made. Unfortunately, the technique is subject to certain errors, both systematic and random, which are described in Section 1.5. These errors, which are in part due to aberrations in the lens, limit the minimum size of the area that can be selected. Modern TEMs usually have at least two condenser lenses to focus the image of the electron source onto the specimen and five imaging lenses (Figure 1.3) which are given varying names by different manufacturers; I will adopt the nomenclature used for FEIlPhilips instruments. This larger number of imaging lenses allows a greater range of magnification, both of the image and of the diffraction pattern, than is possible with the three-lens arrangement in Figure 1.4.

1.3 SAD in the TEM Once you have chosen the area from which you wish to obtain a diffraction pattern, you only need to: insert a diffraction aperture, select the diffraction mode, select the required camera length (the magnifica tion of the diffraction pattern), remove the objective aperture and focus the pattern. An example of a diffraction pattern from a single crystal taken at two different camera lengths is shown in Figure 1.6. If the area selected is to be accurate, it is important that the image of the specimen is accurately focused in the plane of the diffraction aperture (see Section

Figure 1.6. Diffraction patterns of the mineral titanite (- CaTiSiO s), which is monoclinic ([100] zone axis), taken at camera lengths of (a) 707 nm and (b) 1.43 m, allowing for print size. Note the rotation of about 15° clockwise between the patterns in (a) and (b).

8

Electron Diffraction in the TEM

1.6). The diffraction and the projector lenses are programmed within a given range of magnification (the SA, or selected-area, range) so that the plane of the diffraction aperture (the first image plane) is always focused on the viewing screen. At the same time, the objective lens operates at a more-or-Iess fixed excitation so that it focuses the image in that plane. Further experimental details of how to obtain a SAD pattern are given in Section 1.9.

1.4 Low- (or small-) angle diffraction Some biological and other organic crystals have atomic repeats much greater than 10 nm, and the range of camera lengths available by normal SAD may only give a small diffraction pattern from them (remember the reciprocal relationship that we noticed in Section 1.1 between the object and its diffraction pattern; more detail is given in Section 2.3). For instance, a spacing of 100 nm in the object requires a camera length of 54 metres for 100 kV electrons, if the spacing of the spots in the pattern is to be 2 mm (for how this value is arrived at, see Section 2.3), a minimum value for easy measurement on the negative. This camera length is about eight times larger than the maximum normally available in the SAD mode. Larger camera lengths can be obtained using a different procedure. Here, the objective lens is switched off or reduced to a minimum and the condenser system is focused on the object plane of the diffraction lens. A small spot size (the nominal diameter of the beam at the object), obtained by a strongly excited Cl lens, and a small C2 aperture are essential. The subsequent lenses further magnify the diffraction pattern, and camera lengths of the order of several hundreds of metres can be obtained. Details of the procedure differ from one microscope to another, but the technique can be used with any microscope for which there is a flexibility in control over all the lenses.

1.5 Limitations to the accuracy of SAD The area of the specimen defined by the diffraction aperture in the image plane of the objective lens will not generally correspond exactly to the area from which the associated diffraction pattern comes. There are three sources of error. Firstly, if the image is incorrectly focused, the plane of the diffraction aperture will not coincide precisely with the first image plane and diffracted rays originating from outside the area selected by the aperture will contribute to the pattern. The error involved is proportional to 11f, where !1f is the focusing error. A similar error will

Diffraction and the electron microscope

9

occur if the specimen is not in the eucentric plane (when the specimen is in this plane and the image is in focus , the objective lens current is an optimum value). This is because the focal length of the objective lens, even when accurately focused on the object, will differ by some value !1f from its correct value if the specimen is at an incorrect height. Adjustment of the specimen height is possible on all modern microscopes. The third error in the area selected is caused by spherical aberration in the objective lens; a phenomenon that can only currently be corrected for with a customized (and expensive) lens (Raider et al., 1998; Krivenek et al., 1999). Spherical aberration is a lens defect that causes electrons scattered furthest from the optic axis to be brought to focus closer to the lens than rays that are near-axial (Figure 1.7); in other words, the focal length f is shorter for rays that are scattered at a high angle. Thus, even if you manage to focus the image accurately, diffracted beams coming from areas outside the selected one will contribute to the diffraction pattern. The effect is shown in Figure 1.8, which shows one diffracted beam and the undeviated beam. The undeviated rays from the area x-y in the specimen (the dot-dashed lines) are focused through the principal axial focal-point at 0 in the back focal-plane at a distance equal to the focal length, fo, from the lens. If the lens were perfect, the rays diffracted by the specimen at an angle ex to the optic axis would follow the path shown by the dotted lines, after passing through the lens, and the diffraction spot would appear at B in the back focal-plane. Both the undeviated and diffracted rays would be focused in the normal image plane at YX (note the inversion of the image with respect to the object, as is also apparent in Figure 1.1). A diffraction aperture placed at YX in the image plane would then select the area x-y in the specimen. For a lens with spherical aberration, however, the diffracted ray is more strongly focused along the full line to position C, which is slightly closer to the lens than B and lies in a different (back focal-) plane at a distance fa from the lens. The result is that the image of the object x-y formed by the rays entering the objective lens at angle ex is at Y'-X'; i.e. the end points of the image are displaced distances XX' and YY' (which are unequal) in the plane of the diffraction aperture relative to the image

Figure 1.7. Spherical aberration in a lens. Marginal rays are brought to focus nearer to the lens than near-axial rays. The former therefore have a shorter focal length, f~ , than the latter, f o.

10

Electron Diffraction in the TEM

Figure 1 .8 . The effect of spherical aberration of the objective lens on the accuracy of the area selected by the diffraction aperture. The diagram shows one diffracted beam at an angle cx to the optic axis and the undeviated beam . B is the position of the diffraction spot for a perfect lens and C is the position of the spot for a lens with spherical aberration . C is slightly closer to the objective lens than 0 and B because the focal length, f a.- is slightly shorter for marginal rays than the focal length for axial rays, f o. The image of the object x- y formed by the diffracted rays is at Y'-X', whereas the image formed by the undeviated beam is at V- X. The displacement between the two images is proportional to MC s cx3 where M is the magnification of the objective lens and Cs is the spherical aberration constant for the lens. Diagram courtesy of P.B. Kenway.

from the undeviated beam. These distances are proportional to MCs(i where M is the magnification of the lens and Cs is the spherical aberration constant of the lens. So, for a lens with spherical aberration, the area selected in the object using the diffraction aperture corresponds to XY only for the direct beam; it is displaced by a distance proportional to c s(i for each diffracted beam; in other words each diffracted beam 'selects' a different area of the specimen and the error increases very rapidly with scattering angle because of its dependence on the cube of IX. Thus there is little point in trying to isolate an area smaller than about 0.5 !!m in the specimen. If the magnification of the objective lens is 40 times, this figure translates to an aperture size of 20 !!m in the first image plane. Even with a high-resolution TEM (very low Cs) operating at 300 400 kV, the area that can be isolated for SAD is no better than 0.1 !!m. The accuracy of SAD can be improved if the operating voltage is increased. This is a consequence of the fact that the scattering angle IX is proportional to A, the wavelength of the radiation, and A decreases with voltage (see Appendix D). However, the improvement is not spectacular

Diffraction and the electron microscope

11

as Adecreases from 3.7 x 10- 3 nm for 100 kV electrons to 1.64 x 10- 3 nm for 400 kV electrons, a change of 56%. A more effective (and cheaper!) alternative is described in the next section.

1.6 Diffraction using small probes We can achieve a dramatic decrease in the size of the area from which the diffraction pattern comes by focusing the electron beam down onto the specimen and dispensing with the diffraction aperture in the first image plane. The beam is no longer parallel and the area selected is, to a first approximation, equal to the size of the beam, known as the probe. Convergent-beam electron diffraction (CBED), as the technique is generally known, was first discovered in 1939 by Kossel and Mollenstedt, but has only been developed since the 1970s with the advent of instruments designed for high-resolution microanalysis. The only major problem with using this technique arises in beam-sensitive specimens (see Section 1.8.2) because of the high current densities in the focused electron beam. For such specimens CBED may be impossible, even with the use of a cooling stage and high voltages. As we have seen, in conventional SAD an approximately parallel electron beam is incident on the specimen, and the resulting diffraction pattern from a periodic sample consists of an array of sharp spots in the back focal-plane of the objective lens (Figures 1.1, 1.4, 1.9a). If, instead, the incident beam is convergent (Figure 1.9b), the spots become discs and their diameters depend upon the convergence angle 2a, which, in turn, is controlled by the size of the C2 aperture and the lens configuration (see below). Figure 1.10 shows diffraction patterns in which four different convergence angles were used. As you can see, if the convergence angle is large, the discs overlap and it can be difficult to measure the periodicities in the pattern. In fact, these wider-angle patterns can give us a lot of useful crystallographic information (a topic that will be covered in Chapter 6), but for the moment we will confine ourselves to the situation in which the discs do not overlap and will refer to such patterns as microdiffraction patterns. Sometimes you will come across the term Kossel-Mollenstedt (or K-M) patterns for such patterns and the term Kossel patterns for the situation when the discs overlap. In modern TEMs, a convergent probe may be formed in most operating modes; i.e. the TEM mode (microprobe and nanoprobe) and the STEM (scanning transmission electron microscope) mode. You can form a CBED pattern in the TEM mode in any TEM that can produce a small probe ( ~ lllm in size) with a convergence angle of > 20 mrads. This may not be possible on TEMs made before the late 1970s. Most modern TEMs use a condenser-objective lens, as illustrated in Figure 1.11. The specimen is placed in the centre of the very strong magnetic field

12

Electron Diffraction in the TEM

Figure 1.9. The formation of (a) a conventional (selected-area) electron diffraction pattern and (b) a convergent-beam electron diffraction pattern. In (a) the area AA' is selected by means of an aperture in the first intermediate image plane (see Figure TAb), whereas in (b) the area BB' selected is determined by the probe size. The diameter of the discs in the CBED pattern depends on the convergence angle 2a.

between the pole pieces ofthe objective lens, the upper part of which, the prefield lens, acts as a very strong condenser lens immediately in front of the specimen to focus the electron beam onto the specimen. The second half of the lens is the objective lens that forms the image and diffraction pattern of the specimen. The auxiliary lens (or mini-lens) above the prefield lens in Figure 1.11 has the effect of partially nullifying the converging effect of the prefield lens, allowing a larger area to be illum inated in the imaging mode. When a CBED pattern is formed in the TEM mode all the lenses in the illumination system are used (Figure i.11a) and the electron beam is focused on the specimen using the C2 lens, In the STEM mode of modern TEMs the auxiliary lens is switched off, the first condenser lens is strong (small spot size) and the second condenser lens is either very weak or switched off. In the STEM imaging mode a small probe is scanned over the area of interest using two pairs of scan coils situated below the second condenser lens as shown in Figure 1.3 (see Keyse et al. 1998 for an introduction to STEM techniques). Clearly your TEM must be fitted with a STEM system for you to be able to do this! In this mode the electron beam is focused on the specimen using the objective lens. The convergence angle at the specimen in the STEM mode is several times larger than that obtained in the TEM mode for the same C2 aperture (Figure 1.11b).

Diffraction and the electron microscope

13

Figure 1 .10. Convergent-beam electron diffraction patterns of synthetic Mg2Ge04 spinel (F cubic, a = 0.825 nm) taken using convergence angles of: (a) 1.4 x 10- 3 , (b) 2.3, (c) 4.9 and (d) 8.1 milli-radians. (a) and (b) are referred to as microdiffraction or Kossel- M6l1enstedt (K-M) patterns as their diffracted discs do not overlap; they were taken in the 'microprobe mode' of a Philips 400T TEM using 30 and 50 Ilm C2 apertures, respectively. (c) and (d) were taken in the 'nanoprobe mode' with 30 and 50 Ilm C2 apertures, respectively. The zone axis was near [110).

In the Philips 400 series of microscopes a so-called high-resolution STEM mode, in which both the C2 and auxiliary lenses are switched off, is also available for CBED. Note that in older machines STEM attachments were available, but the electron optical design varied from machine to machine. In the FEIlPhilips range of microscopes (the 400, CM and Tecnai series), a nanoprobe mode is available which uses the same lens configuration as in STEM operation. Here, however, C2 is used to focus the beam onto the specimen, as in the TEM mode. The convergence angles produced in the nanoprobe mode are intermediate in size between those in the TEM and STEM modes for the same size of C2 aperture. The convergence angles produced in the STEM and nanoprobe modes will be too large to produce a microdiffraction pattern in many samples (the patterns shown in Figure 1.i0c and d were both taken in the nanoprobe mode). Details of how to obtain CBED patterns are given in Section 1.9.

14

Electron Diffraction in the rEM (a)

(b)

c, lens

C2 1ens C2 aperture

Auxiliary lens Prefield lens

Specimen

Imaging

objective lens

Figure 1.11 . Schematic ray diagrams for probe formation in a TEM with a condenser-objective lens. The objective lens consists of two parts: the prefield and the imaging objective lenses; the specimen sits between the two. The auxiliary lens has the effect of partially nullifying the converging effect of the prefield lens, allowing a larger area to be illuminated in the imaging mode. (a) TEM mode, (b) mode in which the auxiliary lens is switched off. In STEM operation, the beam is focused using the objective lens. This lens configuration is also used in the so called nanoprobe mode on FEl j Philips instruments. In the nanoprobe mode the C2 lens is used to focus the beam. Note that, although the focal lengths of the auxiliary and prefield lenses are shown as roughly equal. in reality the former is several times larger than the latter. Adapted from Champness PE, Mineral. Mag., 1987, with the permission of the Mineralogical Society, London.

1.7 Spatial resolution What spatial resolution can be achieved using CBED methods? I have said earlier that the resolution is, to the first approximation, equal to the diameter of the electron probe; but what is that? You will find, in manufacturers' brochures and manuals, tables showing nominal probe sizes for different spot sizes and operating conditions (TEM or STEM), but what exactly do these values mean? They are normally the calculated values at 'full width at half maximum', FWHM; in other words, the width of the probe at half its maximum intensity, and assume that the intensity profile of the beam is Gaussian (in a Gaussian probe 50% of the total current is contained within a disc of diameter equal to the FWHM and 90% is contained within the full width at 10th maximum, FWTM), This

Diffraction and the electron microscope

15

assumption may be far from the truth. The images of focused electron probes under various conditions are shown in Figure 1.12, together with their profiles. The probe on the far left is approximately Gaussian in shape, but the others are not. The 'tails' in the intensity distributions of the other probes have been produced by spherical aberration because the probes are highly converging (remember that spherical aberration causes electrons travelling furthest from the optic axis to be brought to focus closer to the lens than rays that are near-axial). For the probe in Figure 1.12d the tail contains an estimated 95% of the total probe current and extends to 1000 nm, despite having a FWHM of only 10 nm. If the probe size is defined as the diameter that contains 90% of the beam current, the spatial resolution for CBED when such a STEM probe is used can be more than 40 times the FWHM, compared with 1.82 times the FWHM for a Gaussian probe. One way of decreasing the convergence angle is to use a smaller C2 aperture (Figure 1.11), at the expense, of course, of beam intensity. But it

Figure 1 .12. Micrographs and schematic drawings of the electron density distributions in electron probes formed under various operating conditions in a Philips EM 400T. A 70-~m C2 aperture was used in each case, and the same excitation of C1 was used in (a), (b) and (c) . In (d) a lower excitation of C1 was used. (a) In the 'conventional' TEM, or microprobe, mode the convergence angle is low and the probe is essentially Gaussian. (b) In the TEM nanoprobe mode, when the auxiliary lens is switched off, the convergence angle is greater and there is significant spherical aberration. This results in a non-Gaussian probe. (c) The STEM mode shows similar characteristics to the nanoprobe mode. (d) A STEM probe with an even higher convergence angle gives rise to an even larger 'tail' in the electron distribution. In (b), (c) and (d) the tails would be reduced if a smaller condenser aperture had been used. Reproduced from Cliff G and Kenway PB, Microbeam Analysis, 1982, with the permission of the San Francisco Press Inc.

16

Electron Diffraction in the TEM

will not be possible to use the ideal size of aperture for each operating condition (unless your microscope has a facility for continually varying cr, see Section 1.10.1) as there are usually only three or four apertures to choose from . To minimize the effects of spherical aberration, in addition to using the most appropriate aperture, the beam must be well aligned, the condenser astigmatism corrected and all the apertures in the illumination system accurately centred. If you are concerned with knowing the characteristics of your probe, the best solution is to photograph it and obtain its profile using a microdensitometer on the photographic image, as shown in Figure 1.12. Another factor that affects the size of the area from which a microdiffraction pattern comes is the thickness of the specimen. This is because, as the beam penetrates the specimen, it spreads out. The beam spreading is proportional to the thickness of the specimen to the power 3/ 2 and inversely proportional to the accelerating voltage (see for instance Williams and Carter, 1996). Thus, it is sensible to use as high a voltage and as thin a sample as possible to attain the highest resolution, though of course very thin samples and very small probes will not produce very intense diffraction patterns and will require long exposures. Although I have sounded a note of caution about nominal 'probe sizes' and beam broadening, it is still possible to obtain microdiffraction patterns from areas as small as 2 nm with current instrumentation and a field-emission gun (FEG). With a LaB 6 gun the equivalent value is about 10 nm. In modern TEMs, diffraction patterns with sharp spots can be obtained from areas a few tens of nanometres in diameter by first creating a small probe in TEM or nanoprobe mode, by using a small C2 (30 !lm or less) aperture, and then defocusing the probe to give parallel illumination. The Riecke diffraction pattern, sometimes called micro-micro diffraction, is then seen when the diffraction mode is selected. There are also a number of scanning methods for obtaining diffraction patterns from small areas which are outside the scope of this Handbook, but are covered by Williams and Carter (1996) and Keyse et al. (1998) .

1.8 Problems with specimens 1.8.1 Specimen preparation The standard methods for preparing biological specimens for the TEM are covered by Misell and Brown (1987), and the methods for non biological specimens are covered by Goodhew (1984) and Williams and Carter (1996). Artefacts may arise in the preparation process that introduce spurious detail into the electron diffraction pattern.

Diffraction and the electron microscope

17

Negative staining of biological samples may result in modification of the structure of the sample and the stain itself may recrystallize under the electron beam. One solution is to dispense with the stain and use a supporting medium such as glucose; an even better method is to observe the specimen in the frozen-hydrated state or to use an environmental cell in which the specimen may be observed in the wet state (Misell and Brown, 1987). Electropolishing of metals sometimes produces a crystalline and/or amorphous oxide film on the surface of the specimen, for example on Mg and AI, and ion thinning may also re-deposit material on the surface of non-metallic specimens. Careful ion polishing will normally remove these surface films.

1.8.2 Beam damage Organic materials such as polymers, proteins etc., together with inorganic salts, such as chlorides and bromides, and some silicate minerals, such as quartz, feldspar and clays, degrade during observation in the electron microscope because of damage due to ionization and/or heating from the electron beam. Often the material becomes amorphous (because the electron beam causes atomic bonds to be broken) and the diffraction pattern is lost (Figure 1.13); other materials transform to different compounds that can be identified by electron diffraction and X ray analysis. Often the damage is so rapid that it is difficult to record a diffraction pattern under normal operating conditions. There are several methods that you can use to minimize this type of beam damage. • Operate at the highest possible kV. (The so-called capture cross section for damage is lower the higher the kV.) • Cool the specimen to the temperature of liquid nitrogen in a specially designed cold-stage. (The use of liquid helium appears only to be a marginal improvement over liquid nitrogen and is a lot more expensive!) • Make preliminary adjustments such as setting the illumination conditions and focusing the pattern in a different area of the specimen from that you intend to use for recording. This can be done automatically on some instruments. • Use a low beam-current and increase the exposure time accordingly. Or use an image intensifier. • Use a short camera length, thus decreasing the exposure required. The pattern can be enlarged later. • Encapsulate the specimen in a thin film of, for instance, carbon or calcium stearate. The protective effect is thought to be the result of the reduction in secondary damage. The diffusion of atomic and molecular species through the specimen is reduced and their recombination with damaged species is increased (see Misell and Brown, 1987).

18

Electron Diffraction in the TEM

Figure 1 .13. Effect of radiation damage on the alkali feldspar albite, NaAISi 3 0 s, at 200 kV on the image (left) and diffraction pattern (right) . (a) After 1 min, (b) 5 min, (c) 12 min. The nominal beam flux was 3.2 x 10- 2 cm 2 . Note that the extinction contours visible in the image in (a) and (b) are no longer visible in the image in (c). The diffraction pattern present initially has disappeared after 12 min and is replaced by a faint diffuse ring . Reproduced from Lorimer GW and Champness PE, High Voltage Electron Microscopy, 1974, with the permission of Academic Press.

The damage suffered by metals under the impact of the electron beam is of a different nature to that described above. This is called knock-on or displacement damage and occurs when electrons knock atoms out of their sites, so is directly related to the beam energy. Light metals such as Al and Mg suffer knock-on damage at 200 kV and, at 400 kV, metals with an atomic weight below that ofTi are damaged (see Williams and Carter, 1996). However, this damage is very slow and does not normally cause a problem for recording electron diffraction patterns.

Diffraction and the electron microscope

19

1.9 Obtaining and recording a SAD pattern in the TEM The complete procedure for obtaining a pattern is as follows. • Select the required field of view; this must be within the SA range of magnification for FEIIPhilips microscopes. Centre the beam and spread it to fill the field of view. • Focus the image by using the Objective focus knob. Note that the image has minimum contrast when the objective aperture is removed and does not wobble when the Wobbler is switched on. • Adjust t he specimen height so that the specimen is in the eucentric plane (to ensure that the specimen is always at the same height for diffraction; i.e. the height for which the camera constant has been calibrated and the objective lens is working at its optimum setting). a. Use the beam stop to mark a prominent feature of the specimen and tilt the specimen by about 20° about the major tilt axis; the image will move across the screen. b. Adjust the specimen height using the z control (the thumbwheel on older Philips models) until the image returns to the centre of the screen. c. Re-zero the tilt, re-centre the image with the specimen translators and re-focus the image. d. Repeat steps a-c until there is minimum movement of the image. Note that on the CM and later series of FEIIPhilips TEMs there is an Autofocus switch which sets the eucentric height; you then only have to refocus the image. Alternatively there is an 'a-Wobbler' control that, when depressed, rocks the major tilt by ± 15° about zero; the z control is then used to adjust the height until the image no longer appears to move about the centre of the screen. • Remove the objective aperture. • Focus the second condenser lens (the Intensity control on FEIIPhilips machines and the Condenser control on JEOL machines) and centre the beam using the Deflection (FEIIPhilips) or Trans (JEOL) control. • Defocus the second condenser lens and refocus the image. • Insert a diffraction aperture (you will have a choice of three or four sizes) and centre it over the region whose diffraction pattern you wish to see. If the aperture does not appear in the image, you will need to remove the aperture, decrease the magnification, spread the illumina tion and re-insert the largest aperture, centre it, and gradually increase the magnification again while keeping the aperture in view with the alignment controls. • On JEOL microscopes depress the Sam/Rock switch and focus the aperture with the Diffraction focus knob. • Select the diffraction mode.

20

Electron Diffraction in the TEM

• Choose the required camera length using the selector switch. (The camera length is changed by variation of the excitation of the intermediate and projector lenses.) Figure 1.6 shows an example of a pattern recorded at two different camera lengths. • Underfocus the second condenser lens (usually an anti-clockwise rotation of the knob) by several coarse steps to obtain a more parallel electron beam. The more C2 is defocused, the sharper the diffraction spots will be. Aperture sizes of 200 J.lm in the first condenser lens, Cl, and 100 J.lm in C2 are typical values for imaging purposes, but if high beam coherence is required in diffraction, for instance for diffraction from materials with large atomic repeats such as biological crystals or polymers, smaller Cl and C2 apertures should be used. Reduction of the Spot size using the Cl control (increasing the excitation of Cl) also increases the coherence of the electron beam (coherence is a difficult concept in physics, but is a way of defining how well the electrons in the beam are 'in step' or 'in phase' with each other; a parallel beam is more coherent than a convergent beam). It should be noted that all these measures for increasing the coherence of the beam will also reduce the intensity of the diffraction pattern and result in the need for longer exposures. Cooling the specimen to the temperature of liquid nitrogen also improves the sharpness of the spots because it reduces thermal diffuse scattering in the specimen, the scattering produced by the thermal motion of the atoms. • Focus the diffraction pattern using the Diffraction focus (FEll Philips) or SAlHD diffraction camera length control (JEOL). This focuses the diffraction lens accurately on the back focal-plane of the objective lens. (If the objective aperture is replaced, you should also see a sharp image of it). • If necessary, the pattern can be centred on the screen using the Diffraction point alignment control (FEIIPhilips) or the shift knob of the Deflector-Projector control (JEOL). In either case this procedure is achieved by deflection coils. It may be necessary to centre the pattern for each camera length. • Correct any astigmatism of the diffraction lens (Section 1.11). • If you want to take a photograph of the pattern, the exposure time needed will depend on the amount of defocus of C2, the type of specimen, etc. The exposure meter cannot be used for this purpose. The only way of finding the correct exposure is by experience or making a series of photographs at different exposure times. If the central beam is very intense compared with the other spots, the beam stop can be inserted and a double exposure taken. The first exposure includes the beam stop and the second is recorded without it for a length of time of about one 10th of the first exposure. An example ofthe use of the beam stop is shown in Figure 1. 6. If you have a CCD (charge-coupled detector) imaging system or an image-plate system you will need to refer to the manufacturer's manual. Note that the CCD camera could be damaged when an intense diffraction pattern is focused on it.

Diffraction and the electron microscope

21

1.10 Obtaining a CBED pattern 1.10.1 TEM mode To form a microdiffraction pattern in the TEM mode the procedure is as follows. • Make sure the specimen is in the eucentric plane and that the image is focused. • Select a small C2 aperture (10-50 ~m in diameter) and centre it. • Decrease the spot size two or three clicks with the Spot size control (the excitation of Cl determines the spot size, which, in turn, determines the size of the area from which the diffraction pattern will be obtained). Remember that decreasing the spot size also decreases the electron-beam current at the specimen (it is proportional to cl). You will probably have to correct the condenser astigmatism as you change the spot size. • Focus the beam down onto the area of interest using the C2 lens control. • Switch to the diffraction mode and remove the objective aperture. The pattern should now be visible. If the discs overlap, you will have to repeat the procedure from the second point using a smaller C2 aperture. Note: on the FX series and later JEOL machines the rJ. Control provides a continuous control of the convergence angle by changing the excitation of the auxiliary or mini-lens. A similar device will soon be available on the FEIlPhilips Technai range. • Use Diffraction focus to focus the image of the C2 aperture at the edge of one of the discs. • You should check that the beam is accurately focused on the specimen. The procedure is to view the central beam through the binoculars and to overfocus (strengthen) either the C2 or the objective (Focus) lens so that an (out-of-focus) image is visible in the disc (Figure 1. 14a). Then weaken the lens and the image will expand to higher magnifications until an inversion point is reached at exact focus (Figure 1.14b). At underfocus, an image will again be seen that is inverted with respect to the image at overfocus (Figure 1.14c).

1.10.2 STEM mode The procedure is as follows: • Obtain a focused image in STEM on the cathode-ray tube (see Keyse et al., 1998 or Williams and Carter, 1996 for a description of the operation in STEM). • Stop the beam scanning by selecting Spot on the STEM console. • You may have to remove the STEM detector if it is above the TEM screen, or lower the TEM screen if the detector is below. Position the

22

Electron Diffraction in the TEM

Figure 1.14. Procedure for focusing a CBED pattern by adjusting the strength of the objective or C2 lens. Under overfocus (a) or underfocus (c) conditions you see an image of the specimen in the central disc, but at exact focus (b) the disc contains non-spatial contrast. Reproduced from Williams DB and Carter ECB, Transmission Electron Microscopy, 1996, with the permission of Plenum Press, New York.

spot on the region of interest. A CBED pattern should be visible on the fluorescent screen of the TEM because the microscope is operated in the diffraction mode during STEM. • You can change the camera length and focus the image of the C2 aperture as in the TEM modes. However, in TEMs in which the C2lens is switched off in STEM operation, the diffraction pattern can only be focused using the objective lens.

1.11 Alignments that are important for diffraction The routine alignments of the illumination and imaging systems that need to be are carried out before operation of the TEM are described by Chescoe and Goodhew (1990). One of these alignments that directly affects the diffraction pattern is correction of the astigmatism in the condenser lens. Astigmatism arises when the lens field is not perfectly symmetrical about the optic axis and results in a 'smearing out' of the image when it is not precisely in focus, and an unsharp image when apparently at focus . In the diffraction pattern, condenser astigmatism results in the diffraction spots being elliptical. Correction of astigmatism in the condenser lens is achieved by adjustment of the condenser stigmators, as described by Chescoe and Goodhew (1990). Astigmatism in the diffraction lens also affects the diffraction pattern; in effect, it makes the magnification of the pattern on the screen or photograph unequal in different directions. 'Ring' patterns (see Section 2.5) show a series of concentric ellipses rather than circles. Any astigmatism is corrected as follows.

Diffraction and the electron microscope

23

• Focus the image of a specimen within the SA range of magnifications and at the eucentric height. • Remove the specimen. • Select a small spot size with the Cl control and centre on the optic axis. • Select the diffraction mode. • Defocus C2 by several coarse clicks to obtain defocused illumination. • Select the required camera length and centre the beam on the screen if necessary. • Adjust the diffraction focus control until the image crossover is visible on the screen (Figure 1.15a) • Adjust the diffraction stigmator controls until the crossover is a symmetrical three-pointed pattern as shown in Figure 1.15b.

Figure 1 .15. Correction of astigmatism in the diffraction lens. (a) Uncorrected; (b) corrected.

Note that not all microscopes have the requisite stigmators to allow this correction.

2

The reciprocal lattice and Bragg's Law

In Chapter 1 we saw how a diffraction pattern is formed by a simple lens in its back focal-plane. We also noted that the pattern is related in a reciprocal fashion to the object from which it comes: a grating, or other periodic object, of spacing d produces a row of spots perpendicular to the grating with a spacing proportional to lid. This reciprocal relationship may, as we shall see, be extended to three-dimensional gratings, i.e. crystals, to give what is known as the reciprocal lattice. If you are not familiar with the crystal systems, Miller indices and zone directions, it is advisable to read Appendix A before tackling this chapter.

2.1 Electrons as waves It is well known that light and electrons have both wave-like and particle like characters. The relationship between their two characters is shown by Planck's equation:

E=hc/ A

where E is the energy of the photon or 'particle', c is the velocity oflight (-,-,3 x 108 ms - I), A is the wavelength (see below) and his Planck's constant (6.6256 x 10- 34 Js). However, it is the wave-like nature of electrons that we need to consider if we want to understand how they interact with crystals to produce diffraction patterns. Electrons and light waves, like water waves, are transverse waves. That means that the disturbance or displacement they produce (in the electromagnetic field in the case of light) is perpendicular to their direction of travel. Figure 2.1 shows the sinusoidal profile of a light or electron wave in which the distance x travelled by the wave from its source is plotted against the displacement y. The maximum value of the displacement is called the amplitude, A, of the wave (the intensity, I, of the wave is simply proportional to A 2 ). The distance between successive maxima (or any two other equivalent points) is the wavelength, A. The wavelength of visible light waves varies between 390 nm (violet light) and 707 nm (red light) (1 nm = 10- 9 m = 10 A). The wavelength of

25

26

Electron Diffraction in the TEM

Figure 2.1 . The displacement y of a wave with distance x. A is its amplitude and A is its wavelength.

electrons depends on their velocity, v, and consequently varies with the accelerating voltage, V, used. The relationship between the velocity and wavelength is given by the de Broglie equation: A=h/mv

where m is the relativistic mass of the electron. The energy given to the electron is: 1 eV=2"mv2

where e is the charge on an electron. Hence: h A= Y!2meV

The wavelengths of electrons calculated from this equation for common values of V are shown in Appendix D. Note that the wavelength for electrons accelerated at 200 kV (2.508 pm) is five orders of magnitude smaller than the wavelength of visible light and is about two orders of magnitude smaller than the size of a typical atom. This is the reason why electrons are diffracted by the atoms in a crystal, but light waves are not; light cannot 'see' the atoms because it is a fundamental law of physics that radiation cannot detect detail in an object that is less than about half its wavelength.

2.2 Interference of waves We must now consider how two or more diffracted waves interact with each other. For waves of the same wavelength vibrating in the same

The reciprocal lattice and Bragg's Law

27

plane, which is what we are mostly concerned with in electron diffraction, the rules that govern their interaction or interference are very simple; the principle of superposition states that the resultant wave can be obtained by the summation of the component waves. Figure 2.2a shows two waves with the same wavelength and amplitude, A , that are in phase, i.e. their maxima and minima coincide. The resultant wave, shown on the right, is a wave of the same wavelength, but with twice the amplitude, 2A. The waves are said to show constructive interference and the resultant amplitude is the maximum that could be achieved by the interference of the two waves. As the wave profiles are identical, if they are shifted by ?C, constructive interference will also be obtained if the path difference, .1, between the two waves is a whole number of wavelengths. On the other hand, if the maxima of one wave coincide with the minima of the other (Figure 2.2b), destructive interference occurs and the resultant displacement and the intensity are zero. In this case, the path difference, .1, is ))2 or any odd multiple of ))2. Waves

Figure 2.2. The superposition of two waves of the same wavelength and amplitude, A. (a) The waves are in phase; constructive interference; path difference nJ.. , where n is an integer. The resultant amplitude is 2A. (b) The waves are out of phase; destructive interference; path difference (n + 1/ 2) 'A..

28

Electron Diffraction in the TEM

with a path difference intermediate between those shown in Figure 2.2a and b will obviously produce a resultant amplitude between zero and 2A.

2.3 Bragg's Law Now that we understand how waves interfere we are in a position to look into how crystals diffract electrons. The situation is more complex than with the diffraction from the one- or two-dimensional gratings and grids that we considered in Chapter 1 because crystals are three dimensional and can contain many hundreds or thousands of atoms in their unit cells or repeat units. However, the equation that is most useful for understanding the geometry of the diffraction process in crystals is remarkably simple. W.L. Bragg envisaged diffraction in crystals in terms of reflections from planes. For this reason, we refer to the diffraction pattern being formed by reflections from sets of planes in the crystal. Figure 2.3 shows three successive crystal lattice planes with Miller indices (hkl) and spacing d hkl , in a projection in which we are looking along the planes, so that they project as lines. A beam of electrons of wavelength .It. is impinging on the planes at a glancing angle e and being reflected by the planes, also at angle B. For the incident beam on the left, X and G are equivalent points for the rays impinging on successive planes P and Q; likewise, X and H are equivalent points on the rays that are reflected. The path difference between rays reflected by P and Q is therefore GY + YR. For there to be constructive interference and a maximum in the intensity of the reflected beam, this distance must be equal to a whole number of wavelengths, .It. (in the figure it is actually shown to be equal to .It.). Looking at the geometry of Figure 2.3 we can see that, since angle GXA equals 90° and

Figure 2 .3 . The Bragg equation. P, Q and R are three successive lattice planes, (hk/) in a crystal. The incoming radiation, wavelength A, is incident on the planes, spacing d hkl at a glancing angle 8 and is reflected by the planes at angle 8. The path difference between the rays reflected by planes P and Q is A, which, by geometry, is equal to 2dsin 8.

The reciprocal lattice and Bragg's Law

29

angle AXP is e, angle PXG equals 90 - e. As PXY is 90°, the angle GXY is equal to e. In the right-angled triangle XGY: sin e= GYld, ... GY =d sin e As GY = YR, the total path difference is 2d sin interference:

e,

and for constructive

2dhkl sin e= nA

where n is an integer representing one, two, three, etc. wavelength path differences. This is Bragg's Law. When this equation is obeyed, e is known as the Bragg angle. Although Bragg's approach considers the radiation to be reflected from crystal planes, there is a very important difference between these 'reflections' and the reflections of light from a mirror: light is reflected whatever the angle of incidence, whereas radiation incident on a set of crystal planes is only reflected or diffracted at the specific angles given by Bragg's Law. This difference is a consequence of the fact that the crystal is three dimensional and specifically that, for rays reflected from the top plane (as with light), the path difference is always zero and the waves always interfere constructively. In light optics, when n = 1 in Bragg's Law we refer to the first-order diffracted beam, when n =2 to the second-order diffracted beam, etc. For diffraction from crystal planes, however, we conventionally write: 2dhkl sin e= le,

i.e. n = 1.

For example, rather than referring to the second-order reflection from the (100) planes, we consider that the radiation is diffracted by planes of half the spacing, i.e. the (200) planes (Figure 2.4). (The Miller indices are reciprocals of the fractional intercepts of the planes on the unit-cell axes, Appendix A.) In terms of Bragg's equation we can write: dhkl ) . d 2 ( --nSIn e=A=2 nh

.

nk niSIn

e.

Figure 2.4. (a) The Bragg condition for the second-order reflection from the (100) planes. If the path difference, GY + YH, between rays reflected by successive planes is 2A, the Bragg equation can be written: 2d,oosin (} = 2A; (b) The same condition, but considered as the first order reflection from the (200) planes. If GY + YH = 2A, then QY + YR = A. This distance is clearly equal to Q'R' + Y' R', the path difference for the (200) set of planes.

30

Electron Diffraction in the rEM

It is clearly more convenient to refer to the '200 reflection' than to 'the

second-order reflection from the (100) planes'. Notice that, when we refer to reflections from planes, we omit the brackets that we use when we refer to the planes themselves; i.e. the (hkl) planes give rise to the hkl reflection. (Note that multiple indices such as 200, 300, etc. are sometimes called Laue indices to distiguish them from Miller indices, which have no common factors.) The angle that the diffracted beam makes with the incident (undeviated) beam is 28 (Figure 2.4a). It follows that the distance from the diffraction spot to the centre of the diffraction pattern is proportional to 28. But from Bragg's Law: sin 8", 8= JJ2d (because 8 is small for electrons: 0.14 or 2.5 x 10- 3 radians for a crystal spacing of 0.5 nm and 200 kVelectrons). In this equation, we can see once again the reciprocal relationship between the spacing of the diffraction spots and the spacing of the crystal planes from which they come. Each set of diffracting planes (hkl), spacing d hkl , produces a spot in the diffraction pattern at a distance R from the centre and in a direction perpendicular to the planes. From Figure 2.5 we can see that: 0

R/L = tan 28",28 (because 8 is small)

where L (called the camera length) is the distance of the specimen from the screen or film on which the diffraction pattern is displayed. In an electron microscope, this is not a physical distance, but a 'projected' distance which varies with the setting of the imaging lenses. We can combine the above equation with Bragg's Law: A= 2dsin 8",2d8, ... dR = AL.

Figure 2 .5. Schematic diagram showing the geometry of the formation of an electron diffraction pattern . On the film, the spot A occurs at a distance R from the central spot, 0 (that formed by the direct beam) in a direction perpendicular to the planes. L is known as the camera length .

The reciprocal lattice and Bragg's Law

31

AL is known as the camera constant and relates the distance of a spot from the origin of the diffraction pattern to the d-spacing of the set of planes from which it comes. The camera constant can be determined using a standard (see Section 2.10), and hence the d-spacing correspond ing to a reflection can be found once R has been measured.

2.4 The reciprocal lattice The angles in Figures 2.3-2.5 have been greatly exaggerated and, in practice, the electron beam is diffracted from crystal planes that are almost parallel to the electron beam. (For a crystal spacing of 0.5 nm the Bragg angle for 200 kV electrons is 0.0025 radians = 0.14°.) If there are several planes parallel to the electron beam, they will each produce a diffraction spot in the electron microscope at a distance ?Lld from the centre of the diffraction pattern and along the direction of the normal to the plane (Figure 2.6). The angle cP that any two spots subtend at the spot from the undeviated beam is equal to the angle between the normals to the planes. When a number of planes are parallel to a single direction, they are said to constitute a zone and the common direction is the zone axis or zone direction (Appendix A). Thus, when the incident electron beam is parallel to a zone axis in the crystal, the diffraction pattern consists of a lattice of spots that bears a reciprocal relationship to the real (direct) lattice of the crystal - the reciprocal lattice. Such diffraction patterns are normally identified by the zone axis to which the electron beam is parallel. It follows that the indices hkl of all the spots in the pattern are

Figure 2.6. Schematic diagram of the formation of a diffraction pattern from a single crystal in the electron microscope. The beam is parallel to a zone axis and two of the planes in that zone are shown. They produce spots 1 and 2 in the diffraction pattern. and the angle 4> that the spots subtend at the spot from the direct beam is equal to the angle between the norma Is to the planes themselves.

32

Electron Diffraction in the TEM

related to the indices ofthe zone axis [UVW] to which the beam is parallel by the Weiss zone law (or zone equation): hU + k V + lW =0 (see Appendix A). We can define the reciprocal lattice as a lattice of spots, each of which represents a set of planes (hkl) of spacing d in the real lattice. Each spot lies at a distance g = lld, the reciprocal lattice vector, from the origin and is aligned in the direction perpendicular to the planes. (Strictly the vector is g and g = I g I is its modulus). This definition allows us to construct the reciprocal lattice for any crystal whose unit cell parameters we know (d spacings of planes can be calculated using the equations in Appendix C). Let us look at the reciprocal lattice for the [001] zone of an orthorhombic crystal. In this system, the axes are at right angles, but a -=f. b -=f. c (see Table A.i). In Figure 2.7a the real lattice is projected onto the (001) plane. It contains the x and y axes, and some of the members of the set of planes (100), (010) and (110) have been drawn in projection as lines. The reciprocal lattice spot for the (100) set of planes will lie along the normal to the (100) planes at a distance: lid 100 = lIa from the central spot, 000, which comes from the undeviated beam, as shown in Figure 2.7b. The 200 spot will lie in the same direction as 100, but at a distance of: lId 200 =2/a. In fact, there will be a row of spots along this direction, consisting of the

Figure 2 .7 . Sections of the direct and reciprocal lattices for an orthorhombic crystal. (a)

Projection of the direct lattice onto the (001) plane; (b) the corresponding [001] reciprocal lattice.

The reciprocal lattice and Bragg's Law

33

100,200,300,400.... reflections. This direction is called the x* axis (a star signifying a parameter in the reciprocal lattice) and the repeat along it is called a* (the vector is a*). In the same way the (OkO) series of planes will produce a row of spots perpendicular to the (010) planes with a spacing: b* = l/d olO = lib.

This is the y* axis of the reciprocal lattice. The (110) set of planes will produce a spot along their normal (Figure 2. 7b) at a distance of:

gllO

1 -= d llO

~1 -+ b 2 a2

(see Appendix C). In fact, you will find that the reciprocal lattice spot for any plane that you draw in Figure 2.7a is along the normal to that plane in Figure 2.7b. The three-dimensional reciprocal lattice for an orthorhombic crystal is shown in Figure 2.8. The third dimension z* is perpendicular to the (001) planes of the real lattice and the repeat along the axis is: e* = 1/do01 = lie.

The following relationship holds for any crystal system, simply by vector addition: ghkl

=ha* + kb*

+ lc* =ghOO +

gOkO

+

gool

In other words, a reciprocal lattice point hkl is found by going h units along a*, k units along b* and I units along c*. For example, in Figure 2.8 the 112 reflection lies one unit along the negative x* direction (-a*), one unit along the negative y* direction (-b*) and two units along the positive z* direction (2c*). Also, for any crystal system: a* = lId lOo ; b*=l / dOlO; e*=1/d o01 ·

Thus, a* is always perpendicular to the plane (100) even when a is not. Also: • x* is always perpendicular to y and z; • y*is always perpendicular to z and x; • z* is always perpendicular to x and y; • a* is the angle between the x* and y* axes and is equal to the angle between the normals to the (010) and (001) planes; • f3* is the angle between the x* and z* axes and is equal to the angle between the normals to the (lOO) and (001) planes; • y* is the angle between the x* and y* axes and is equal to the angle between the normals to the (lOO) and (010) planes. The mathematical definitions of the reciprocal lattice in vector notation are given in Appendix E.

34

Electron Diffraction in the TEM

Figure 2.S . Part of the three-dimensional reciprocal lattice of an orthorhombic crystal. The x', y' and z' axes are at right angles. The g-vector for reflection 112 is shown.

Although the 'real' or direct lattice and the reciprocal lattice look geometrically similar, there is one vital difference between them. Each node ofthe real lattice is identical and anyone can be taken as the origin; in the reciprocal lattice, however, each node is distinct as it represents a different set of planes. The origin of the reciprocal lattice is 000 and represents the undeviated beam. The [010] reciprocal lattice for a monoclinic crystal is shown in Figure 2.9, together with the (010) projection of the real lattice. For this system: a =1= b =1= C, a = y =90°, {3 > 90°. Thus, the x-and z-axes are shown with an obtuse angle {3 between them. In the reciprocal lattice, the spot 100 will lie along the normal to the (100) planes at a distance from the origin of: lid 100 = 1/(a sin f3) =a* or I a* I The sin {3 term arises because the x and y axes are not at right angles, i.e. d lOO = a sin {3. Similarly, the 001 spot will lie along the normal to the (001) planes at a distance:

The reciprocal lattice and Bragg's Law

35

Figure 2.9. Sections of the direct and reciprocal lattice for a monoclinic crystal. (a) Projection of the direct lattice onto the (010) plane; (b) the corresponding [010] reciprocal lattice. Some of the (201) planes are draw in (a). In (b) the corresponding reciprocal lattice point is found in a direction normal to the planes.

lId 001 = lie sin /3 = c*. The resultant reciprocal lattice is a parallelogram in which the angle between x* and z* is ~* which is equal to 180 - /3. As a further example, we will look at the [001] reciprocal lattice of a hexagonal crystal. This crystal system also has axes that are not orthogonal: the x- and y-axes are at 120 (the y angle) and there is a third axis, u, in the (001) plane that is symmetrically equivalent to x and y and at 120 to them (Figure 2.10a). For this reason, as explained in Appendix A, we normally use four indices (the Miller-Bravais indices, order x, y, u, z) to describe hexagonal (and trigonal) crystal planes and the diffraction spots from them. Figure 2.lOb shows the [001] reciprocal lattice section through the origin with a number of the reflections indexed. Here y* is 60 (180-y) and: 0

0

0

a* =b*=_I_- _ 1 d 1010 - -a-s-in-6-0-

0

2.4.1 The 180 ambiguity in indexing the diffraction pattern 0

Every diffraction pattern from a zone axis can be indexed using a positive or negative set of indices, i.e. a particular spot may be indexed as hkl or as hkl (Figure 2.11a, b). If you need to find the orientation of the crystal producing the diffraction pattern with respect to another crystal, two

36

Electron Diffraction in the rEM

Figure 2 .10. Sections of the direct and reciprocal lattice for a hexagonal crystal. (a) Projection of the direct lattice onto the (0001) plane; (b) the corresponding [001] = [0001] reciprocal lattice.

different answers will be obtained for the two different methods of indexing the pattern because they are equivalent to a rotation of the crystal by 180 about the zone axis (Figure 2.11c, d). This ambiguity is irrelevant to most applications of electron diffraction, but needs to be resolved for certain analyses; for example, the determination of the burgers vectors of dislocations. Edington (1975) explains in detail how the ambiguity may be removed. 0

Figure 2 .11 . The influence of reversing the indices on the diffraction pattern in (a) and (b) on the effective position of the specimen in (c) and (d) . Adapted from Edington JW, Electron Diffraction in the Electron Microscope, 1975, with permission of Macmillan Press.

The reciprocal lattice and Bragg's Law

37

2.5 Diffraction patterns from polycrystalline materials Up to now we have dealt with diffraction from single crystals. If the area of the specimen selected by the diffraction aperture contains crystals in several orientations, the diffraction pattern will consist of the sum of the individual patterns. In the case where the specimen consists of very many crystals of random orientation, the spots are so close together that they fall on a series of continuous rings (Figure 2.12) and form a so-called powder diffraction pattern. Each ring comes from one set of planes of spacing d and the radius R of the ring is equal to ALld. There will be one ring from each set of planes in the structure that satisfies Bragg's Law. If AL is known, the d-spacings corresponding to the rings can be calculated.

2.6 Diffraction patterns from amorphous materials A diffuse ring pattern indicates that the specimen is amorphous. Such patterns arise from the support film, e.g. carbon, or areas of the specimen that have no crystallinity. The d-spacings of the diffuse rings roughly correspond to the average nearest and next-nearest atomic spacings in the material. An example of a diffraction pattern from an amorphous phase is shown in Figure 2.13 (bottom right). In this case, the lack of crystallinity is the result of radiation damage by the electron beam.

Figure 2 .12. Electron diffraction pattern from polycrystalline gold: the Miller indices of the planes contributing to the diffraction rings are shown.

38

Electron Diffraction in the TEM

Figure 2 .13. The phase relationships for reflections by lattice planes for (a) (001) and (b) (002) planes in a crystal w ith a body-centred lattice. The dots represent lattice points. The path differences given are relative to the reflected ray from plane A.

2.7 Systematic absences If the lattice of the crystal is not primitive, certain reflections that would otherwise be present in the diffraction pattern have zero intensity; in other words, they are absent. You must be aware of the rules that govern when such reflections are systematically absent or forbidden. Otherwise you may not be able to index experimental diffraction patterns, i.e. to identify the zone axis whose planes are contributing to a pattern and to identify the Miller indices of the individual spots and of the planes from which they come.

The reciprocal lattice and Bragg's Law

39

The ongm of systematically absent reflections will be covered quantitatively in Chapter 5, but here it will be shown how the absences for a body-centred lattice can be derived by taking a more qualitative approach. Figure 2.13 shows the lattice points at the corners and body centre of the unit cell (remember that the lattice points may represent a large number of atoms that form the repeat unit or motif ofthe structure). In Figure 2. 13(a) , a beam of electrons is incident on the (00l) set of planes at the Bragg angle 8001 . That means that the reflected electrons from successive (001) planes A and A' are in phase and have a path difference of A. However, there is an identical plane, B, halfway between the A and A' planes, and electrons reflected from it will be out-of-phase with a path difference of ?J2 compared with the reflection from plane A. Therefore, destructive interference will occur and the resultant intensity will be zero. The planes A, A' and B make up part of the set (002) (halfthe spacing of the (001) planes); in Figure 2.13b, the electrons are incident on these planes at the Bragg angle 8002 ; reflections from successive planes of the set will have a path difference of Aand be in phase. The 002 reflection will therefore be present. Similar arguments show that reflections 400, 600, etc. will be present, but 300, 500, etc. will be absent; 110, 220, 330 .... reflections will all be present, but 111, 333, 555 .... will be absent. Consideration of these absences shows that, for this lattice type, if h + k + l is odd, then the reflection is absent. Table 2.1 shows the conditions for reflections to occur for all the possible lattice types. Figure 2.12 is a powder diffraction pattern from gold. Because we know that gold is a face-centred cubic we can index the powder rings. For cubic crystals: a

d hkl

=

J h2 + k 2 + l2

Table 2.1 . Conditions for reflection for different lattice types Lattice type

Coordinates of lattice points

Primitive, P Body centred, I All face centred, F C-face centred, C B-face centred, B A-face centred, A ' Rhombohedral, R (obverse) 'Rhombohedral, R (reverse)

0,0,0 0,0,0; 0,0,0; 0,0,0; 0,0,0; 0,0,0; 0,0,0;

Conditions for reflection None, all present

1/ 2, 1/ 2, 1/ 2 0, 1/ 2, 1/ 2; 1/ 2, 0, 1/ 2 ; 1/ 2, 1/ 2, 1/ 2, 1/ 2, 1/ 2, 0, 1/ 2 0, 1/ 2, 1/ 2 2/ 3, 1/ 3, 1/ 3; 1/ 3, 2/ 3, 2/ 3

°

0,0,0; 2/ 3, 1/ 3, 2/ 3; 1/ 3, 2/ 3, 1/ 3

° h+k=2n

h + k + 1 = 2n (even)

h, k , 1 all even or all odd

h+I=2n k + 1= 2n h-k-/= 3n

h - k + / = 3n

Conditions for non -standard lattice types A and B, (100) and (010) faces centred respectively, are given for completeness. ' When indexed using hexagonal indices. If rhombohedral axes are used (which is rare) the lattice is primitive. The inverse and reverse rhombohedral cells differ only by a rotation of 180 about the z-axis. 0

40

Electron Diffraction in the TEM

(Appendix C) and we also know from Bragg's Law that: ,\

,\

d hkl = 2 sin () '" 2() '

Therefore: 2() ex: ..jh2

+ k 2 + l2

Thus, for cubic crystals the indices of the rings in a powder diffraction pattern have progressively increasing values of N =h 2 + k 2 + l2 from the centre of the pattern outwards. So the first ring will have N = 1, 2 or 3, depending on whether the lattice is P, I or F (Table 2.2). The first four rings in the Au pattern in Figure 2.12 are therefore: 111, 200, 311 and 222.

2.8 Standard patterns 2.8.1 Cubic patterns For cubic crystals: a

d hkl

Table 2.2. Possible h 2

h2

1 2 3 4 5

6 8 9

10 11 12 13 14 16 17 18

+ k2 + P

=N

+

e

= J h 2 +k2 + l2

+ P values

P hkl

100 110 111 200 210 211 220 300, 221 310 311 222 320 321 400 322, 410 330, 411

for the cubic lattice types I

F

hkl

hkl

110 200

111 200

211 220

220

310 222

311 222

400

400

330, 411

Note that h 2 + k 2 + P cannot equal 7 or 15 because no sums of three squared integers add up to these values. Remember that, in the cubic system, because a = b = c, you can permute the indices to find planes of the same form. For example, 200 is of the same form as 200, 020, 020, 002 and 002 and therefore the d-spacings of all these planes are the same. Also, although they are not planes of the same form, the (300) and (221) planes have the same d-spacing because h 2 + k + P is equal to 9 for both of them.

The reciprocal lattice and Bragg's Law

41

and therefore the ratio of any two d-spacings, d 1ld 2 , and hence the ratio of any two g or R values, in a cubic diffraction pattern is independent of the lattice parameter, a. This means that the diffraction pattern for a particular zone for any cubic crystal with the same lattice type will always look the same, except for scale. Figure 2.14 shows four high symmetry Clow-index) reciprocal lattice planes for each of the three different lattice types that occur for cubic crystals. Although the diffraction patterns of prominent zones can (with practice) be identified by comparing them by eye with the standard patterns, you may find it helpful to measure the patterns to be sure of an identification. For this

Figure 2.14. Four standard diffraction patterns for each of the th ree lattice types found in cubic crystals. They are drawn for the same lattice parameter and camera constant. Ratios of the principal spot spacings and the angles between some of the g-vectors are given . (a) The primitive cubic lattice. All possible reflections are present. (b) The body-centred cubic lattice. The reflections all have h + k + I even. (c) The face-centred cubic lattice. The reflections have h , k and I all odd or all even .

42

Electron Diffraction in the TEM

Figure 2.14. (b)

reason, the ratios of the principal spot spacings and some of the angles between them are given. Another useful thing to remember is that, if you know the camera constant (we will see in the Section 2.10 how to measure this), you can work out d for the spots, using the equation: d = J.L/R. The value obtained can then be compared with calculated or tabulated values of the material concerned. Alternatively, once you have identified the zone axis of a diffraction pattern from an unknown cubic material and indexed the spots, you can find the value of the a lattice parameter from the d-values using the equation above.

2.8.2 Hexagonal close-packed patterns A number of pure metals, for instance Mg, Ti, Zr, have the hexagonal close-packed structure (see Hammond, 2001, for details of the structure).

The reciprocal lattice and Bragg's Law

43

Figure 2.14. (c)

Because the ratio of the unit cell axes cia is approximately a constant for this structure, the diffraction pattern from a particular zone will, like those from cubic crystals, look the same, apart from the scale. Standard patterns of hexagonal close-packed structures are therefore published (Figure 2.15). You should note however that, because the hexagonal system has a lower symmetry than the cubic system, the hexagonal close packed structure gives rise to many more distinct reciprocal lattice planes. This means that the reciprocal lattice sections cannot always be uniquely identified as a result of a quick inspection, and measurement of the pattern may be essential. An example of this ambiguity is shown in Figure 2.15b and d: the [120] = [0110] and [122] = [0112] reciprocal lattices are very similar, both in shape and size.

44

Electron Diffraction in the TEM

Figure 2,15. Six standard diffraction patterns for the hexagonal close-packed structure. Ratios of the principal spot spacings and the angles between the g-vectors are given. The patterns are drawn for a cia ratio of 1.633. The positions of the spots will differ from those shown with a change of cia. The positions marked x show reflections that are 'forbidden', i.e. they are systematically absent (see text for details).

The reciprocal lattice and Bragg's Law

45

The positions marked x in the schematic patterns of Figure 2.15 show reflections that are 'forbidden', i.e. they are systematically absent, not because of the lattice type (which is primitive), but either because of the presence of a symmetry element known as a c-glide plane (see Appendix B) parallel to {l100} in the structure or because all the atoms are in positions of high symmetry, known as special positions, in the unit cell. This kind of absence is covered in Chapter 5 and the reason need not bother us at this point. These 'forbidden' reflections reappear in the diffraction pattern of any sample of normal thickness by a process known as double diffraction (see Section 7.1), so you would be unaware that they were 'forbidden'! You may notice that, for the [120] = [0110] pattern, half the reflections are missing and are not marked x, for instance 0001, 0003, 2111, etc. These reflections are also forbidden for the same reason as those marked x in the other patterns but, in this case, they do not reappear by double diffraction.

2.8.3 Patterns from the diamond structure Diamond, silicon and germanium have face-centred cubic lattices and so show systematic absences in their diffraction patterns when h, k and l are not all odd or all even. However, like the hexagonal close-packed structure, there are two atoms per lattice point and both are in special positions in the unit cell. This leads to extra conditions for reflections to be present: h + k + l is odd or h + k + l = 4n, where n is an integer (Figure 2.16).

2.9 Computer indexing of electron diffraction patterns For any crystal that is not cubic or hexagonal close-packed, indexing of the diffraction patterns is best done with the aid of a computer. There are several programs that generate reciprocal lattice sections (e.g. Figure 2.17). Some will also index experimental patterns for you if you input the d-spacings for two spots and the angle between them. Some programs can be used 'on-line' at the microscope if the instrument has facilities for measuring d-spacings; you may even be able to use the program to tilt the stage of the TEM to the zone axis you want once two other zone axes have been identified! See Appendix F for a list of computer programs concerned with electron diffraction.

2.9.1 Input data The input data for the computer program may simply be the cell parameters and the lattice type, as in the program used to produce

46

Electron Diffraction in the rEM

Figure 2.16. Four standard diffraction patterns for the diamond cubic structure. They are drawn for the same lattice parameter and camera constant as Figure 2. 14 . Rat ios of the principal spot spacings and the angles between some of the g-vectors are given. In addition to the absences for the face-centred lattice, additional absences occur because all the atoms are in special positions in the unit cell. The extra conditions for reflections being present are: h + k + I is odd or h + k + 1= 4n, where n is an integer. Many of these reflections appear in the diffraction pattern by double diffraction, as shown in the figure by crosses.

Figure 2.17, but other programs require the space group and the positions of the atoms to be given. The most comprehensive source of data for the cell parameters, lattice type and space group is the Powder Diffraction File. An example of a card from the file is shown in Figure 2.18. The middle box on the left-hand side gives the crystallographic data. The first line gives the crystal system (Sys.), tetragonal in this case, followed by the space group (S.G.). You can learn more about space groups in Appendix B, but all you need to know at this stage is that the first letter of the symbol is the lattice type; P, or primitive, in this case.

The reciprocal lattice and Bragg's Law

47

Figure 2.17. An adaptation of a diffraction pattern_generated by computer.The [011] zone-axis pattern from plagioclase feldspar which is C-face-centred triclinic with a = 0.8169, b = 12851, c=0.7124 nm, IX = 93.63, f3 = 116.4, r = 89 .46°. Note that the reflections have h + k even.

The second line in the middle box gives the unit-cell parameters, a, b, c, in Angstroms (1 A= 0.1 nm). Where a value is left blank it is implied that it is equal to the one preceding it. In Figure 2.18, for example, a = b as rutile is tetragonal. In the third line the inter-axial angles ri, /3 and Y are shown. In the example these values are not given because, for all tetragonal crystals: ri= /3= Y= 90 As another example, for a hexagonal crystal the values of ri, /3 and y would also not be given because, for all hexagonal crystals, ri= /3= 90 and Y= 120°. The relationship between 0

•

0

21-1276 d

3 . 25

1.69

2.49

3.25

no.

1/1,

100

60

50

100

n toniua Oxide

iC (RutU.)

1/1,

bkl

100 3.25 50 2.487 s.c. 7

2.297 I 2.111 25 Sys. Tetnlonal S.C. P4.f_ (136) 10 2.054 C 0.6442 2.9592 A 4 . 5933 b, 60 1.6174 a {3 D. y Z 2 4.250 1.6237 • 20 Rd. Ibid.

1.4797 10 10 1.4521 1.4243 2 ca ey Sip n '" {3

20 2V 1.3591 D .. p Color

12 Rd. 1.3465 2 1.3041 4 1.2441 No illpUrity over o.oon 2 1.2006 6 1.1702 4 1.1413 2 1.1143 I 1.0936 4 1.0127

110 101 200 III 210 211 220 002 310 221 301 112 311 202 212 321 400 410 222 330

R.d. Cclol A 1.54056

Fih~r

Mono.

Dia.

Cuco(f 1/ 1 J OiffractOMter

Rd. ~~!!""I lure... of Standat'dl. Mono. 25.

'.

zone axes (compare with Figure 2.14a and c). You will also notice that the g vectors for the (220) planes of the matrix and the (111) planes of the precipitate are parallel. Therefore, these two sets of planes must be parallel in the real lattice. The orientation relationship can therefore be written as: (110)matrixil(1 I l)precipitate; [112]matrixll[112]precipitate

(remember that the (110) planes are parallel to the (220) planes). You will also notice that the 111 spot from the matrix and the 110 spot from the precipitate coincide. Thus, we could also have written: (111)matrixll (110)precipitate. I should emphasize that the above relationship is only one way of expressing the orientation relationship between the phases. The zone axes, for instance, could be described by the symbols of anyone of the 24 zones in the set < 112>. It is conventional to give one specific orientation relationship rather than expressing the planes as forms, {hkl}, and the zones as belonging to one of a set < UVW>. The indexing of the planes and directions should be self-consistent, i.e. the quoted direction should lie in the quoted plane, as above.

The reflecting sphere

61

Figure 3 .7 . (a) Diffraction pattern from an as- cast nickel- aluminium bronze alloy. The matrix is face· centred cubic, a = 0.36 nm and the precipitate is primitive cubic, a = 0 .29 nm. (b) The indexed pattern. The matrix reflections are shown as large dots and the precipitate spots are shown as smaller dots. Diffraction pattern reproduced from Hasan F et al., Metal!. Trans., 1982; 13A: 1337- 1345, w ith permission of the Minerals, Metals and Materials Society/ AS M International.

From the coincidence of the I11ma trix and 1l0pre cipitate spots we can conclude that the d-spacings for the corresponding planes are equal, i.e. d ll1m =d llOp , and, using the equation relating d to a, h, k and l (Appendix C), that amatrix1aprecipitate =J 31J 2 =1.22. (The cell parameters of the two phases are 0.36 and 0.29 nm.)

3.2.2 Twinned crystals A twinned crystal is one which consists of two or more parts that are oriented in a specific crystallographic relationship to each other. The

62

Electron Diffraction in the TEM

relationship is normally one in which there is a reflection across a plane (the twin plane) or a rotation of 180 about the twin axis between the lattices of the two individuals. Figure 3.8 shows a diagram of such a twinned crystal in which the relationship is a reflection in the (110) plane. It can also be described as a 180 rotation about the normal to the (110) plane, though this is less obviously apparent. Because a twinned crystal consists of two (or more) orientations of the real lattice, the diffraction pattern from it will show one (or more) superimposed single-crystal patterns. A diffraction pattern in which the twin plane is normal to the plane of the pattern can be used to identify the twin plane. Figure 3.9a is a diffraction pattern from a twinned region of a Ti-6AI-4V alloy which has the hexagonal close-packed structure. Figure 3.9b identifies the reciprocal lattices from the two twin individuals. Comparison of one of the patterns with Figure 2.15e shows that the zone axis is [121] and that the second pattern can be derived from the first by a reflection in the plane normal to the g-vector for the (1011) planes. Therefore, the twin plane is (1011). There are 12 planes in the form {lOll} in the crystal class 6/mmm - (1011), (1011), (1011), (1011), (1101), (1101), (1101), (1101), (0111), (0111), (0111), (0111), i.e. 12 planes that are equivalent in terms of symmetry. Thus, we would expect there to be six orientations of the twins: six rather than 12 because the (1011) and (1011) planes etc. are parallel. 0

0

3.3 Determining habit and composition planes The physical interface between intergrown phases such as precipitates or stacking faults is known as the habit plane and the interface between twin individuals is known as the composition plane. Determination of these interfacial planes is an important element in the characterization of the material containing them. The easiest way to determine the orientation of a planar interface such as the composition planes in Figure 3.9c is to tilt the specimen so that the interface is vertical, i.e.

Figure 3 .8 . Lattice of a twinned orthorhombic crystal. The twin plane is (110).

The reflecting sphere

63

Figure 3.9 . Twinning in a Ti- 6AI- 4V alloy which has the hexagonal close-packed structure, C = 0.4684. (a) Diffraction pattern from the twins. (b) Diagram that identifies the spots from the two twin individuals. One reciprocal lattice is shown as dots and the other as open circles. Underlining of Miller indices is a standard way of indicating that the reflection comes from a twin. The zone axis is [121] = [0111] and the twin plane is identified as (1011). (c) Image of the twins in which their composition plane is parallel to the electron beam. The image is in the correct relative orientation to the diffraction pattern and shows that the composit ion plane of the twins is also (1011). Note the streaking in the diffraction pattern normal to the composition planes resulting from their narrow width (see Section 7 .2). The image was recorded in the dark-field mode using a spot from one of the twinned individuals (arrowed) . As a consequence only one set of twins appears bright in the micrograph. Diffraction pattern courtesy of G.W. Lorimer.

a = 0.2951,

parallel to the electron beam. This is best done in a tilt-rotate stage that has a large range of tilt, usually ± 60°. The procedure is to rotate the sample in the holder until the trace that the interface makes with the sample surface is parallel to the tilt axis. In a side-entry stage, the tilt axis is parallel to a traverse direction of the specimen (the left-hand control in the FEIlPhilips range of microscopes). You need to rotate the specimen until a slight movement of the specimen transverse that is parallel to the tilt axis moves the image of the interface along its length. Then, having made the specimen eucentric, the specimen should be tilted until the image of the precipitate or defect shows minimum thickness and the interface appears sharp. The interface should then be vertical. It is now a simple matter to determine the Miller indices of the interface from the diffraction pattern; taking into account the rotation between the image and the diffraction pattern (see Section 2.11), the interface will be

64

Electron Diffraction in the TEM

perpendicular to the g-vector from the planes forming the interface. The twin interfaces in Figure 3.9c are vertical and the micrograph has been rotated so that it is in the correct relative orientation to the diffraction pattern in Figure 3.9a. The g-vector for the (1011) planes is perpendicular to the composition planes so we can conclude that the composition plane of the twins is (lOll). The twin and composition planes are the same in this case. This is usually, but not always, the case. A further example of the determination of a habit plane in this way is shown in Figure 3.10, which shows small, Cu-rich platelets, known as G-P zones, in a AI-4.5% Cu alloy. The matrix AI is face-centred cubic and the precipitates have the same structure. Again, the image and diffraction pattern are in their correct respective orientation and the precipitate interfaces are vertical. The diffraction pattern is from the [001] zone axis and the two sets of precipitates have interfaces parallel to (100) and (010). Because the (001) planes are symmetrically equivalent to (100) and (010) (the form (1001) there are precipitates parallel to (00l) as well. These are not easily seen in Figure 3.10b because they are perpendicular to the electron beam. In cases where the above technique is not feasible, for instance if it is not possible to tilt the interfaces to the vertical or if the defect is contained within the thin specimen and does not intersect the surface, then trace analysis is appropriate. This technique is described in detail by Edington (1975) and Hammond (1993).

3.3.1 The importance of crystal orientation The diffraction patterns that I have used to illustrate the determination of orientation relationships and habit planes are from low-index (high

Figure 3 .10. Platelets of Cu-rich G-P zones in a AI-4.5% Cu alloy. The AI is face-centred cubic and the precipitates have the same structure as the matrix. (a) [001] diffraction pattern . No separate diffraction spots are seen from the precipitates, but their small width has resulted in streaks perpendicular to their interfaces (see Section 7.2). (b) The image is in correct relative orientation to the diffraction pattern . Diffraction pattern courtesy of P.P. Prangnell.

The reflecting sphere

65

symmetry) zones. These zones are normally the most informative and it is usually only necessary to find one such zone axis in order to be able to determine the orientation relationship unambiguously. Procedures for tilting the sample so that the electron beam is parallel to a particular zone axis are described in Section 4.3. However, there may be times when you can find a parallel zone axis for each phase, but there are no common g-vectors indicating planes that are parallel in each phase. In this case, it will be necessary to tilt to a second zone axis and to record the tilt angle between the two. Any planes that are parallel in the two phases can then be determined by plotting the information on a stereographic projec tion as described by Williams and Carter (1996) and Hammond (1993).

3.3.2 Dark-field imaging The normal method of forming an image in the TEM is to insert the objective aperture around the incident beam in the back focal-plane of the objective lens and to project the image of the specimen formed by the lens onto the viewing screen (Figure l.4a). This procedure excludes most, if not all, of the diffracted beams from interfering in the image plane and areas that are diffracting strongly appear darker in the image than those that are not. In particular, areas where there is no specimen appear bright; hence, the method is called bright-field imaging. If a diffraction pattern consists of the superimposed patterns from more than one phase, the technique of dark-field imaging may be used to determine which spots originate from which phases. The technique consists of allowing a single diffracted beam to pass through the objective aperture, such that the bright areas in the image come from the phase responsible for the spot. The image of the twins in Figure 3.9 was taken in the dark-field mode using a spot from one of the twin individuals (the one that is arrowed in Figure 3.9a). As a consequence, only one set of twins appears bright in the image. Although a dark-field image can be formed by displacement of the objective aperture from the optic axis to the diffraction spot (Figure 3.11a), the image is of poor quality because aberrations and astigmatism are introduced. However, most modern microscopes allow the incident beam to be tilted so that the diffracted beam passes along the optic axis (Figure 3.11b). This is called centred dark-field imaging. The method is as follows. • Adjust the specimen height so that it is eucentric. • Obtain a bright-field image and focus it. • Obtain a diffraction pattern from the desired area. • Decide which hkl reflection you wish to use for the dark-field image. Tilt the specimen so that the spot is as bright as possible. The (hkl) planes should then be at the Bragg angle () to the incident beam. • Underfocus the second condenser lens and mark the position of the incident beam with the beam stop.

66

Electron Diffraction in the TEM

Figure 3.11 . The formation of dark-field images. (a) The objective aperture is displaced so that it allows an off -axis diffracted beam to pass through it. This produces a poor-quality image. (b) The incident beam is tilted so that the diffracted beam is parallel to the optic axis. This produces an image with high resolution. Adapted from Williams DB and Carter CB , Transmission Electron Microscopy, 1996, with the permission of Plenum Press, New York.

• Switch to the dark-field mode and use the dark-field tilt controls to bring the diffraction spot diametrically opposite to the chosen one onto the position on the screen where the incident beam was previously positioned. This spot will now be strong and the (hkl) planes will be at e to the incident beam. The hkl reflection will be weak. • Switch off the dark-field deflectors and insert and centre a small objective aperture. • Switch the dark-field deflectors back on and adjust the dark-field tilt controls so that the hkl reflection is in the centre of the aperture. This should be the only reflection visible in the aperture. • Switch to the image mode. The image is best focused in the bright-field mode. If you find that the illumination moves during this procedure, it is likely that the tilt coils are misaligned. They may be realigned according to the manufacturer's manual.

Exercises 3.1 Figure 3.12 is a diffraction pattern from an Cl-iron specimen which is body-centred cubic, a = 0.2866 nm, containing a face-centred cubic precipitate of Fe2TiSi. Index the patterns from the two phases by comparison with Figure 2.14b and c, and determine the orientation relationship between them. Calculate the lattice parameter of the precipitate.

The reflecting sphere

67

Figure 3.12. Diffraction pattern from an ex -iron specimen which is body-centred cubic , a = 0.2866 nm, containing a face-centred cubic precipitate of Fe2 TiSi. Reproduced from Hammond C, The Basics of Crystallography and Diffraction, 1997, with the permission of Oxford University Press.

3.2 Figure 3.13 is a representation of the diffraction pattern from as-cast nickel-aluminium bronze (eu with approximately 10 wt. % Al, 5 wt. % Ni, 5 wt. % Fe). The matrix is face-centred cubic, a = 0.36 nm and the Fe-rich precipitate, Krv, is primitive cubic, a = 0.29 nm. The matrix spots are shown as dots and the precipitate spots as open circles. Index both patterns with the help of Figure 2.14a and c, and determine the orientation relationship between the matrix and the precipitate.

Figure 3.13. Representation of a diffraction pattern from as-cast nickel- aluminium bronze. The matrix is face-centred cubic and the precipitate is primitive cubic. The matrix spots are shown as dots and the precipitate spots as open circles.

4 Finding your way around reciprocal space: Kikuchi diffraction

All the diffraction phenomena that we have looked at so far have been the result of elastically scattered electrons, i.e. those that have not lost energy. However, as the thickness of the specimen increases, some of the electrons will lose a small amount of energy ( ~ 50 eV). The effects of these inelastically scattered electrons are visible in most spot patterns, such as those shown in Figures 2.24 and 3.5, both as a diffuse halo around the undeviated beam and as an overall faint background intensity. The inelastically scattered electrons can subsequently be elastically scattered (i.e. Bragg diffracted) by lattice planes and produce a phenomenon known as Kikuchi lines. Kikuchi lines will be best seen in diffraction patterns from areas of the specimen that have a low density of defects and are about half the thickness that the beam can penetrate or thicker. If the specimen is thinner than this, only spots will be seen; ifit is very thick, only Kikuchi lines will be seen (see Figures 4.5 and 4.8), whereas areas of intermediate thickness will show both spots and Kikuchi lines (Figure 4.1). Kikuchi patterns are very useful to the electron microscopist because, as we shall see, they facilitate finding your way around reciprocal space and determining the exact orientation of the crystal. A full treatment of the origin of Kikuchi lines requires use of the theory of Bloch waves, but for our purposes the much simplified explanation given below will suffice.

4.1 How Kikuchi lines form The intensity distribution of the inelastic spectrum as a function of scattering angle is shown in Figure 4.2 ; it is at a maximum in the forward direction and falls off with scattering angle. In Figure 4.3a a set of lattice planes (hkl) are shown close to, but not exactly at, the Bragg angle e to

69

70

Electron Diffraction in the TEM

Figure 4.1 . Diffraction patterns from austenitic stainless steel (face-centred cubic) showing spots and Kikuchi lines. Note the pairs of parallel light and dark lines such as AA' and BB'. The incident beam is approximately parallel to [110] and the strongly diffracting reflection is 222. There is a small tilt between each pattern; note how this causes a particular crossover point on the pattern (marked with a dot) to move around the pattern. (a) 222 is exactly on the reflecting sphere (s = 0). (b) The 222 and 222 reflections are equidistant from the sphere (the symmetry position) . (c) The excess Kikuchi line is on the far side of the 222 spot from 000, so s is positive. (d) The excess Kikuchi line is on the near side of the 222 spot from 000, so s is negative.

the incident beam. However, two rays from the inelastic spectrum (see Figure 4.2) are incident on the planes at the Bragg angle and will be diffracted by them as shown. As ray 1 is closer to the forward direction than ray 2, it is more intense (Figure 4.2), and an excess number of electrons over the background will arrive in the back focal-plane at B; correspondingly, there will be a deficiency of electrons at D. Thus, there is a bright line at B and a dark line at D in the diffraction pattern; these are the Kikuchi lines. The bright line is always the one further from the

Finding your way around reciprocal space: Kikuchi diffraction

71

Figure 4 .2. The intensity of the inelastic scattering as a function of scattering angle.

incident beam direction 000. Strictly, if ray 1 is incident on the (hkl) planes, then ray 2 is incident on the (hkl) planes, as the two sets of indices refer to the same sets of planes, but viewed in the opposite sense. Thus, in Figure 4.3a the bright Kikuchi line is associated with the hkl or +g reflection and the dark Kikuchi line is associated with the hkl or - g reflection. The diffracted rays actually form cones of semi-angle 90 - 8, called Kossel cones, and what we see in the diffraction pattern is a pair of parabolas where the cones intersect the Ewald sphere. The parabolas appear as straight lines in the diffraction pattern because the angles involved are very small. The ± g pair of lines and the region between them is known as a Kikuchi band. The angular separation of the pair of lines is 28, their spatial separation in the diffraction pattern in the back focal-plane is g,which of course is the same as the distance of the diffraction spot from the origin of the pattern at 000, and they are perpendicular to the g-vector. It follows that, because a Kikuchi line is parallel to the plane with which it is associated, the angle between any two lines is equal to the angle between the corresponding planes. Each reflection has an associated pair of Kikuchi lines and, if the specimen is tilted, they move as if rigidly attached to it. If the specimen is tilted by a small angle IX, the lines will move a distance r across the pattern on the screen, and, from simple geometry, r=L IX, where L is the camera length. For a camera length of 1000 mm, this means a shift of about 30 mm per degree of tilt. The change in the spot pattern for such a small angle of tilt is nothing like as dramatic as this, as can be seen in Figures 4.1 and 3.5; the intensities ofthe spots change as they move closer to or further away from the reflecting sphere, but their positions do not. It is the dramatic movement of the Kikuchi lines with a small angle of tilt that allows us to use them to determine the exact orientation of the crystal to within about 0.1 degree, as shown below. In order to characterize certain defects such as dislocations and stacking faults, it is important to set up two-beam conditions in which only one set of planes is strongly diffracting, i.e. the relevant reciprocal lattice point lies exactly on the reflecting sphere and the deviation parameter s = O. It is also important that s is positive if you want to form images of defects with good contrast (see Williams and Carter, 1996).

72

Electron Diffraction in the TEM

Figure 4 .3. Ray diagram showing the geometry of Kikuchi lines. (a) The lattice plane (hkl) is close to, but not exactly at, the Bragg angle 11 to the incident beam . G is the diffraction spot hkl. (b) A clockwise rotation of the crystal from its position in (a) has brought the lattice plane to the Bragg condition with respect to the incident beam. Now the bright Kikuchi line passes through the diffraction spot G and the dark line passes through the origin at 000.

Finding your way around reciprocal space: Kikuchi diffraction

73

Kikuchi lines enable you to carry out these tasks, to find the exact orientation of the crystal or of orientation changes, such as across a low angle grain boundary, and to orient the crystal to take a pair of stereo images (see Williams and Carter, 1996); none of these things are possible with the spot pattern alone. Figure 4.4 is a schematic that shows, on the left, four different positions of the diffraction spot relative to the reflecting sphere and, on the right, the positions of the corresponding Kikuchi lines in the diffraction pattern. If you imagine the specimen in Figure 4.3a being tilted clockwise until the bright Kikuchi line 1 passes through the diffraction spot G, then the dark Kikuchi line 2 will pass through the central spot 000, as shown in Figure 4.3b, and the lattice plane (hkl) will be at the exact Bragg angle e to the incident beam, the deviation parameter s = 0 and the diffraction spot will be at its brightest. Thus, to produce two-beam conditions, it is simply a matter of moving to an area of the sample that is thick enough to show both spots and Kikuchi lines in the diffraction pattern, and tilting the specimen until the bright Kikuchi line associated with the spot passes through it and the dark line passes through the centre spot. This is the situation for the 222 spot in Figure 4.1a.

Figure 4 .4 . The positions of Kikuchi lines in the diffraction pattern (on the right) and the corresponding position of the diffraction spot relative to the reflecting sphere (on the left) . The full line represents a bright Kikuchi line and the dashed line represents a dark Kikuchi line. At the symmetry position in (d) the lines are of equal intensity.

74

Electron Diffraction in the TEM

In Figure 4.4b, the diffraction spot is inside the reflecting sphere, so s is positive. This situation can be arrived at from that in Figure 4.4a by a clockwise rotation of the crystal at Q. A clockwise rotation of the crystal in Figure 4.3a from the exact Bragg condition will move the Kikuchi lines so that the dark line lies between 000 and G and the bright line lies on the far side of G from 000, as shown on the right-hand side of Figure 4.4b. In Figure 4.1b, s is positive for the 222 reflection. Conversely, if s is negative (spot outside the reflecting sphere) the Kikuchi lines are displaced so that the dark Kikuchi line is on the far side of 000 from G, as shown in Figures 4.4c and 4.1d. When the hkl and hkl reflections are at an equal distance from the reflecting sphere, as in Figure 4.4d, we say that we have the symmetry condition for those reflections. Our simple explanation of the formation of Kikuchi lines breaks down here because it predicts that, because they are equidistant from G or G' and 0, the two Kikuchi lines should be of equal intensity and indistinguishable from the background. That this is not the case is clear from Figure 4.1b; there is a band of higher intensity bounded by the Kikuchi lines.

4.2 The determination of the deviation parameter s The deviation parameter s is important in the quantitative analysis ofthe contrast seen in images of crystalline material. As we have seen, the sign of s can be obtained from inspection of the diffraction pattern if it contains Kikuchi lines. In addition, the magnitude of s can be obtained from the displacement, !:ill, of the Kikuchi line from the corresponding diffraction spot (Figure 4.3a). At the symmetry position, if eis expressed in radians and because eis small, we can write (Figure 4.4d): s '" g

Also:

e.

gl2 '" 1IJt. x

e.

s =g2A12.

Rearranging:

At the symmetry position, !:ill =R12 and at the exact Bragg condition, s = 0 and !:ill = O. Therefore, by simple proportions: si!:ill = g2 Al2 -;- RI2

or:

S

=g2Jt. x !:illIR.

4.3 Kikuchi maps and their uses We have seen that every pair of planes (hkl) and (hkl) gives rise to a Kikuchi band, i.e. a pair of bright/dark lines, and that, when the planes

Finding your way around reciprocal space: Kikuchi diffraction

75

are parallel to the incident beam, the band is symmetrical about the spot from the undeviated beam. It follows that, at the exact zone axis, the Kikuchi bands from all the planes in the zone are centred on the undeviated beam (Figure 4.5). Thus, if we wish to orient the crystal so that the electron beam is accurately parallel to the zone axis, we need to tilt the crystal so that all the Kikuchi bands intersect at the centre of the pattern. When the electron beam is close to a zone axis, as in Figure 4.6a, the position of the zone axis relative to the undeviated beam can readily be identified. Note that it is easier to see Kikuchi lines if the diffraction aperture is removed and the electron beam is focused more than normal (see Williams and Carter, 1996, Fig. 20.11). This is because a convergent beam samples a smaller area than SAD and a small area is less likely to be deformed. Kikuchi patterns taken exactly along a zone axis have the useful property that they indicate the symmetry of the crystal along that axis. This is illustrated by Figure 4.5, which compares the symmetry shown in the Kikuchi patterns by the [111] germanium and [001] = [0001] magnesium zone axes. Ge is cubic with the diamond structure and Mg is close-packed hexagonal. Both spot patterns show hexagonal symmetry (see Figures 2.14 and 2.15), but the [111] Kikuchi pattern from Ge shows three-fold symmetry, whereas the [001] pattern from Mg shows six-fold symmetry.

Figure 4 .5. Kikuchi patterns in which the electron beam is exactly along a zone axis. In both cases, the specimen is too thick to show diffraction spots. (a) The [111] zone of Ge, showing three-fold symmetry. The narrowest Kikuchi bands correspond to the {220} planes. This pattern can be compared with the schematic Kikuchi map in Figure 4.7. (b) The [001] zone of Mg, showing six-fold symmetry. The prominent bands originate from the {10TO} planes. Reproduced from Levine E et al., J. Appl. Physiol. , 1966; 37: 2141-2148, with permission of the American Institute of Physics.

76

Electron Diffraction in the TEM

Figure 4 .6. (a) A diffraction pattern taken at 100 kV from aluminium with the beam direction close to [011] . (b) Schematic diagram showing the 200 and 311 Kikuchi bands and the position of the undeviated beam 000. The zone direction is at a tilt of 7.5° about the normal to the (200) planes together with a tilt of 0.98° about the normal to the (022) planes.

Kikuchi maps are schematic representations ofKikuchi patterns for a number of zones in which the Kikuchi bands are drawn with a width proportional to g. Maps are published in the literature for the primitive, face-centred and body-centred cubic lattice types, the diamond-cubic structure, and for the hexagonal close-packed structure (e.g. Figure 4.7). They may be computed for any other crystal lattice type using some of the computer packages listed in Appendix F, or you can compile your own experimentally by photographing the Kikuchi pattern at each prominent zone. These maps can be used to recognize zone axes from their symmetry, at least in the simpler crystal systems. They can also be used rather like road maps to tilt the specimen to a desired zone. For instance, if you recognised from its Kikuchi or spot pattern that a diamond-cubic crystal was oriented with the [233] zone axis approximately parallel to the incident electron beam, you would know from the map in Figure 4.7 that tilting the sample along the ± 022 Kikuchi band (the narrowest one) would bring you to the [011] or [111] zone, depending on the direction of tilt. In fact, tilting along the narrowest Kikuchi band (which represents the set of reflections with the largest d-value in the zone) will almost always bring you to a more prominent, lower index, zone (unless you are

Finding your way around reciprocal space: Kikuchi diffraction

77

Figure 4.7. A schematic Kikuchi map for diamond-cubic crystals showing zone axes within about 20° of [111 J. The indices of some of the prominent Kikuchi bands and zones are shown . Note that the indices of only one of the pair of lines that makes up a band are shown. The < 11 0 > zones are 35.26° away along one of the {022} Kikuchi bands in the directions indicated (see Appendix C). Compare with Figure 4.5a.

at the lowest index zone, such as [001], already). When tilting the specimen in this way, it is important that the specimen is initially at the eucentric height (see Section 1.9); if you find that you have to use the minor tilt axis and you do not have software that corrects for its non eucentric behaviour, you may have to return periodically to the image in order to relocate the area of interest, to adjust the specimen height and to focus the image. Alternatively, if spots are visible in the diffraction pattern, the diffraction pattern can be defocused so that an out-of-focus image is visible in the undeviated beam and any movement of the specimen can be compensated for with the specimen traverses. Orienting the crystal so that the beam is along a particular zone axis has become easier now that software is available that will index diffraction patterns on-line and tilt the specimen automatically to the required axis once two other zones have been identified (see Appendix F). You should note, however, that such labour-saving devices are no substitute for understanding what is going on in reciprocal space!

78

Electron Diffraction in the rEM

4.4 Finding the exact orientation of the crystal The Kikuchi pattern can be used to find the exact orientation of a crystal when the incident beam is not exactly along a zone axis. An example is shown in Figure 4.6. The diffraction pattern in Figure 4.6a is from a sample of aluminium in which the incident beam is close to [011]. As the zone axis is at the point at which the Kikuchi bands intersect, this point can be identified and its distance from the incident beam can be measured, as shown schematically in Figure 4.6b. In order to calibrate distance against angle, the spacing ofa pair of Kikuchi lines (or the spacing ofthe corresponding spots), R, is measured; then, as 0= sin - 1(?J2d), 0 can be calculated from the known d-spacing and electron wavelength. R is equivalent to twice the Bragg angle, 29 and therefore the distance X in Figure 4.6b is equivalent to an angle of x =X x (2 02oolR2oo)0. For the example in Figure 4.6, a = 0.404 nm and therefore d 200 = 0.202 nm and 0=0.525° (for 100 kV electrons A=0.0037 nm, Appendix D) (Figure6.4a). R200 = 7.0 mm and X =50 mm; therefore, X= 7.5°. Similarly, the distance Y = 6.50 mm and the corresponding angle y = 0.98°. Thus, the crystal is 7.5° from [011] rotated about the normal to the (200) planes (which is the same as the [100] direction in the cubic system) plus 0.98° from [011] rotated about the normal to the (022) planes (or the [011] direction). The resultant angle of tilt, Z, can be worked out from the formula (Gard, 1971): Tan z=(tan 2 x + tan2 y + tan 2 x tan 2 y)1I2. In this case, the resultant tilt is 7.6°. Note that there is an a 180° ambiguity in the sense of the direction of the resultant tilt, as outlined in Section 2.4.l. For crystals that are not close to a recognizable zone axis, the procedure for finding the exact orientation is described by Williams and Carter (1996).

Exercises 4.1 Calculate the value of the deviation parameter s for the 222 reflection from the stainless steel specimen in Figure 4.1b, c and d . The lattice parameter a = 0.3157 nm and the wavelength was 0.0037 nm (lOO kV electrons).

4.2 Figure 4.8 is a Kikuchi pattern from a spinel which is face-centred cubic. Identify the beam direction from the symmetry of the pattern and identifY the indices of the prominent Kikuchi bands. Determine the cell parameter. Note that the space group of spinel (Fd3m) has, in addition to the systematic absence for the F lattice, the additional absence that for hkO reflections h+ k = 4n, where n is an integer. The

Finding your way around reciprocal space: Kikuchi diffraction

79

Figure 4 .8 . A Kikuchi pattern from a spine I which is face centred cubic.

camera constant was 2.86 nm mm. Which Kikuchi band would you 'travel' along to reach the closest < 110> zone? By what angle would you have to tilt the specimen? 4.3 Figure 4.9 is a diffraction pattern from aluminium which is face centred cubic, a =0.404 nm. The accelerating voltage was 100 kV (11.=0 .0037 nm) The beam is close to the [011] zone direction and the ± 200 and ± 022 Kikuchi bands are indicated. Calculate the tilt needed to bring the zone axis exactly parallel to the electron beam.

Figure 4 .9 . Diffraction pattern from aluminium which is face centred cubic, a = 0.404 nm. The beam is close to the [011] zone direction and the ± 200 and ± 022 Kikuchi bands are indicated .

5

The intensities of reflections

We saw in Section 3.1 that the intensity of a given diffraction spot depends upon the thickness of the crystal and the deviation of the reflection from the exact Bragg position, i.e. the exact orientation of the crystal with respect to the incident beam. Clearly, the intensity will also depend upon the types of atoms that make up the crystal and their positions in the unit cell. In this chapter, we will investigate this dependence and look into the kinematic and dynamical theories of electron diffraction.

5.1 The atomic scattering amplitude, f In Chapters 2 and 3, we looked at diffraction in terms of reflections from lattice planes. In reality, of course, it is the atoms within the structure that diffract, or 'scatter', the electrons, and specifically the electrons and nucleus within them. The atomic scattering amplitude, f, is a measure of the efficiency of an isolated atom in diffracting electrons and is defined as the ratio of the scattering amplitude of the atom divided by that of a single electron; it has the dimensions of length. The value of f falls off rapidly with scattering angle as shown in Figure 5.1 and it does so more rapidly the larger the radius of the atom. Au and Al have about the same atomic radius (0.144 and 0.142 nm, respectively), but that of Cu is slightly smaller (0.128 nm); as a consequence, the scattering factor for Cu falls off slightly less steeply with scattering angle than those for Au and Al. Scattering is also more efficient the higher the atomic number of the atom and the longer the wavelength ofthe electrons (i.e. the lower the accelerating voltage).

5.2 The structure factor,

Fhkl

The structure factor, Fhkh is a measure of the amplitude scattered by all the atoms in a unit cell into the reflection hkl, and, like f, has 81

82

Electron Diffraction in the TEM

Figure 5.1. The variation of the atomic scattering factor, f , with (sin e)/A for Au (Z = 79), Cu (Z = 29) and AI (Z= 13) , showing that elastic scattering decreases with angle away from the undeviated beam (e = 0°) and increases with the atomic number, Z. f has dimensions of length .

dimensions oflength. However, Fhkl is not a simple sum of all the values offbecause we have to take into account the phase difference between the waves scattered by the individual atoms in the summation. In Section 2.2, we met the concept of the path difference, L1, between scattered rays. The phase difference, 4Y, is a way of expressing the extent that the rays are out-of-step or out-of-phase with each other as an angle, rather than as a distance. A path difference A. between two rays is taken to be equivalent to a phase difference of 360 or 21t radians. Therefore, by proportions, a path difference of L1 is equivalent to a phase difference of 4Y = L1 x 2rt!A. radians. Fhkl is normally expressed as a vector or as a complex number (for an introduction to vectors and complex numbers and their use in crystal lography, see Hammond, 2001): 0

N

Fhkl =

N

L

fn(cos 4Yn+sin i4Yn) = L fnexp i4Yn= I Fhkll exp ihkl n=l n=l

= I Fhkll (cos hkl+i sin hkl)

where N is the total number of atoms in the unit cell, the subscript n denotes the nth atom, I Fhkl I is the modulus of F hkl , hkl is the phase of the resultant reflection hkl and i = H. The intensity diffracted by the unit cell into the hkl reflection, hkl, is the square of the amplitude F hkl : hkl = F hkl

X

F* hkl =

(n~l fn cos 4Yn)

2+ (

n~l fn sin 4Yn)

2

where F*hkl is known as the complex conjugate of Fhkl and is equal to I Fhkll (cos hkl-i sin hkl)' (If a complex number is expressed as z =x + iy, then its complex conjugate is z* = x - iy and z.z* = x 2 + y2.) The intensity is a scalar, rather than a vector or complex, quantity. To evaluate Fhkl we need to know how to calculate 4Yn, and hence hkl. I will take a semi-quantitative approach; the full mathematical treatment can be found in Hammond (2001) or Williams and Carter (1996).

The intensities of reflections

83

Figure 5.2 shows a projection of an orthorhombic unit cell onto the (001) plane and four atoms, with the trace of the set of planes (hOO) (where h = 6) indicated. If we assume that the atom A, for which the x coordinate is zero, scatters the electrons into the hOO reflection with a path difference .1 = 0 and a phase angle 4> = 0; the atom A' in the equivalent position to A in the next unit cell, i.e. with x = a, will scatter the electrons with a path difference hA and a phase angle of 2nh radians and atom B, with x coordinate alh on the first (hOO) plane from the origin, will scatter with a path difference of A and a phase angle 2n. By simple proportions, atom C with an arbitrary x coordinate aX n will scatter into the hOO reflection with a path difference Ahxn and a phase angle of 4>n = (2nIA).Ahxn = 2nhx n. Thus, we can associate a distance ofaxn along the x-axis with a phase angle of 2nhxn. Similarly, an atom with a fractional coordinate Yn along the y-axis would scatter electrons into the OkO reflection with a phase angle 2nkYn and an atom with a fractional coordinate Zn along the z-axis would scatter electrons into the OOl reflection with a phase angle 2nlz n. In the general case, the phase of electrons scattered into the hkl reflection by an atom with fractional coordinates XnYnZn will be: 4>n =2n(hx n + kYn + lZn).

We normally use the equation for the structure factor for the unit cell in its exponential form because this makes evaluation of the equation easier. The equation therefore becomes: N

Fhkl

= 2: fn n= l

exp 2 ni(hxn + kYn + lZn).

5.2.1 Systematic absences due to lattice type Using the equation for F hkl , we are now in a position to derive mathematically the systematic absences for a lattice type. We will take

Figure 5 .2. Projection of a unit cell on (001) and four atoms A B, C and A' (the atoms A and A' are equivalent). The planes (hOO) (h = 6) are shown in projection as dashed lines. The black dots are lattice poi nts.

84

Electron Diffraction in the TEM

the body-centred lattice as an example (see Figure 2.13). For every atom at Xn, Yn, Zn there is an identical atom at Xn + 1/2, Yn + 112, Zn + 112 (see Appendix A). The structure factor becomes: N/2

F hkl = l: fn [exp2 rci(hxn +kYn +lzn)+exp2 rci{h(x n + 1I2)+k(Yn + 1I2)+l(zn+1I2)}] n= l

N /2

= l:fn[exp2rci(hxn+kYn+lzn) x {1+exp2 rci(h+k+l)/2}]. n= l

Now, as expnrci = (_l)n: Fhkl

=

N /2

l: fn [exp 2 rci(hxn + kYn + lZn) if h + k + l is even and

n=l Fhkl

if h + k + l is odd.

= 0

So, reflections that have h + k + l odd are absent, as we noted in Table 2.1.

5.2.2 Crystal with a simple structure Caesium chloride, CsCl, is cubic and has one Cs and one Cl atom in the unit cell. If Cs is taken to be at the origin of the unit cell then Cl is at the body centre. (Note that the lattice is not body centred, however, as the atoms are not identical; it is primitive, each lattice point representing one Cs and one Cl.) If we take Cs at the origin, 000, then Cl is at 112, 1/2, 112. The structure factor is: Fhkl

=fcs exp 2rci(0) + fCI exp 2rci[hl2 + kl2 +lI2] =fcs + fCI

if h + k + l is even

=fcs-fcI

if h + k + l is odd.

Thus, the reflections that are absent if the lattice type is truly body centred are equal to the difference in the atomic scattering factors, and therefore weak, for the primitive CsCl structure.

5.2.3 Systematic absences due to translational symmetry elements If you are not familiar with translational symmetry elements and space groups, it is suggested that you read Appendix B before tackling this section. Space-group symmetry elements that involve translation result in systematic absences, although in most cases the systematically absent spots do occur in the diffraction pattern by double diffraction (see Section 7.1.1). A c-glide plane parallel to (010) is taken as an example. For every atom at Xn, Yn, Zn there is an identical atom at Xn, -Yn' Zn + 112 (Figure 5.3). Substituting these two atomic positions, the structure factor becomes:

The intensities of reflections

85

Figure 5.3. Schematic diagram showing the operation of a c glide plane parallel to the (010) plane. For every atom at fractional coordinates Xn , Yn , Zn there is an identical atom at Xn , - Y n' Zn + 1/ 2. The dashed line is the symbol for a glide plane with translation within the plane of projection .

F hkl =

N /2

L

n=l

fn [exp 21ti(hxn + kYn + lZn>+ exp 21ti(hxn - kYn + l(zn+ IJ2})]

N /2

L fn exp 21ti(hxn + kYn + lZn)[l + exp 21ti( - 2kYn + 1I2)], n=l For the case when k is zero: =

F hOl =

N /2

L

n=l =0

fn exp 21ti(hxn + lZn) [1 + exp 2 1ti(1I2)]

if l is odd.

In other words, hOl reflections are absent if l is odd (Figure 5.4). Other systematic absences due to translational symmetry are shown in Table 5.1.

Figure 5.4 . Schematic diffraction pattern of the [010] zone of an orthorhombic crystal that has a c glide plane parallel to (010) . All the reflections that appear in the pattern have I even (black dots) . The systematically absent reflections are shown as open circles.

86

Electron Diffraction in the TEM

Table 5.1 . Conditions for reflection for translational symmetry elements Symmetry element

Symbol

Class of reflection

Conditions for reflection

Glide plane / / (100)

b

Okl

k I k k

c

n

d Glide plane / / (010)

a

c

hOI

n

d

Glide plane / / (001)

a b n

hkO

d Glide plane / / (110)

c

hhl

n d

h I h h h k h h

+ +

I I

= = = =

2n 2n 2n 4n

+ +

= = I = I =

2n 2n 2n 4n

+ +

= 2n = 2n k =2n k = 4n

I I 2h

+

=2n =2n I = 4n

Screw axis / / x

2,.42 4,.43

hOO

h h

= 2n =4n

Screw axis / / y

2,.42 4,.43

OkO

k k

= 2n = 4n

Screw axis / / z

2,.42, 6 3 3, ,3 2,6 2,6 3 4,.42 6, ,6 5

001

Screw axis / / [110]

2,

hhO

= = = = h

2n 3n 4n 6n

= 2n

n = odd integer, 2n = even integer etc. Note: systematic absences for lattice types are given in Table 2.1.

The systematic absences for all the 230 space groups are given in the International Tables for X-ray Crystallography, Volume I (Henry and Lonsdale, 1952) or the more recent International Tables for Crystal lography, Volume A (Hahn, 1984). The example shown in Figure 5.5 is the entry for P4 2/mnm (full symbol P4 2/m 21/n 2/m), which is the space group ofrutile (see Figure 2.18). The lattice is primitive and the structure has a 42 screw tetrad axis parallel to the z-axis with a mirror plane perpendicular to z (symbol 4z1m); screw diads parallel to the x- and y axes and diagonal glide-planes perpendicular to them, (symbol 21/n); diads parallel < 110> and a mirror plane parallel to the {110} planes (symbol 2/m). The right-hand column in Figure 5.5 lists the conditions limiting possible reflections (i.e. the conditions are those that need to be fulfilled for the reflections to be present) and the first group of entries (headed General) apply to any crystal with this space group. The only condition listed is for Okl reflections, for which k + 1= 2n. This is the result of the n-glide plane parallel to the (100) plane in the space group. The x and y-axes are symmetrically equivalent in the tetragonal system and there is therefore also an n-glide plane parallel to (010), which leads to

The intensities of reflections

P~/mnm

Dita

No.

136

P 4Jm 2./11 2/m

4/11/ m 11/

87

Tetragonal

Origin at centre (mmm)

Pi_ oK pooition&,

Co-ordinates or equiYllient positions

..:'=~

Condition. Umitin• possible reIIec:tion. General:

x,y,z; x,y,l; y,x,z; y,x,l;

R,j,z; R,j,l; j,R,z; j,R,I;

l+x.l-y.l+z; l+x.l-y.l-z; l+y.l-x.l+z; I+y.l-x.l-z;

l-x.l+y.l+z; l-x.l+y.l-z; l-y.l+x.l+z; l-y.l+x.l-z.

16

k

j

8

j

m x,x,z; R,R,z; l+x.l-x.l+z; l-x.l+x.l+z;

8

j

m x.y.O; R.j.O; l+x.l-y.l; l-x.l+y.l;

8

Ir

4

g

mm

x,R.O; R,x.O;

l+x.l+x.l; l-x.l-x.l·

4

/

mm

x,x,O;

l+x.l-x.l; l-x.l+x.l·

4

r

mm

0.0,z; 0.0,1; I.U+z; I.U-z.

4

d

4

c

2

b mmm

0.0.1; 1.l.0.

2

a mmm

0.0.0; I.M.

Irk/: No condition.

IrkO: No condition.

0Ic/: k+I-2n

Irhl: No conditions

Special: as above. plus

x,x,l; R,R,I;

y,x.O; j,R.O;

l+x.l-x.l-z; l-x.l+x.l-z.

I+Y.l-x.l; l-y.l+x.l.

2 O.!,z; 0.1,1; O.U+z; O.U-z;

1.0.z; 1.0,1; 1.0.1+z; 1.0.I-z.

a 0.1.1; 2/m

.f,.f,O;

group number

1.0.1; O.I.t; 1.0.t.

0.1.0; 1.0.0; O.l.l; l.O.i.

Irkl: lr+k-'1II; 1-'111

} no extra conditions

Irkl: lr+k+I-2n } Irkl: lr+k-'1II; 1-'111

} Irkl: lr+k+I= 2n

Figure 5.5. Symmetry information as given in the old edition (Henry and Lonsdale. 1952) of the International Tables for Crystallography for space group number 136, P4 2 /mnm (full symbol P4 2 /m2,/n2/m) .

the (unstated) condition that for hOl reflections h + l =2n. The conditions for the two screw axes are not given specifically as they are conditions that are referred to as 'tied' to those for the n-glide planes; the screw tetrad parallel to the z-axis gives rise to the condition that for OOl

88

Electron Diffraction in the TEM

reflections, 1= 2n and the screw diads parallel to the x- and y-axes give rise to the condition that for hOO or OkO reflections, h or k = 2n, respectively (Table 5.1). All of these conditions are special cases of those stated above for the n-glide planes. The special conditions listed below the general conditions only apply if all the atoms are in the special equivalent positions in the unit cell whose coordinates are listed in the central column. Many of the computer programs listed in Appendix F allow you to type in the space group, and sometimes the atomic positions as well; diffraction patterns can then be generated that take account of all systematic absences and, in some cases, of double diffraction when it arises.

5.3 The kinematic and dynamical theories of electron diffraction As we saw in Section 3.1, in addition to the contribution of the structure factor, the intensity of a diffracted beam also depends upon the deviation of the reciprocal lattice point from the exact Bragg condition, as shown in Figure 3.6. The intensity also depends upon the thickness of the specimen, t. If the intensity of the incident beam is equal to 1, the total variation in intensity of the diffracted beam can be expressed by the equation: p2

_ sin 2(11:ts ) hkl-

(~S)2

where ~ is a material parameter called the extinction distance that is related to the structure factor, F hkl , by the expression: ~ = 11:Vc ( cos (J)/ AFhkl

where Vc is the volume of the unit cell, A is the wavelength of the electrons and (J is the Bragg angle. ~ is a few tens of nanometers for most reflections of most inorganic materials. The above expression for the intensity is only strictly accurate for very thin specimens because it assumes that the intensity of the diffracted beam is small in comparison with that of the incident beam. These are so called kinematic conditions. In particular, the equation is clearly invalid for very small values of s because the calculated diffraction intensity then becomes equal to (11:t/~)2, which is greater than 1 if the thickness of the crystal is greater than ~/11:, i.e. the diffracted intensity would be greater than the intensity of the incident beam! For crystals thicker than about one third of the extinction distance, when the intensity of the diffracted beam becomes significant and the diffracted wave can itself be re-diffracted (so-called multiple scatter ing), the dynamical theory is needed. The simplest form of this theory considers the interaction between the undeviated beam and one

The intensities of reflections

89

diffracted beam. In other words, this two-beam theory assumes that all other diffracted beams are very weak. The more comprehensive many beam theories that have been developed show that the two-beam theory gives a good approximation to reality. The two-beam theory predicts that, if we define a quantity called effective deviation parameter, s' where: s' =

[S2 +

(i

rr/ 2

then the resultant diffracted intensity for a particular reflection from a perfect crystal of thickness t is given by:

r _ sin2(rcts') hkl-

(SS,)2

which is the same as the kinematic expression, except that s' has replaced s. Now, when s is zero, s' is equal to S- 1 and hkl =sin 2 (rct/S). Note that these equations predict that 'f'2hkl is periodic in t and s'. As a consequence, the intensity of the undeviated beam, 'f'2o is also periodic in a complementary manner as, in order to conserve energy,

r

'f'6 =1- 'f'~kl' In addition to predicting the intensity of the diffracted and undeviated beams, these expressions describe features in the image, such as extinction contours and thickness fringes, very well, particularly when absorption is take into account. Further details of this subject are beyond the scope of this book, but you can find out more from Williams and Carter (1996), Thomas and Goringe (1979) or Hirsch et al. (1965).

5.3.1 Measuring the structure factor, F hk1, and the extinction distance, ~ Clearly, if the structure of a crystal is already known, it is a simple matter to calculate the values of Fhkl and S (tables of the values of fare given in the International Tables for X-ray Crystallography, Volume Ill, MacGillavry and Rieck, 1983, and in Hirsch et al., 1965). However, if the structure is not known, it is a far from straightforward process to determine these values from conventional electron diffraction patterns of inorganic materials because of the way in which the intensities of the reflections depend upon the orientation and the thickness of the sample. In favourable circumstances, however, it is possible to measure Fhkl and S of inorganic materials by convergent-beam and other methods (see, for example, Spence and Zuo, 1992 or Spence, 1992). Biological samples, on the other hand, are often thin enough for kinematic conditions to apply and structure factors can be measured from conventional diffraction patterns (see Misell and Brown, 1987). In favourable circumstances it has even been possible to 'construct' the crystal structures of biological materials by Fourier synthesis. This

90

Electron Diffraction in the TEM

process involves mathematically 'adding together' the diffracted beams in the same way that a lens does (Section 1.1). The amplitudes of the diffracted beams, IFhkZI are obtained from the diffraction patterns and the phases are obtained from images of the specimen (e.g. Unwin and Henderson, 1975).

Exercises 5.1 (a) Write down the co-ordinates of an atom related to an atom in a general position X n , Yn, Zn by a screw diad parallel to the y-axis. (b) From the expression for Fhkz deduce the systematic absences. (c) What is the physical reason for these absences? (d) Look at Table 5.1 and determine what other translational symmetry elements would also lead to these absences. 5.2 The [010] zone-axis pattern in Figure 5.4 was described in the text as an example of the effect of a c-glide plane parallel to (010). What else could produce the systematic absences seen in this section and how could the two possibilities be distinguished?

6 Determination of the Bravais lattice, point group and space group

In this chapter, we will see how electron diffraction can help us to determine the crystal system of a material, its lattice type, its point group and its space group. Most of these methods use a convergent electron beam, a technique that was introduced briefly in Chapter 1. You will need to have a good understanding of crystallography and space groups to follow the material in this chapter. If your understanding is patchy, it is recommended that you first read Appendices A and B, and possibly some of the references at the end of them.

6.1 Determination of the crystal system from conventional electron diffraction patterns With the large tilt angles that are available in modern TEMs it is possible to examine large volumes of reciprocal space. It is, in principle, a straightforward matter to decide whether or not the crystal is cubic, hexagonal or has lower symmetry from observation of the geometries of a series of spot patterns tilted through large angles. However, it is not so easy to distinguish between the systems of lower symmetry by this method. It is important to tilt the sample to prominent zone axes (i.e. ones with low indices), as described in Section 4.3, as these will show the highest symmetry characteristic of the sample. If, for example, no diffraction patterns with four- or six-fold symmetry are found, the crystal cannot be cubic or hexagonal. The angles between prominent zones can also help to identify a crystal as cubic because, in this system, the angles are not dependent on the chemistry of the material (the angles between zones in the cubic system are given in Appendix C.3). 91

92

Electron Diffraction in the TEM

6.2 Convergent-beam methods

6.2.1 Zonal repeats parallel to the electron beam When a convergent electron beam is used to form a diffraction pattern, the range of incident angles leads to a significant excitation of the reflections from the higher-order Laue zones or HOLZs. If the electron beam is exactly along a zone axis of a crystal, as shown schematically in Figure 6.1, it is clear that the spacing, H*, of the reciprocal lattice layers perpendicular to the electron beam, and hence the zone-axis repeat in the crystal, can be derived from the radius, G, of the HOLZs. For the first order Laue zone or FOLZ, assuming the angle ex to be small, from triangle QFP: 2ex= AG l radians and from triangle FOP: ex =H*IG l . Equating the two expressions for ex gives:

H* =GiAl2. Similarly, for the second-order Laue zone, or SOLZ: H*=G~Al4.

The spacing of the reciprocal layers is given by:

H* =N / r[UVWl where r[UVW] is the zonal repeat and the value of N takes account of systematic absences due to lattice type (Section 2.7). N is either 1, 2 or 3, as set out below. • For P or R lattices: N =1 for any axis. • For F lattices: N = 2 if U + V + W is even, otherwise N = 1. • For I lattices: N = 2 if U, V, Ware all odd, otherwise N = 1. • For C lattices: N = 2 if U and V are both odd, otherwise N = 1. • For R lattices where hexagonal indices have been used: N U - V + W =1= 3n, where n is an integer, otherwise N =1.

=3

if

From the FOLZ ring the zonal repeat is therefore given by:

Figure 6.1 . Diagram illustrating the intersection of laue zones with the reflecting sphere when the electron beam is parallel to a zone axis. The zero-, first and second-order laue zones (called the ZOlZ, FOlZ and SOlZ, respectively) are shown.

r r

Determination of the Bravais lattice, point group and space group

r [UVW] =

2N/ (AGi) =

(~) (~

93

where RI (= ALG I ) is the radius of the FOLZ measured on the film and AL is the camera constant. Similarly, from the SOLZ ring: r [UVW]

= 4N

/(AG~) = (~) (;:;

In terms of the unit-cell parameters, the value of the zonal repeat is:

r 2 [lJVW]=UZa 2 + V2b 2 + WZc 2 + 2VWbccos a + 2WUcacosf3 + 2UVabcos y HOLZs are best seen in patterns recorded at a short camera length and

R is most easily measured if a convergent beam with a moderate to large convergence angle is used, i.e. conditions under which the diffracted beams overlap (Kossel pattern). This is because the intensity in an individual HOLZ then appears as one or more continuous rings; compare Figure 6.2a and b. When measuring R, you should measure the innermost ring of the set if there is more than one. It is also better to measure the FOLZ rather than a higher-order ring because, if the scattering angle is too large (a", 10°), the measurements may suffer as a result of lens distortions. The effect of the lens distortion in reciprocal space should be measured using a standard specimen with an accurately known zonal repeat parallel to the electron beam. The distance R and the camera constant ).L should be measured as accurately as possible in order to minimize the errors in H *, as both quantities are squared in the equation

Figure 6.2. [001] CBED patterns from the spinel gahnite, ZnAI 2 0 4 , which is cubic with space group FcI3m (full symbol F4, / d3 2 / m). Patterns were taken at an original camera length of 210 mm in a Philips 400T electron microscope. (a) Pattern taken under microdiffraction conditions in the microprobe mode with a 30 ~m condenser aperture. Individual reflections can be seen in the ZOLZ and the FOlZ. (b) The same pattern recorded under Kossel conditions in the nanoprobe mode with a 1 00 ~m condenser aperture. The FOlZ now consists of a series of closely spaced, continuous rings .

94

Electron Diffraction in the TEM

for r[UVW]. (Note that an error in J.L gives a % error that is different in the HOLZ from in the zero-order Laue zone, or ZOLZ.) The diffraction astigmatism should also be corrected carefully (Section 1.11). The measurement of the zonal repeat parallel to the electron beam allows the presence of polytypes (materials with the same chemistry, but different stacking sequences, and hence different lattice repeats, along one axis) to be detected. It may also allow the distinction between cubic and tetragonal crystals to be made if the diffraction pattern is viewed along [001]. In this latter case, the crystal system can be determined from a set of diffraction patterns from a single axis.

6.2.2 Geometry of CBED patterns from HOLZs The crystal system and lattice type can be determined from the positions of the reflections in the HOLZ compared with those in the ZOLZ. Zone-axis patterns, or ZAPs, need to be recorded in specific directions of high symmetry (Morniroli and Steeds, 1992). In addition, differences between the periodicity of reflections in the ZOLZ and the FOLZ indicate the presence of a glide plane perpendicular to the electron beam. The visibility of reflections in HOLZs may be enhanced by the use of a stage cooled by liquid nitrogen or by reducing the operating voltage (atoms scatter lower-energy, longer-wavelength electrons more strongly, see Figure 5.1). If the FOLZ reflections still cannot be seen, the crystal should be tilted along each of the symmetry elements in the ZOLZ net until reflections belonging to the FOLZ appear, as shown in Figure 3.5.

Finding the crystal system and lattice type. Figure 6.3a shows a [010] microdiffraction pattern of synthetic MgGe03 pyroxene (a single-chain silicate) in which individual spots in the ZOLZ and FOLZ can be seen; in Figure 6.3b, the positions of the reflections relative to each other are shown diagrammatically. The ZOLZ is an oblique, two-dimensional net and, from the extension ofthe x*- and z*-axes into the FOLZ, you can see that the FOLZ stacks vertically above the ZOLZ, except that it is displaced by half a repeat in the x* direction. The reciprocal lattice is therefore monoclinic in shape and it is centred on the C (x*-y*) face; for reflections hOl in the ZOLZ, h = 2n, where n is an integer, whereas in the FOLZ, for reflections hll, h =2n + 1 (see Figure G.2b for a diagram of a C face-centred reciprocal lattice). These observations show that the crystal is C-face centred monoclinic, the y-axis or [010] direction being the unique diad axis in the crystal class. Detecting glide planes by comparing the ZOLZ and the FOLZ. In Figure 6.3, the spacing of the reflections along the z*-axis is halved in the FOLZ compared with the spacing in the ZOLZ. This is the result of the presence of a c-glide plane parallel to (010) in the space group as this type of glide plane results in hOl reflections being absent if 1 is odd see (Table 5.1). Thus, for the ZOLZ, where all the reflections have indices hOl, 1 =2n,

Determination of the Bravais lattice, point group and space group

95

Figure 6.3. (a) [010] microdiffraction pattern of synthetic MgGe03 pyroxene taken at an original camera length of 290 mm with a divergence angle of 1.4 x 10- 3 radians, 120 kV. Individual reflections can be seen in the ZOlZ and FOlZ. (b) Diagram of the pattern in (a). The superposition of the ZOlZ net (shown by the dotted lines) and its extension into the FOlZ shows that the FOlZ stacks vertically above the ZOlZ, except that it is displaced by half the a* repeat. The spacing of the reflections along the z* -axis is also halved in the FOlZ compared with that in the ZOlZ. From this one pattern, it can be concluded that the crystal is monoclinic and that the partial diffraction symbol is C1 c1. The space group is either C2/c or Cc. Reproduced from Champness PE, Mineral. Mag., 1987, with the permission of the Mineralogical Society, London.

whereas for the FOLZ, where the indices are hll, there are no restrictions on the I index. Another example of a glide plane that can be detected by comparison of the geometry of the ZOLZ and the FOLZ is shown in the [001] pattern from spinel in Figure 6.2a . The reflections in the FOLZ have a spacing along x* and y* that is half the value of the spacing in the ZOLZ. This difference is the result of the d-glide plane perpendicular to the z-axis (parallel to the plane of the projection) in the space group Fd'3m (full symbol F41/d '3 2/m) to which spinel belongs. The systematic absences resulting from this symmetry element occur for hkO reflections when h + k i= 4n, where n is an integer (see Table 5.n Also, because of the F lattice, hand k must be even in the ZOLZ, where 1=0 (h, k and I must be all odd or all even, see Table 2.1). In the FOLZ, the reflections have indices hk 1 and the only restrictions on the indices are that hand k must be odd (again because of the F lattice).

Finding the partial extinction symbol. The information that can be obtained from microdiffraction patterns about lattice type and glide planes can be combined in a partial extinction symbol (Morniroli and Steeds, 1992), which looks very like a point-group or space-group symbol (Appendices A and B) and can be used as a first step in finding the full point group or space group. The complete partial extinction symbol for monoclinic crystals can be obtained from the [010] microdiffraction

96

Electron Diffraction in the TEM

pattern alone. The symbol for the pyroxene in Figure 6.3 is C1el. The symbol C indicates the lattice type and the next three symbols refer to the X-, y- and z-axes, respectively. The symbol 1 in the second and fourth positions indicates that there is no symmetry parallel to the x- and z-axes (because the crystal is known to be monoclinic) and the c in the third position indicates the c-glide plane perpendicular to the y-axis. The two possible space groups that would give rise to this partial extinction symbol are C2/c and Cc. The reason why these two space groups cannot be distinguished by means of micro diffraction patterns is that the diad axis in space group C2/c does not lead to any systematic absences in the reflections. However, we will see in Section 6.2.3 that the presence of a diad, or the lack of it, can be detected by other CBED methods. Although a single [010] micro diffraction pattern is sufficient to determine the partial extinction symbol for monoclinic crystals, for the cubic system both < 001 > and < 011 > patterns are needed. The partial extinction symbol for the < 001 > pattern from the spinel in Figure 6.2 is either la •• or Fd •• (Figure 6.4a). Once again, the first symbol is the lattice type and the second refers to the glide plane perpendicular to the X-, y and z-axes (which are equivalent in the cubic system). The two dots that take up the third and fourth positions indicate that nothing can be concluded from the < 001 > pattern about the symmetry along the < 111> and < 011 > directions, respectively. In other words, the pattern could have been produced by an I lattice with an a-glide plane perpendicular to the beam or by an F lattice with a d-glide plane perpendicular to the beam. The two possible < 011> microdiffraction patterns corresponding to the pattern in Figure 6.4a are shown diagramatically in Figure 6.4b and c and are quite distinctive. A microdiffraction pattern of the spinel taken with the electron beam along the axis is shown in Figure 6.4d; clearly, the pattern matches Figure 6.4c and the partial diffraction symbol is Fd ••. The two possible space groups corresponding to this partial diffraction symbol are Fd3m and Fd3. Morniroli and Steeds (1992) provide tables and theoretical microdif fraction patterns that allow the partial diffraction symbol to be determined from experimental micro diffraction patterns for all the crystal systems except triclinic. The patterns may also be drawn with the aid of computer software (see Appendix F).

6.2.3 The symmetry of CBED patterns So far, we have only considered the information that can be obtained from the positions of the reflections in ZAPs. However, there is a wealth of detail within and between the diffracted discs of a CBED pattern recorded at the exact zone axis that can be used to provide information about the point group and space group ofthe crystal. Although a detailed treatment of CBED methods is beyond the scope of this book, I hope, by way of some examples, to give you an idea of what information it is possible to derive from CBED and how it is obtained. Further details about theory and

Determination of the Bravais lattice, point group and space group

97

Figure 6 .4 . (a-c) Some schematic microdiffraction patterns for the cubic system adapted from Morniroli and Steeds (1992) . The partial diffraction symbol is shown in the bottom right-hand corner in each case, the Bravais lattice is given in the bottom left-hand corner (c stands for cubic) and the glide plane perpendicular to the electron beam is g iven at the top. The rec iprocal unit cells in the lOll and the Fall are indicated by rectangles so that their relative sizes are clear. The circled spots in the Fall and the dashed lines through them indicate rows that are aligned with those in the lOll. (a) < 001 > zone-axis pattern for the partial diffraction groups la •• or Fd••. (b) The < 011 > zone-axis pattern for the partial diffraction group 1•• -. (c) The < 011 > zone-axis pattern for the partial diffraction group F •• - . The dash in the fourth position of the symbols in (b) and (c) indicates that there is no glide plane perpendicular to the < 011 > directions. (d) < 011 > microdiffraction pattern from the spinel in Figure 6.2. It matches the schematic pattern in (c) rather than (b), so the partial diffraction symbol is Fd•• .

98

Electron Diffraction in the TEM

methodology can be found in Eades (1988a, 1988b, 1992), Loretto (1994), Spence and Zuo (1992) and Williams and Carter (1996). It is vitally important for the applications described below that the zone axis of interest is exactly parallel to the electron beam. It is usually most convenient do the preliminary sample tilting with a large spot size so that there is plenty of illumination on the screen and Kikuchi lines can be more easily seen. The final stage of centring is difficult to accomplish with the goniometer alone, especially if the crystal of interest is small. Rather than tilt the specimen, the electron beam can be tilted to line up with the zone axis of the crystal. This operation misaligns the microscope (making you unpopular with the next user!) and it must be re-aligned before good images can be obtained. However, the misaligment does not affect the diffraction pattern. The electron beam can be tilted in one of two ways: the condenser aperture can be moved mechanically or, alternatively, the microscope can be operated in the dark-field mode (see Section 3.3.2) and the dark-field tilt controls can be used to tilt the beam. The latter method is preferred as you can easily re-align the microscope by reverting to the bright-field mode. A further practical point: there is a wealth of information in CBED patterns over a broad range of angles (up to 5° or so) and over a broad range of intensities. All this information cannot be recorded in a single film exposure, both because of the scale of the information and because the intensity range is beyond that of any film. Therefore, in recording CBED patterns on film for the purposes of determining crystal symmetry, several exposures are needed. The detail seen in ZAPs when the specimen is sufficiently thick is of two basic kinds: broad, diffuse features within the discs (Figures 6.5b and 6.6a) and sharp lines both within the discs and outside them (Figures 6.2b, 6.6a and 6.6b) The broad contrast in a ZAP arises from dynamic interactions within the ZOLZ (I will call it zero-order information). Because it is associated with quite short extinction distances (Section 5.3.1), it is sensitive to thickness and can, in favourable instances, be used to find the thickness ofthe specimen (see Spence and Zuo, 1992; Williams and Carter, 1996). The symmetry of the zero-order information is the projected, two-dimensional symmetry of the crystal along the zone axis, and belongs to one of the 10 two-dimensional point groups (Table 6.1 and Figure 6.7). The sharp lines within the discs arise from three-dimensional diffraction: they are the result of elastic scattering by the planes corresponding to reflections in the HOLZs. These HOLZ lines (some times called deficit lines) are sensitive to very small changes in lattice parameters and can, in principle, be used to measure the latter to an precision of ~ 0.2% by computer simulation (see Spence and Zuo, 1992; Williams and Carter, 1996). A corollary of this property is that small lattice strains degrade the visibility of the HOLZ lines. The HOLZ lines occur in pairs (like Kikuchi lines) with a bright (excess) line associated with the HOLZ disc responsible for it and a parallel, dark line present in the disc from the undeviated beam (the bright-field disc). The dark

Determination of the Bravais lattice, point group and space group

99

Figure 6 .5 . [100] microdiffraction patterns from the mineral olivine, (Mg,FehSi0 4 . (a) The specimen is sufficiently thin that no dynamic detail is seen in the discs. (b) Microdiffraction pattern from a thicker area of the same specimen. The discs contain broad, fuzzy features that arise from dynamic interactions within the lOll. In (a) the reflections 001 are genuinely absent when I is odd . This absence is the resu lt of an n-glide plane parallel to (010) and a screw diad parallel to the z-axis in the space group Pbnm ( = P 2, / b 2 ,/n 2, /m) . In (b) the 'forbidden' 001 reflections are present, but contain a line of dynamic absence or GM line parallel to z' which indicates that the intensity in these reflections appears by double diffraction. Note that every other reflection along y' is systematically absent because of a b-glide plane parallel to (100) ; these reflections cannot reappear by double diffraction from within the lOll. Reproduced from Champness PE, Mineral. Mag., 1987, with the permission of the Mineralogical Society, London.

lines outside the discs are the result of inelastic scattering from the HOLZ planes. They are the same as the Kikuchi lines that arise from ZOLZ planes in both conventional, SAD and in CBED and are known as HOLZ Kikuchi lines, They are continuous with the HOLZ lines within the discs, but are generally a little less sharp, Because extinction distances for HOLZ reflections are long, typically several micrometres, you will need a thick crystal (several extinction distances) if you want to see sharp HOLZ lines. However, the radius of the HOLZ ring is the most important factor affecting visibility (the smaller the better); the perfection of the crystal is also important. Fig ures 6.2b and 6,6b show HOLZ Kikuchi lines, together with (ZOLZ) Kikuchi lines and excess HOLZ lines. These figures were taken from thick crystals at short camera lengths and moderate to large convergence angles, 2a, the best conditions for observing these features. Identification of phases from ZAPs. As the HOLZ detail is associated with very long extinction distances, it is relatively insensitive to the thickness of the sample. ZAPs from high-symmetry directions can therefore be used as an aid to identification of phases. An atlas of CBED patterns for common alloy phases has been published by Steeds et al. (1984). CBED can distinguish between polymorphs (phases with the same chemical formula, but a different crystal structure) and compounds

100

Electron Diffraction in the TEM

Figure 6.6. [010] CBED patterns of clinopyroxene MgGe03 taken at two different camera lengths, but the same moderate value of 2cx . (a) Pattern taken at a long camera length (1150 mm) showing deficient HOll lines in the bright-field disc and zero-order scattering in the other lOll discs. Both the BF (full) and WP (proj) symmetries are 2. (b) Pattern taken at an original camera length of 290 mm showing Kikuchi bands and excess HOll lines. The WP (full) symmetry is also 2. The first-, second- and third-order laue zones are labelled 1,2 and 3, respectively. Reproduced from Champness PE, Mineral. Mag., 1987, with the permission of the Mineralogical Society, London.

that contain light elements, such as the various borides of molybdenum, which EDX cannot do (Steeds et al., 1984).

Determination of the point group from ZAPs. There are four pieces of information contained in ZAPs that can help you to determine the point group of your material (Eades, 1988a), although, because of variations in experimental conditions, it will not always be possible to determine all of them. The pieces of information are as follows. • The bright-field symmetry, i.e. the symmetry of the sharp HOLZ lines within the 000 disc; here called BF (full). • The projection bright-field symmetry, i.e. the symmetry of the broad features within the 000 disc; here called BF (proj). • The symmetry of the whole pattern, i.e. the symmetry of the HOLZ lines and HOLZ Kikuchi lines in the pattern as a whole; here called WP (full). • The projection symmetry of the whole pattern, i.e. the symmetry of the broad features in the zero-layer discs; here called WP (proj). The first step in finding the point group is to find what is known as the diffraction group of the material. There are 31 of these (Tables 6.2 and 6.3) and they describe the full three-dimensional symmetry of a CBED

Determination of the Bravais lattice, point group and space group

101

Table 6.1. The relationship between the projection diffraction groups and the 2D symmetries of CBED patterns Projection diffraction group

Symmetry of 2D information

1R 21R m1R 2mm1R 31R 3m1 R 41R 4mm1R 61R 6mm1 R

WP (proj)

BF (proj)

1 2

2 2

m 2mm

2mm 2mm

6

3

3m

6mm

4

4

4mm

4mm

6

6

6mm

6mm

After Eades, 1988a.

Table 6 .2 . The relationship between the 31 diffraction groups and the full (3D) symmetries of CBED patterns Diffraction group

1R 2 2R 21R mR

Symmetry of high-order (3D) information WP (full)

BF (full)

1 1 2 1 2 1

1 2 2 1 2

m m1 R

m m

2mRmR

2

2mm

2 RmmR 2mm1R 3 31R 3mR

3m

3m1R 4 4R 41R 4mRmR

4mm

4 RmmR 4mm1R 6 6R 61R 6mRmR

6mm

6 RmmR 6mm1 R

2mm m 2mm 3 3 3

3m 3m 4 2 4 4

4mm 2mm 4mm 6 3 6 6

6mm 3m 6mm

m m 2mm 2mm 2mm m 2mm 3 6

3m 3m 6mm 4 4 4

4mm 4mm 4mm 4mm 6 3 6

6mm 6mm 3m 6mm

Projection diffraction group 1R 1R 21R 21R 21R m1R m1R m1R 2mm1R 2mm1R 2mm1R 2mm1R 31R 31R 3m1R 3m1R 3m1 R 41R 41R 41R 4mm1R 4mm1R 4mm1R 4mm1R 61R 61R 61R 6mm1 R 6mm1R 6mm1R 6mm1R

pattern. Possible point groups can then be found from Figure 6.8, as will be shown later. In favourable cases, the ZAPs from only one high symmetry zone axis are needed to find the point group. Note that it is

102

Electron Diffraction in the TEM

Figure 6.7. Illustration of the 10 two-dimensiona l crystallographic point groups. Reproduced from O' Keefe M and Hyde BG, Crystal

Structures I: Patterns and Symmetry, 1996, with permission of the Mineralogical Society of America.

unnecessary, for the purposes of using Tables 6.1 and 6.2 and Figure 6.8 to find the point group, to understand the meaning of the symbols used for the diffraction groups and projection diffraction groups. The internal symmetry of dark-field reflections at the exact Bragg condition may also be used to help determine the possible diffraction group, as described by Buxton et al. (1976) and Steeds (1979, 1984). However, although the additional use of the dark-field symmetry will uniquely determine the diffraction group for a ZAP (whereas the use of the four pieces of information described above may not), it is often easier and quicker to tilt the crystal to another zone axis or to use other available information about the sample (such as that described in Section 6.2.2) in order to determine its point group. I will illustrate the use of Tables 6.1 and 6.2 and Figure 6.8 with an example. Figure 6.6 shows two [010] ZAP patterns of the MgGe03 pyroxene of Figure 6.3 taken at two different camera lengths. Figure 6.6a shows the BF (full) and the WP (proj) information; Figure 6.6b shows the WP (full) symmetry. (Note that, although the WP (full) symmetry is present in the ZOLZ, the HOLZ detail is often weak, as here, and it is usually better to record a pattern showing HOLZ reflections in order to determine the WP symmetry.) All three available pieces of information show diad (two-fold) symmetry. From Table 6.2, the diffraction group is either 2 or 21R and the projection diffraction group is 21 R. Table 6.1 confirms these findings. Figure 6.8 shows that these diffraction groups are consistent with point groups 21m, 3m (full symbol 32Im), 2 and 32. But, as we found from the microdiffraction patterns that the lattice is

103

Determination of the Bravais lattice, point group and space group

Table 6.3. The diffraction group symmetry seen in CBED patterns from different zone axes Poin.! group

m3m 43m 432

Point group

m3 23

Point group

3mR

< 110 > 2mm1R m1 R 2mRmR

< 111 > 6R 3

< 100 > 2mm1R 2mRmR

< UVO > < UVW >

[001] 6mm1 R 3m1R

< 100 > 2mm1R m1R m1R 2mRmR

m1R 2mRmR

< UVO >

< UVW >

2 RmmR

2R 1 1

3m

6/mmm 6m2 6mm

6mm

622

6mRmR

Point group

6/m

6 6

Point group

3m 3m

32

Point group 4 3

Point group

4/m

4 4

Point group

4/mmm 42m 4mm 422

Point group

mmm mm2 222

Point group

2/m m 2

Point group 1 1

< UVO > < UUW > < UVW >

< 100 > 4mm1R 4 RmmR 4mRmR

< 111 > 6 RmmR

[001] 61R 31R 6 [001] 6 RmmR

3m

3mR

m

mR < 100 > 21R 1R 2

2 RmmR mR

2R 1

< 110 > 2mm1R

2 RmmR

2mm

m

mR

[001] 41R 4R 4

< UVO >

< UVW >

2 RmmR mR mR

2R 1 1

< 100 > 2mm1R 2mRm R m1 R 2mRmR

< 110 > 2mm1R m1 R m1 R 2mRmR

4mRmR [001] 2mm1R

2mm

2mRmR [010] 21R 1R 2

mR

2R 1 1

< uvo > < uuw> < UUW > < uvw>

m

mR mR

2 RmmR

2 RmmR

m m

m m

mR

mR

2R 1 1 1

2R 1 1

< UVW > 2R 1

4mm

2 RmmR

m

< UUW > < UVW > 2 RmmR

[001] 6R 3

[001] 4mm1R 4 RmmR

2 RmmR mR mR

[100].[010] < UOW > 2mm1R 2 RmmR m m1 R mR 2mRmR

< UOW >

< UVW >

2 RmmR

2R 1 1

m

mR

< UOW > < UVO > 2 RmmR mR

m

mR

2 RmmR mR mR mR

< UUW > < UVW > 2 RmmR

m m

mR

2R 1 1 1

< UVO > < UVW > 2 RmmR mR mR

2R 1 1

< UVW > 2R 1

After Buxton et a/. , 1976.

monoclinic C and the space group is either C2/c or Cc, the correct space group is C2/c (point group 2/m), This example shows the power of convergent-beam methods, From one set of diffraction patterns taken along the [010] axis the space group has been determined, A conventional electron diffraction pattern of this axis will give the a, c and f3 cell parameters and the radius of the [010] HOLZ rings can be used to find the b parameter (Exercise 6,2).

104

Electron Diffraction in the TEM

Figure 6 .8 . Relationship between the diffraction groups and the crystal point groups. Note that the higher the symmetry of the diffraction group (i .e. the higher it is in the table), the fewer are the possibilities for the point group. In fact. 11 diffraction groups uniquely define the point group (circled). Reproduced from Buxton et al.• Phi/' Trans. Ray. Soc .• 1976; 281 A: 171 - 193. with permission of the Royal Society.

Determining space groups from dynamic absences. As we shall see in Section 7.1.1, certain reflections (those that should be absent in an electron diffraction pattern because the space group contains a transla tional symmetry element) reappear by double diffraction (Section 7.1) if the crystal is thicker than about 5 nm. The symmetry elements involved are (1) glide planes parallel to the electron beam that have a component of translation perpendicular to the beam and (2) screw diad axes that are perpendicular to the electron beam. Fortunately, when such doubly diffracted spots are recorded under convergent-beam conditions at an exact zone axis, they show a characteristic central line of missing intensity, the so-called dynamic absence or GM line (Gj91nnes and Moodie, 1965; Figures 6.5b and 6.9). The lines of absence are present for all sample thicknesses, occur at all operating voltages and become wider

Determination of the Bravais lattice, point group and space group

105

Figure 6.9. Schematic diagram of the appearance of lines of dynamic absence (represented by the heavy horizontal lines) in a CBED pattern. The GM lines occur in every other diffracted disc in a row containing the bright-field disc.

as the thickness of the specimen becomes smaller. In the kinematic limit (i.e. a very thin crystal), the line of absence fills the reflection completely; the reflection is truly absent, as in Figure 6.5a. The lines of absence occur along a principal axis of the ZAP and are parallel to the g-vectors of the reflections, which is also the direction of the translation causing the dynamic absence. When a forbidden reflection is tilted to be exactly at the Bragg angle, and if three-dimensional effects (i.e. HOLZ lines) are relatively weak, a second black line, perpendicular to the first, is seen in the disc, forming a black cross. As we have seen, lines of dynamic absence or black crosses indicate either that there is a glide plane parallel to the beam, with a glide component perpendicular to it, or a screw diad axis perpendicular to the beam. Note that the 41> 4 3 , 6 1, 6 3 and 6 5 screw axes all include the 21 operation (see Figure B.l). If the diffraction group of the zone axis is known, you can deduce the significance of the GM line, i.e. whether it is the result of a screw axis, a glide plane, or both (Table 6.4). We can use Figure 6.5b as an example of the use of Table 6.4. The diffraction group for the [100] zone axis of olivine (point group mmm) is 2mm1 R (Table 6.3). The single row of GM lines in the OOl reflections for which 1 is odd is therefore the result both of a glide plane parallel to (010) and of a screw diad parallel to the z-axis. The glide plane is an n-glide (i.e. (a + c)/2) as the space group is Pbnm (=P 21/b 21/n 21/m). The identity of the glide plane could be determined by tilting the crystal to the [010] zone axis and recording a microdiffraction pattern. The reflections in the ZOLZ would show absences for h + 1 #- 2n, whereas the FOLZ would show no absences. If the point group of a material is known, the procedure described above will uniquely identify 181 of the 230 space groups. Techniques that can be used to distinguish all but four ofthe others are described by Eades (1988b).

106

Electron Diffraction in the TEM

Table 6.4. Deduction of the origin of GM lines in zero-layer reflections from the diffraction group Single row of zero-layer GM lines

Perpendicular rows of zero-layer GM lines

Cause

mR 2mR mR

2mRmR 4mRmR

Screw axis parallel to each row of GM lines

m

2mm

2mm 4mm

Glide plane parallel to the zone axis and each row of GM lines

2 RmmR

4 RmmR

Glide plane if parallel to WP (full) mirror or screw axis if perpendicular to WP (full) mirror

2 RmmR

Glide plane parallel and screw axis perpendicular to WP (full) mirror

2mm1R 4mm1R

Glide plane and screw axis parallel to each row of GM lines'

m1R 2mm1R

Adapted from Eades, 1988b. 'This is the case for double diffraction routes within the zero layer. If the G M lines are produced by double diffraction via HOlZ reflections, there are space groups for which the GM lines can be produced by a glide plane or a screw axis alone.

6.2.4 The Tanaka method In microdiffraction patterns, such as those shown in Figures 6.5 and 6.6a , the maximum size of each diffraction disc, i.e. the angular field of view, is determined by the Bragg angle as the discs should not overlap significantly. For materials with large unit cells (small distances between spots in the diffraction pattern) this can be a severe limitation if the object is to determine symmetry information from the pattern. A number of methods have been devised to overcome this problem (see Spence and Zuo, 1992; Tanaka and Terauchi, 1985), but the only one that does not require a modification to the microscope is the defocus method due to Tanaka et al. (1980). In this method, the electron beam is focused to a probe as in a normal CBED pattern but, in this case, the focus is not in the plane ofthe specimen but in the plane of the diffraction aperture (the first image plane) (Figure 6.10a). This plane will contain a spot diffraction pattern (Figure 6.1 Ob) and the diffraction aperture can be used to isolate one of the diffracted beams (Figure 6.10c). The microscope is then switched to the diffraction mode and a single disc of the CBED pattern will be seen on the screen of the microscope (Figure 6.11). The method recommended by Eades (1984) for obtaining a Tanaka pattern for the bright-field disc is as follows. • Start with a normal condenser aperture and choose a convenient magnification. • Set the specimen at the eucentric height and focus the image. • Overfocus the objective lens by the desired amount. This is likely to be tens of micrometres (see Table 6.5). Note: the image could be underfocused, but overfocus seems to give better results.

Determination of the Bravais lattice, point group and space group

107

Figure 6.10. Schematic diagrams to illustrate the formation of a Tanaka CBED pattern . (a) The electron probe is focused a distance !:J.f below the specimen, in the plane of the diffraction aperture (the first image plane of the objective lens). (b) A spot diffraction pattern is formed in the plane where the probe is focused. (c) A diffraction aperture isolates one of the diffracted beams and a single disc of the CBED pattern will be seen on the screen of the microscope when it is switched to the diffraction mode. The ray that is drawn in shows that each point in the Tanaka pattern comes from a separate part of the specimen .

• Introduce a diffraction aperture small enough to isolate the undeviated beam and centre it. This aperture is likely to be 5 or 10 Jlm in diameter, considerably smaller than those used for normal SAD . • Switch to the diffraction mode and remove the condenser aperture or exchange it for a larger one. The larger the aperture the larger is the angular field of view. It is preferable to use a large aperture rather than none because the latter procedure introduces spherical aberration. To obtain a Tanaka pattern from a dark-field disc, the same procedure is followed , but the diffraction aperture is moved so that the required diffracted beam passes along the optic axis of the microscope (Section 3.3.2). There is no need to tilt the illumination. One disadvantage of the Tanaka method compared with the standard method of forming a CBED pattern is that, because the probe is not focused onto the specimen, the pattern comes from a larger area than normal and each part of the pattern is obtained from a different part of the specimen (as shown by the diffracted ray in Figure 6.10c); this area depends upon the operating parameters, but can be several micrometres (Table 6.4). Thus, patterns are subject to distortion if there is buckling of the foil or a change in the thickness of the sample. A further disadvantage over the standard method is that a shadow image of the specimen is superimposed on the diffraction pattern. However, there are applications in which a mixture of diffraction and image information can be advantageous (Spence and Zuo, 1992).

108

Electron Diffraction in the TEM

Figure 6.11. Bright-field Tanaka pattern from the 24R polysome of the AI. Sn oxide mineral nigerite. [001] zone axis at 150 kV. The pattern was recorded at a camera length of 1050 mm in the microprobe mode of a Philips EM430 using a defocus value of 60 Ilm and a 200 Ilm C2 aperture. The circle below the pattern represents the size of the largest CBED disc that could be used without overlap in a conventional CBED pattern at this orientation . Table 6.5. The Tanaka method: values of the defocus, !'J.f, that are needed and the diameter, 0 , of the area of the specimen contributing to the pattern for a range of operating parameters mrad (degrees)

p (nm)

Diffraction aperture (Ilm)

10 20 40 60 80

4 30 250 900 2000

0 .2 1 9 30 70

ex (.57) (1 .1) (2.3) (3.4) (4.6)

d-spacing of planes of smallest g in diffraction pattern (nm)

D/ M (Ilm/ Ilm)

0.5/ 6.7 2.8/ 24 8.4/ 52

0.8/ 1.5 1 .0/ 13 5.6 / 47 17/ 105

0.1/ 0.5 0.16/ 4 2.5/ 34 14/ 120 42 / 270

0.02/1 0.32 / 8 5/ 67 28/ 240 84/ 540

0.1

0 .2

0 .5

1 .0

The calculations are for a microscope operating at 100 kV in which the spherical aberration coefficient Cs = 2 mm and the magnification of the image-forming part of the objective lens is 35 x . From Eades, 1 984. * (! > ex; normal CBED can be used. ex = semi-angle of probe; p = diameter of focused probe.

Determination of the Bravais lattice, point group and space group

109

Exercises 6.1 Figure 6.12a is a [001] CBED pattern from a polytype of SiC. Measure the radius of the FOLZ and, from the table below, decide to which polytype the pattern corresponds (hexagonal axes have been used). Voltage 200 kV, A=2.51 pm, camera constant)L= 1.17nmmm. Polytype

c (nm)

Lattice type

4H 6H 5R 21R 27R

1.0053 1.508 3.770 5.278 6.7996

Hexagonal P

Hexagonal P

Trigonal R

Trigonal R

Trigonal R

Figure 6.12b is an enlargement of the bright-field spot. From the symmetry shown in (a) and (b) determine the possible diffraction groups and point groups. Reproduced with the permission of JEOL Ltd from Tanaka and Terauchi (1985). 6.2 Given that the space group of MgGe03 is C2/c and that the camera constant for Figure 6.6b is 0.806 nm mm, determine the lattice repeat along the y-axis. The accelerating voltage was 100 kV (A= 0.0037 nm).

Figure 6.12. (a) [001] CBED pattern from a polytype of SiC, (b) Detail of the bright-field disc. Reproduced from Tanaka and Terauchi, Convergent Beam Electron Diffraction, 1985, with permission of JEOL Ltd .

110

Electron Diffraction in the TEM

6.3 Figure 6.13 shows diffraction patterns from the ceramic BaO.Pr203.4Ti02. (a) [001] zone-axis pattern, showing reflections in the ZOLZ and FOLZ. (b) Microdiffraction pattern of the [100] zone axis. (c) [010] pattern that has been rotated about the z*-axis. (d) [100] CBED pattern taken at a low camera length and with a high convergence angle. What is the space group of the material? 6.4 Determine the WP (full) symmetry of Figure 6.2b . What are the possible diffraction groups and point groups? How could these point groups be distinguished?

Figure 6.13. Diffraction patterns from the ceramic BaO·Pr203·4Ti02. (a) [001] zone-axis pattern, showing reflections in the ZOLZ and FOLZ. (Note: these are much less well separated than usual) . (b) Microdiffraction pattern of the [100] zone axis. (c) [010] pattern that has been rotated about the z' -axis to show detail in the FOLZ. (d) [100] CBED pattern taken at a low camera length and with a high convergence angle. Reproduced from Azough F et aI., J. Appl. Cryst. 1995; 28: 577 581 , with the permission of Munskgaard International Publishers Ltd, Copenhagen, Denmark.

Determination of the Bravais lattice, point group and space group

111

6.5 Al 2 CuLi is known to be hexagonal from X-ray diffraction studies and shows the WP (proj) and WP (full) symmetry given below. What is the point group? Zone axis

WP (proj)

WP (full)

[001] [110] [110]

6mm 2mm 2mm

6mm

2mm

m

6.6 What are the BF (proj) and BF (full) symmetries of the nigerite in Figure 6.11? If the WP (full) symmetry is 3m and the BF (proj) symmetry is 6mm, what is the diffraction group for this pattern and what are the possible point groups?

7 The fine structure in electron diffraction patterns

The fine structure, such as streaks and satellites, present in many electron diffraction patterns contains a great deal of information about the defect structure of the specimen. But, as we shall see, a number of different factors can produce similar effects, and caution must be exercised in interpreting them. In some samples, such as commercial alloys, several different types of defect may be present within a small area. It is therefore imperative to correlate detail in the diffraction pattern with features in the image, in particular by forming dark-field images (Section 3.3.2). In this chapter, we shall look at: • • • •

extra spots; streaks and diffuse reflections; spot splitting and satellites; walls of intensity.

7.1 Double diffraction As we have seen in Section 5.3, electrons are very strongly scattered by atoms (several orders of magnitude more strongly than X-rays, for example). As a consequence, a diffracted beam travelling through a crystal can be rediffracted either within the same crystal or when it passes into a second crystal such as a precipitate or twin, as shown in Figure 7.ia. The process, known as double diffraction, is shown in terms of the reciprocal lattice and the reflecting sphere in Figure 7.ib. The incident beam is AO and, as the reciprocal lattice point hlklll lies on the reflecting sphere at B, a diffracted ray CB is produced. The diffracted ray becomes a potential new incident ray EO with its own reflecting sphere centred at C'. A second reciprocal lattice point h2k2l2 will lie on the new reflecting sphere at F and a doubly diffracted ray C'F is produced. 113

114

Electron Diffraction in the TEM

Figure 7.1 . Double diffraction. (a) The primary beam is incident on a set of planes (h,k,/,) at their Bragg angle 11, . The diffracted beam is then rediffracted from a second set of planes (h2k2/2) at their Bragg angle 112 . (b) The process in terms of the reciprocal lattice and the reflecting sphere. Note that the size of the reflecting sphere relative to the reciprocal lattice is appropriate for X-ray, rather than electron, diffraction . See text for details.

However, the reflection will appear to have come from the set of planes (h3k313) whose reciprocal lattice point lies at F'. If the vector OB is gl, OF is g2 and OF' is g3, the indices of the reflection h3k313, can be found by vector addition. As FF' = OB = gl:

g3=g2 + gl and: h3k 313 =h1 + h2' k1 + k2' 11 + 12

Note that the reciprocal lattice point h3k313 is on the original reflecting sphere and, if it is an 'allowed' reflection (i.e. one with a non-zero structure factor), the double diffraction process will merely add to the intensity produced from the (h3k313) planes by the kinematic diffraction process (i.e. conditions under which no double diffraction takes place).

The fine structure in electron diffraction patterns

115

However, if h3k3l3 is 'forbidden' (i.e. its structure factor is zero) an extra reflection will appear in the diffraction pattern, as explained below.

7.1.1 Double diffraction of 'forbidden' reflections In Section 2.8.2, we noted that certain reflections that are forbidden for the hexagonal close-packed structure appear in the diffraction pattern by double diffraction. Let us look at the [100] = [2110] pattern (see Figure 2.15a) as an example. One set of reflections that are 'forbidden' is OOOl where l is odd. These reflections can appear in the pattern via a number of routes: for instance, because 0111 + 0110 = 0001, the 0001 reflection can appear by diffraction firstly from the (0111) planes and then by rediffraction by the (0110) planes (or vice versa). A graphic way of seeing how doubly-diffracted spots arise is to make two copies of the pattern, the second on tracing paper, and to superimpose the second on the first without rotation, but with the origin of the second pattern displaced to a spot of the first pattern. If you do this for the example given above and displace the origin of the second pattern to the 0111 reflection of the first, you will see that the 0110 reflection in the second pattern lies above the position of the forbidden 0001 reflection in the first pattern. The forbidden reflections described above are the result of the presence of a symmetry element containing a translation (a c-glide plane parallel to (l1001; see Appendix B for an introduction to space groups). Such 'absent' reflections normally reappear in diffraction patterns by double diffraction, but there is one situation where they cannot do so, at least from interactions within the zero-order Laue zone (ZOLZ). This situation occurs when a glide plane is perpendicular to the electron beam. An example is the [010] zone-axis pattern from a crystal that contains a c glide plane parallel to (010) (Figure 6.3). The conditions imposed by the glide plane are that hOl reflections will be absent if l is odd (see Table 5.1). As all the reflections in the [010] zone-axis pattern have indices hOl, half of the reflections will be missing and there is no route for double diffraction to occur from within the zero layer of the reciprocal lattice (try it!). In the [100] zone-axis pattern, on the other hand, the reflections have indices Okl and absences will only occur along the z* direction, i.e. OOl when 1is odd, and therefore there is a route for double diffraction to occur. This situation is similar to that of the example of the hexagonal crystal above. Other examples of patterns in which absences that are the result of glide planes show systematic absences that do not reappear by double diffraction from within the ZOLZ are shown in Figures 6.2 and 6.5. Note, however, that systematic absences that occur in the ZOLZ as a result of a glide plane perpendicular to the zone axis can reappear by double diffraction from planes whose reflections appear in the first-order Laue zone (FOLZ). An example is the < 001 > diffraction pattern of spinel (Figure 6.2) in which the 'forbidden' 200 and 020 reflections can occur by a route such as 1 21 1 + 1 21 1=200 (Smith, 1978).

116

Electron Diffraction in the TEM

No reflections that are absent due to the lattice type not being primitive can reappear by double diffraction. Try finding two indices of 'allowed' reflections in the [001] pattern from the face-centred pattern in Figure 2.13c that add together to give the indices of a forbidden reflection such as 100. You will find that it is not possible because all the reflections in this section have indices that are even numbers. Similarly, double diffraction of reflections in the FOLZ cannot produce forbidden reflections because all the reflections in the FOLZ have indices that are odd numbers. The conditions for absence due to certain lattice types and translational symmetry elements are derived in Chapter 5 and an introduction to space group symmetry is given in Appendix B.

7.1.2 Double diffraction of spots from precipitates and twins Double diffraction can also occur between reflections from different phases and twins, and quite complex patterns can result. Figure 7.2a shows a diffraction pattern from an Al-Mg-Si alloy containing Mg2 Si precipitates in which the double diffraction effects are particularly striking. Both phases are face-centred cubic and they are oriented with the relationship: (100)matrixll(110)precipitate [OOl]matrijl[OOl]precipitate

but the spacing of the (110) planes of the precipitate is slightly larger than the spacing of the (100) planes of the matrix so none of the precipitate and matrix spots coincide in the diffraction pattern. The aluminium matrix pattern and the primary pattern from Mg2 Si are shown indexed in Figure 7.2b. If the matrix reflection 020 is allowed to act as a secondary source for diffraction in the precipitate, the spots shown as open circles in Figure 7.2c result. When all the aluminium spots are considered as possible secondary sources in this way, the pattern in Figure 7.2d is obtained. You can verify this by using the overlay technique described above. The multiple grouping of spots resulting from double diffraction is very common and can also result from surface films and twins (Figure 7.3).

7.1.3 Detection of double diffraction in the microscope You may want to know if particular diffraction spots arise from double diffraction. As the process will only occur if dynamical conditions prevail (i.e. when multiple scattering events can take place) the specimen has to have a certain minimum thickness for double diffraction to be seen in the diffraction pattern. This thickness depends on the structure of the specimen, but for a typical silicate, for example, would be about 50 nm. It follows that ifthe specimen is sufficiently thin, you will be able to record a

The fine structure in electron diffraction patterns

117

Figure 7 .2. (a) Diffraction pattern from a Mg 2 Si precipitate in an aluminium matrix. (b)-(d) The interpretation of (a). The large spots represent aluminium reflections and small spots represent precipitate reflections; open circles represent spots arising from double diffraction. (b) Primary patterns. (c) Double diffraction arising from the 020 aluminium reflection as a secondary source. (d) Complete pattern resulting from double diffraction from the other AI spots acting as secondary sources. giving little squares of doubly-diffracted spots. arising in effect from the big square of the AI pattern . Adapted from Hirsch PB et al.. Electron Microscopy of Thin Crystals. 1965. with the permission of Butterworth Heinemann. London.

diffraction pattern under kinematical conditions and the systematic absences will be apparent, as in Figure 6.5a . Since double diffraction relies on two diffracted beams being excited at once, it is useful to tilt the specimen about 10° from the zone axis about the direction containing the reflection that you suspect is doubly diffracted so that the reflections responsible for the double diffraction are no longer on the reflecting sphere. If the suspect spot is doubly diffracted, it will first be strongly reduced in intensity and eventually disappear. An example is shown in Figure 7.4. Here, the OkO reflections with k odd disappear when the crystal is rotated about y* so that only a systematic row of OkO reflections is present in the ZOLZ. This is because, for example, the 'forbidden' 010 reflection requires a route such as 011 + 001 =010 to appear in the diffraction pattern and the (011) and (001) planes are no longer diffracting in Figure 7.4b. Note that if diffraction is limited to a row of systematic reflections, double diffraction can still occur between the excited reflections. An example of this is Figure 7.2; if the pattern is tilted about x* or y* the row of extra spots parallel to the axis would remain. It is also possible to detect reflections that arise from double diffraction by dark-field imaging (see Section 3.3.2). If the precipitate particle or twin intersects the specimen surfaces, the double-diffraction process will be

118

Electron Diffraction in the TEM

Figure 7.3. (a) {111} twins in a (001) gold film. The dark-field image was formed using a beam produced by double diffraction at the boundary between the twins and the matrix; consequently, only the boundaries appear bright. Reproduced from Pashley DW and Stowell MJ, Phil. Mag. 1963; 8: 1605-1632, with the permission of Taylor and Francis. (b) Schematic [001] diffraction pattern for the foil in (a). The large spots represent matrix reflections and small spots represent primary twin reflections; open circles represent spots arising from double diffraction.

Figure 7 .4 . Diffraction patterns from the synthetic leucite Cs 2 CuSi 5 0'2, which is tetragonal. (a) Approximately [100] zone-axis pattern. (b) The crystal has been rotated about the y* -axis so that only the OkO systematic row of reflections is strongly excited. The OkO reflections with k odd have disappeared because they are forbidden by virtue of the screw diad parallel to the y axis in the space group, P4 2 /n 2, / c 2 / m. (see Table 5.1). The 010 reflection , for instance, requires a route such as 011 + 001 = 010 to appear in the diffraction pattern and the (011) and (001) planes are no longer diffracting in (b).

The fine structure in electron diffraction patterns

119

confined to the interface, which will be bright in the dark-field image using a doubly diffracted spot (Figure 7.3). However, if the particle is entirely confined within the specimen, there will be no obvious differences between dark-field images with doubly diffracted or primary precipitate spots.

7.2 Diffraction from small particles In Section 3.1, we saw that the thin dimension of specimens used in the TEM results in a streak or relrod through each node of the reciprocal lattice. The relrod is perpendicular to the thin dimension of the crystal and its length is lit, where t is the thickness of the crystal. This shape effect applies equally to small particles whose atomic constituents have a different scattering power, {, from that of the matrix. The shape of the reciprocal lattice points or relps depends on the shape of the particles. The shape factors are shown for various shapes of particles in Figure 7.5. The point to remember is that, in the reciprocal lattice, 'small become large' and vice versa: if the particle is a cube with side oflength A, in the diffraction pattern there is a rod of diffuse intensity of length approximately 11A perpendicular to each of the faces of the cube; if it is spherical, there is a diffuse shell around each relp; if it is disc shaped, there is a streak through each relp perpendicular to the plane of the disc;

Figure 7 .5 . The shapes of reciprocal lattice 'points', or relps, for various shapes of particles. Note that the subsidiary maxima shown are so weak that they are unlikely to be visible in a diffraction pattern.

120

Electron Diffraction in the TEM

and if it is rod shaped, there are sheets of intensity through each relp. One example of disc-shaped particles is the presence of the G-P zones in Figure 3.10. The (100) and (010) platelets are oriented parallel to the beam and streaks are visible in the diffraction pattern along the x* and y* directions. The habit plane of the platelets can be determined because it is perpendicular to the direction of the streaks.

7.2.1 The distribution ofstreaks in the diffraction pattern Because the diffraction pattern is a section through the three-dimen sional reciprocal lattice, streaks in the reciprocal lattice can produce either streaks or satellites in the diffraction pattern. If s = 0, a streak tangential to the reflecting sphere will be visible in the diffraction pattern (Figure 7.6a). If, however, s # 0, the reflecting sphere cuts the streaks at an angle such that one or more satellites are formed in the diffraction pattern (Figure 7.6b). A satellite pair formed in this way can easily be hkl reciprocal

lattice point Streak from thin foil dimension

(a)

beam

Re~ting sphere

Streak from disc-shaped particles

s=o Streak

•

Undeviated beam

Diffracted spot Diffraction pattern

(b) hkl

000

soOo Main diffracted spot

Undeviated beam

Satellites Diffraction pattern

Figure 7 .6 . (a) Streaking of reciprocal lattice points arising from disc-shaped particles lying parallel to the electron beam, s = O. (b) Satellites about a reciprocal lattice point resulting from the intersection of the reflecting sphere with inclined streaks at s -# O. Adapted from Edington JW, Electron Diffraction in the Electron Microscope, 1975, with the permission of the Macmillan Press.

The fine structure in electron diffraction patterns

121

distinguished from those resulting from spinodal decomposition or periodic antiphase domain boundaries (see Sections 7.4.1 and 7.4.2) because, in the latter case, the spacing of the satellites from the matrix spot is constant whereas, in the former case, the spacing depends on the value of s. For the discs of intensity produced by rod-shaped particles (Figure 7.5d), the streaks in the diffraction pattern will be straight if the length ofthe rods is perpendicular to the incident beam direction. However, if the rods are at some other angle to the incident beam, the streaks will be curved because of the curvature of the reflecting sphere. It is clear that if the shape of particles is to be investigated from the analysis of the streaks that they produce in the diffraction pattern, it is important to tilt the sample carefully.

7.2.2 The effects of elastic strain We have so far only considered the effect on the diffraction pattern of the size and shape of particles that have a different scattering power from the matrix. However, coherent particles (those whose lattice planes are continuous with those of the matrix) produce an elastic distortion of the matrix if the cell parameters of the two phases are different. This distortion produces diffuse scattering in reciprocal space in the direction of the distortion. The effect can be quite intense, and the diffraction pattern can be a more sensitive indication of the presence of small, coherent particles than the image. However, distortional effects are often present at the same time as shape effects and the two are difficult to separate because they usually occur in the same direction (e.g. in AI-eu, Figure 3.10). The main characteristics of uniaxial elastic strain effects are described by Guinier (1958) and are listed as follows (Figure 7.7).

Figure 7 .7 . Schematic diffraction patterns for different types of particles.(a)Thin, strain-free disc on (001) in which there is a difference in scattering amplitude, t, between the matrix and particles. (b) Distorted, coherent disc on (001) where the unit-cell volume of the particle is smaller than that of the matrix. There is no difference in the scattering amplitude, t , between the particle and the precipitate.

122

Electron Diffraction in the TEM

• The length of the streak increases with increasing g (although this is difficult to observe as each reflection must be tilted to s = 0). • There are no streaks through the undeviated beam. • There are no streaks at spots that arise from planes parallel to the direction of the distortion, e.g. a distortion along [001] will cause streaking of the 001 spot, but not of the 100 or 010 spots. In principle, the above characteristics afford a method of distinguishing between shape and distortion effects, but the occurrence of multiple scattering makes this difficult, except in very thin crystals.

7.3 Diffraction from ordered structures 7.3.1 Long-range order At high temperatures, many metal alloys, minerals and ceramics have disordered structures, i.e. some or all of the atoms are randomly distributed on the atomic sites. At lower temperatures, the atoms may show a preference for certain sites and the structure will become ordered. An example is Al3Li, which is face-centred cubic at high temperatures, with the Al and Li randomly occupying atomic positions at the lattice points. But at lower temperatures the Li atoms occupy the corner positions while the aluminium atoms occupy the face-centring positions; as a consequence the lattice becomes primitive (Figure 7.8a). The result is that superlattice reflections that are forbidden for the face-centred lattice (those for which h , k and l are neither all odd nor all even) appear in the diffraction pattern of the ordered phase (Figure 7.8b). The superlattice reflections are always less intense than the main reflections

Figure 7 .8 . (a) The structure of AI3Li. (b) [001] diffraction pattern of AI3Li . Diffraction pattern reproduced by courtesy of P.P. Prangnell.

The fine structure in electron diffraction patterns

123

because their intensity depends upon the difference between the scattering factors of the ordering atoms (see Section 5.2.2). Another example of an ordered structure of this type is CuZn which is body-centred cubic at high temperatures and orders to the CsCI structure (Section 5.2.2) at low temperatures, with the Cu (or Zn) taking up the body-centring position. In this case, the weak superlattice reflections are those for which h + k + l is odd. In other superlattice structures, the unit cell increases in size as a result of atomic ordering. An example is shown in Figure 7.9b of a diffraction pattern from the mineral nigerite, a tin-and titanium-rich oxide of aluminium and zinc. The 'parent' structure, gahnite, ZnAl2 0 4 , is face-centred cubic (Figure 7.9a), but, in nigerite, the ordering of the tin and titanium in layers parallel to the (111) planes of the parent structure results in the unit cell becoming four times larger in that direction (so the reciprocal lattice repeat is one quarter of that of the parent structure). The unit cell of nigerite is trigonal, rhombohedral, and the superlattice direction is the z-axis, c= 1.86 nm. There are a whole series ofpolysomes of nigerite with different z-axis repeats, the value of which depend upon the tin plus titanium content of the unit cell.

7.3.2 Short-range order Point defects are defects that occur on atomic sites. They may be substitutional atoms, vacancies (empty atomic sites) or interstitial

Figure 7.9. (a) The (112] diffraction pattern from gahnite, ZnAI 2 0 4 , which is face -centred cubic. (b) [210] diffraction pattern from nigerite, a tin- and titanium-rich oxide of aluminium and zinc. In the nigerite, ordering of the tin and titanium in layers parallel to (111) of the 'parent' gahnite structure results in the repeat along (1(I]fcc becomin9. !pur times larger (1.86 nm) and the unit cell becoming trigonal. rhombohedral. Note that [111] of the gahnite becomes z' in nigerite because of the change in the choice of unit cell.

124

Electron Diffraction in the TEM

atoms (ones that takes up positions between normal atomic sites). These point defects can order to give a superlattice, as described above, but if there is an insufficient number to give long-range order, short range order can occur. This short-range ordering can give rise to diffuse scattering and has been described in non-stoichiometric metal carbides with composition around MSC5 , in which the carbon vacancies have ordered in octahedral sites around the metal atoms. Figure 7.10 shows three examples of diffraction patterns from vanadium carbide, which is face-centred cubic. The diffuse intensity occurs as circles and arcs, sometimes around spots and sometimes not. Sauvage and Parte (1972) showed that the diffuse intensity forms a surface in reciprocal space as shown in Figure 7.10d; the diffuse scattering in diffraction patterns is explained by the intersection of the reflecting sphere with this surface.

Figure 7.10. The effect of short-range ordering of vacancies on the (a) [001], (b) [111] and (c) [013] diffraction patterns of non-stoichiometric vanadium carbide. (d) The surface formed by the diffuse intensity in reciprocal space. (a)-(c) reproduced from Lewis MH and Billingham J, JEOL News, 1972, with the permission of JEOL USA Inc.; (d) modified from Sauvage and Parte (1972).

The fine structure in electron diffraction patterns

125

7.4 Periodic and modulated structures

Periodic variations in interplanar spacings, variations in structure factor (i.e. atomic species; see Section 5.2), or both together; or a periodic distribution of crystal defects such as antiphase domain boundaries, crystallographic shear planes or dislocations can lead to the occurrence of satellites in the electron diffraction pattern.

7.4.1 Spinodal decomposition and other compositional modulations Spinodal decomposition is a mechanism by which a supersaturated solid-solution may undergo phase separation without a nucleation stage; instead there is a gradual build-up of composition modulations, which is sinusoidal in the initial stages, in the elastically soft directions in the crystal (see, for instance, Porter and Easterling, 1992). A pair of satellite reflections is present in the reciprocal lattice on either side of each diffracted spot at a distance of 11)" from it, where)., is the wavelength of the modulation. The separation of the satellite spots is in the direction of the modulation (Figure 7.11). Any regular intergrowths of two phases or compositional modulations will produce satellite reflections in the diffraction pattern. Figure 7.12 shows a regular intergrowth of magnetite, Fe304, and amorphous silica, Si0 2, produced by heating the natural mineral fayalite, Fe2Si04, in air. The lamellae of magnetite (the phase showing the dark contrast) have a regular spacing of about 15 nm and are parallel to (110). In the diffraction pattern each spot is surrounded by a row of satellites, spacing 15 nm - 1,

Figure 7 .11 . Electron micrograph of a natural alkali feldspar, Nao.64Ko36AISi30s, that has undergone spinodal decomposition to produce composition modulations parallel to approximately (601) . I nset is an enlargement of one of the diffraction spots that shows satellites in the direction of the modulations. The image and the diffraction pattern are in their correct relative orientation. Reproduced from Owen DC and McConnell, Nature Phys. Sci., 1971; 230: 118- 120 with the permission of Macmillan Magazines Limited, London.

126

Electron Diffraction in the TEM

Figure 7 .12. Electron micrograph of a regular intergrowth of magnetite, Fe304, and amorphous silica, Si0 2 ' produced by heating the natural mineral fayalite, Fe2Si04, in air for 3 days at 800°C. Inset is an enlargement of the undeviated beam, showing satellites parallel to g110 of the magnetite. The image and diffraction pattern are in the correct relative orientation .

parallel to gno (inset, Figure 7.12). Note that here there is a row of satellites, rather than a single pair, as occurs with spinodal decomposi tion, because the modulation is a square wave rather than a sinusoidal one (the explanation lies in the mathematical device known as the Fourier Transform of the two wave forms).

7.4.2 Periodic antiphase domain boundaries At high temperatures, the atoms in the structure of CuAu are disordered and the lattice is face-centred cubic, but at lower temperatures the atoms order so that there are alternate layers of gold and copper atoms parallel to the (lOO) planes and the lattice becomes primitive (Figure 7.13a). This kind of ordering gives rise to antiphase domains: domains in the structure that are 'out-of-step' with each other by half a lattice repeat because the ordering can begin on one of two atomic positions that are equivalent in the disordered structure, i.e. the 'corner' or 'face-centring' positions, but which become distinct in the ordered structure (Figure 7. 13a). An antiphase domain boundary, or APB, exists between regions ordered on different 'registers', i.e. a change-over from, say, Au occupying the corner positions to their occupying the face-centring positions. In CuAuII, the antiphase vector (the vector that would bring the two regions back into register) is 112[110], i.e. one half ofthe diagonal of the face of the unit cell. In CuAu, the antiphase domains are periodic with a domain boundary, on average, every five unit cells along the x-axis (Figure 7,13a). As a result of the periodicity of the APBs, diffraction patterns contain satellite spots (Figure 7.13b). Figure 7.13c shows the row of satellites produced by the periodic APBs from one orientation of the array (there are three possible orientations, all of which will occur,

The fine structure in electron diffraction patterns

127

Figure 7 .13. (a) The unit cell of the periodic anti phase structure in AuCu11. (b) [100] electron diffraction pattern from AuCu11. (c) The position of the satellites produced by one orientation of the periodic APBs. The small, closed circles are the primary satellites and the small. open circles are mainly produced by double diffraction. Notice that there is no intensity at the positions of the superlattice reflections such as 110, only satellites on either side of the positions. Adapted from Pashley DW and Powell MJS, J. Inst. Metals, 1959; 87: 419-428, with the permission of the I nstitute of Materials.

because the x-, y-and z-axes are symmetrically equivalent in the cubic system). The primary satellites occur around the superlattice positions such as 110 (indexed on the original face-centred cubic cell) and their distance from the supedattice positions is l/A, where A is the periodicity of the APBs. Double diffraction largely accounts for the satellites on the undeviated beam and the main spots, although there is a small contribution to these satellites from the periodicity of the structure that can be ascribed to the small change in lattice parameter that occurs at the APB, i.e. the effect described in Section 7.2.2 (Edington, 1975).

7.4.3 Regular dislocation arrays Regular dislocation arrays, such as occur at interphase boundaries, can produce weak satellites perpendicular to the dislocation lines. Examples are shown by Edington (1975) and Williams and Carter (1996). Note that, because of the likelihood of double diffraction, careful tilting to two-beam

128

Electron Diffraction in the TEM

conditions (Section 4.1) is essential to eliminate double diffraction and be certain of the origin of the satellites.

7.4.4 Incommensurate structures In modulated structures and superlattices that involve an increase in the size of the unit cell, the wavelength of the fluctuations is often a simple multiple of the unit cell of the basic substructure, in which case the modulation is said to be commensurate. Examples are the periodic antiphase domains in Figure 7.13, in which domain boundaries occur, on average, every five basic (disordered) unit cells, and the four-fold superlattice in Figure 7.9. However, if the periodicity of the fluctuations is not rationally related to the spacing and/or the orientation of the basic periodicity, the modulations are said to be incommensurate. In the Cu Au system, deviation from CuAu stoichiometry, or the addition of small quantities of other elements, causes the average periodicity of the APBs to vary and the structure becomes incommensurate. The distance of the satellite spots from the superlattice positions in the diffraction pattern is then an irrational fraction of the glOO spacing. The term 'incommensurate' can also be applied to structures such as the spinodal intergrowth in Figure 7.11 or the magnetite/silica inter growth in Figure 7.12.

7.5 Planar and linear defects Stacking faults and thin twins, like small disc-shaped particles, will cause streaking in the electron diffraction pattern (see Figure 3.9a). If a set of parallel lattice planes in the crystal is arranged irregularly, either because the distance between them varies or because they are displaced randomly parallel to themselves by a non-constant amount, then the scattering is limited to rows of the reciprocal lattice that are normal to the lattice planes (Figure 7.14). If, instead of the lattice planes being displaced as described above, the planes are regularly spaced, but displaced randomly parallel to themselves by a specific fraction of the unit-cell dimensions, some of the diffraction spots will be sharp and others will be diffuse. A simple example of such stacking disorder, as shown by the mineral wollastonite, CaSi03 , is illustrated in Figure 7.15. Layers of the structure parallel to (100) are randomly displaced a distance b/2. The corresponding diffrac tion pattern is shown schematically in Figure 7.15b; some spots are sharp while others are diffuse and elongated in a direction normal to the fault planes. The diffuse reflections are diffuse only in the x* direction because the atomic arrangement in the individual (lOO) planes is perfect. Because the relative displacement of neighbouring (100) planes is b/2, the diffuse

The fine structure in electron diffraction patterns

129

Figure 7 .14. (a) Planar disorder in which the planes are identical and parallel. but arranged irregularly. (b) Scattering in reciprocal space is limited to rows normal to the planes in the direct lattice. Reproduced from Guiner A. X -ray Diffraction in Crystals. Imperfect Crystals and Amorphous Bodies, 1963, with the permission of W .H. Freeman and Co.

Figure 7 .15. (a) Diagram representing the stacking shown by the mineral wollastonite, CaSi0 3 • projected onto the (001 ) plane. The dots represent lattice points, which, in turn, represent six CaSi0 3 'units'. (b) Schematic diagram of the [001] diffraction pattern corresponding to (a) . (c) Diagram of the stacking lattice which corresponds to all the lattice points of (a). Reproduced from Willis BMT. Proc. Roy. Soc. Lond., 1958; A248: 183- 198. with the permission of the Royal Society.

130

Electron Diffraction in the TEM

spots are those for which k =I- 2n, where n is an integer. The reason for this can be understood by reference to the stacking lattice, which is represented by the full lines in Figure 7. 15c. All the lattice points in Figure 7.15c lie on this lattice, and therefore they must all scatter in phase in directions corresponding to the diffracted beams from this lattice. Since the horizontal cell edge of the stacking lattice is half the length of the lattice of Figure 7.15a, the corresponding cell edge of the reciprocal lattice must be twice as long as that of the reciprocal lattice of Figure 7.15b. Therefore, the sharp spots of Figure 7.14b correspond to diffraction from the stacking lattice and have indices for which k = 2n. The probability of occurrence of the stacking mistakes determines the length and distribution of intensity ofthe diffuse spots. Figure 7.16 shows four optical diffraction patterns of masks based on the wollastonite structure in which the probability of a mistake in the stacking, p, has been varied. The sharp spots are unchanged throughout and correspond to the common stacking lattice. For a small fault with a probability such as p = 0.1 (i.e. on average one in 10 planes will be displaced) the streaking of the k =I- 2n spots is not very marked, but for p = 0.3 it is significant. For p = 0.8, the majority of the structure is face centred and the diffraction pattern shows diffuse reflections in the face-centring positions. When p = 0.5, there is equal probability of either arrangement and the diffuse spots extend continuously along x*. Finally, if identical, parallel lattice rows of spacing a in the crystal are arranged irregularly with respect to each other, the reciprocal lattice

Figure 7.16. Four optical diffraction patterns corresponding to masks based on the faulting in wollastonite, CaSi0 3 (Figure 7. 15a) with probabilities (a) p = 0.1, (b) p = 0.3, (c) p = 0.5, (d) p = 0.8. Reproduced from Willis BMT, Prac. Ray. Soc. Land., 1958; A248: 183-198, with the permission of the Royal Society.

The fine structure in electron diffraction patterns

131

consists of a family of planes, normal to the rows, and spaced at a distance of lIa.

7.6 Thermal diffuse scattering Walls or sheets of diffuse intensity ascribed to directional thermal vibrations have been reported in a number of metals. These walls lie on {110} reciprocal lattice planes for AI, Au, Si and Ge, and on {111} for IX-Fe, and manifest themselves as diffuse streaks in well-focused (C2 completely overfocused) diffraction patterns taken with exposures of 1-2 min (Figure 7.17). The walls are the result of the scattering of rows of atoms in the < 110> and < 111 > directions, respectively; these are the directions joining nearest-neighbour atoms in the two structures. It is supposed that a prominent mode of thermal vibrations is one in which a whole row of atoms along a < 110 > and < 111 > direction, respectively, is displaced as a unit along its length. The diffuse scattering effects have the following characteristics: • their intensity decreases with decreasing temperature and is particu larly strong near the melting point; • the patterns do not change greatly if the specimen is tilted by up to about 10° from the zone axis.

Exercises 7.1 Show that the 'absences' due to a screw diad parallel to the y-axis (Exercise 5.1) will reappear by double diffraction in electron diffraction patterns from crystals of normal thickness.

Figure 7.17. The effect of thermal diffuse scatteri ng on the [111] diffraction pattern of silicon . Reproduced from Rymer TB, Electron Diffraction, 1970, with the permission of Methuen, London.

132

Electron Diffraction in the TEM

7.2 Figure 7.18 is a [100] diffraction pattern from a disordered silicate. On which planes are the faults and what is the fault vector? Estimate the probability of a fault occurring.

Figure 7 .18. [100] diffraction pattern from a disordered silicate.

Appendix A Some basic crystallography

If you are to study crystalline materials in the electron microscope you need to understand the basic principles of crystallography as set out below. For more details, see one of the texts listed in Section A.6.

A.I Lattices, crystal systems and crystal classes Crystals are regular, three-dimensional arrangements of atoms or molecules. These regular arrays or crystal structures give rise to internal and external symmetry. The repetitive nature of the arrange ments of atoms or molecules in crystal structures leads to the concept of the crystal lattice (an array of atoms or molecules at points in space with identical surroundings). There are 14 Bravais lattices, i.e. ways of arranging repeating points in space (Figure A.I). Each lattice point represents a group of atoms, or motif, with identical surroundings. These lattices amount to seven distinct parallelepipeds or unit cells that are primitive (sometimes called simple), symbol P (or R, signifying rhombo hedral), i.e. they have lattice points only at the corners of the unit cell, and seven other unit cells that have the same shape as one of the primitive ones, but with more than one lattice point in the cell. These are centred cells. The centring may be at the centre of the cell, called body centring, symbol I, at the centre of one face of the cell, usually taken to be the x-y face of the cell, symbol C (sometimes called base centred), or at the centres of all the faces of the cell, symbol F (all-face centring). Crystals are classified on the basis of their external or morphological symmetry into seven crystal systems (triclinic, monoclinic, orthor hombic, tetragonal, hexagonal, trigonal and cubic (sometimes called isometric» (Table A.I). The seven primitive unit cells of the Bravais lattices correspond to five of the seven crystal systems. The exceptions are the hexagonal and trigonal systems; trigonal crystals (defined as having one three-fold axis of symmetry) may have a primitive hexagonal lattice or a rhombohedrallattice. This concept is a rather difficult one and need 133

134

Electron Diffraction in the TEM

Figure A .1 . The unit cells of the 14 Bravais lattices.

only concern you if you are working with trigonal crystals. (For further details see Hahn, 1984 or Hammond, 2001.) The classification of the crystal systems is based on a characteristic or essential symmetry (Table AI). Crystals may have more than the essential symmetry and a further subdivision may be made into 32 crystal classes or crystallographic point groups. These are listed in Table Al in terms of the standard Herrnann-Mauguin symbols used. For an explanation of the meaning of the symbols, see Hahn (1984), Hammond (2001) or Glusker et al. (1994).

A.2 Indexing planes Planes in any of the Bravais lattices can be indexed using a system known as Miller indices. First of all, a unit cell is defined (Figure A2a); the unit cells for the different Bravais lattices are shown in Figure Al.

Appendix A

135

Table A .1 . Crystal lograph ic axial and angular relationsh ips and characteristic symmetry of the crystal systems Crystal classes 1 System (point groups)

Axial and angular relationships

Characteristic symmetry

1, T

a # b # c;

One-fold axis (identity or inversion, i.e. a centre of symmetry)

Triclinic

ex#f3#Y 2, m , 2/m

Monoclinic

a # b # c; ex = y = 90°;

Two-fold axis (rotation or inversion, i.e. perp. mirror plane) this being taken as the y-axis

f3 # 90°

222, mm2, mmm

Orthorhombic

a # b # c; ex = f3 = y = 90°

Two-fold axes (rotation or inversion) in three perpendi cular directions (the X- , y- and z-axes)

4, 4. 4/m, 422, 4mm, 42m, 4 /mmm

Tetragonal

a = b # c; ex = f3 = y = 90°

Four-fold axis (rotation or inversion) along the z-axis

23. m3, 432, 43m, m3m

Cubic

a = b = c; ex = f3 = y = 90°

Four three-fold axes each inclined at 54.73° to the X-, y- and z-axes

3, 3.32,

Trigonal

(Hexagonal axes)2

Three-fold axis (rotation or inversion) along the z-axis

3m, 3m

a = b # c; ex = f3 = 90°; y = 120°

(Rhombohedral axes) Three-fold axis (rotation or inversion) along [111], i.e. the axis that bisects x, y and z

a = b = c; ex = f3 = y # 90° Hexagonal 2

6, 6 , 6/m, 622,6mm, 6m2, 6/mmm

a = b # c; ex = f3 = 90°; y = 120°

Six -fold axis (rotation or inversion) along the z-axis

Note: an n-fold rotation axis rotates a crystal face 360/n° to produce an identical face. An inversion axis, also involves inversion of the face, i.e. a point at x, y, z is inverted to - x, - y, - z. 1 For an explanation of these symbols, see Hahn (1984) or Hammond (2001). 2For the hexagonal and trigonal systems it is customary to take three axes, X-, y- and U- , at 120° to each other and normal to the z-axis.

n,

Axes x, y and z are chosen at angles et, f3 and y with unit vectors a , band c, and magnitudes a, band c. In electron diffraction we are concerned with sets of crystallographically equivalent planes because it is these that 'reflect' the electrons. The Miller index of a set of planes is defined in terms of the intercept that one of the two planes on either side of the origin makes on the axes of the unit cell; for instance, in Figure A.2b the plane nearest the origin cuts the axes at a/h, b/k and ell, and (hkl) are the Miller indices of the set. The Miller indices are therefore the reciprocals of the fractional intercepts of the plane on the unit-cell axes. Figure A.2c shows two planes of the set (221); the plane nearest the origin, 0 , makes intercepts of a/2, b/2 and c on the X-, y- and z-axes, respectively. A negative intercept results in a negative component of the Miller indices, written as h. Note that if we had chosen to label the plane on the other side of the origin we would have derived the Miller indices (hkl).

136

Electron Diffraction in the rEM

Figure A .2 . (a) A unit cell with right-handed axes x, y, z, axial repeats a, band c and axial angles ex, {3, y. (b) The lattice plane from the set (hk/) that is nearest to the origin makes intercepts on the X- , y- and z-axes of al h, bl k and cl l respectively. (c) Diagram showing two unit cells and the two planes of the set (221) that are closest to the origin, O. The one closest to the origin makes intercepts of a12, b l 2 and c on the X- , y- and z-axes, respectively .

A set of planes that are related by symmetry are known as a form. For instance, in a tetragonal crystal that has a four-fold rotation axis the planes (100), (010), (100) and (010) are related by the symmetry. These faces can conveniently be described as the form {lOO} or {O1O} etc. Note the use of curly brackets here. Formulae for the angles between different planes in the seven crystal systems are given in Section C.2.

A.2.1 The hexagonal and trigonal systems For most purposes, the hexagonal unit cell is used for the hexagonal and trigonal systems (Table A.i), even though this results in a unit cell three times the primitive one if the lattice is rhombohedral (see Hammond, 2001). In order to emphasize the three- or six-fold symmetry along the z-axis of the unit cell, four indices, known as Miller-Bravais symbols (hkil) are normally used to index planes in these systems. The extra crystallographic axis, u, is at 120 to the x- and y-axes and normal to the z-axis. As the u-axis is not essential to describe the inclination of a plane in three dimensions, there must be a relationship between h, k and i. It is: h + k = -i. 0

A.3 Indexing lattice directions In order to describe a direction in the lattice, we make use of the concept of vectors. In Figure A.3 the direction OA has the indices [121], i.e. to get from 0 to A we move one unit along the x-axis, two units along the y-axis and one unit along the z-axis, or in vector notation r121 =a + 2b + c. Note the use of square brackets for directions. The [110], [110] and [011] directions are also shown. Note that we can use any origin for the vector; different ones are chosen for convenience for [110] and [011]. In general:

Appendix A

137

Figure A.3. Directions in the lattice. OA is r121 = [121]. Note that we can use any origin for the vector; different ones are chosen for convenience for (iTO] and [011] .

ruvw =[UVW] =Ua + Vb + Wc. We are not concerned with the magnitude of the vector used to describe the direction, so we use the simplest set of whole numbers, i.e. [110] rather than [220] or [V2 V20]. A set of directions that are related by symmetry have the symbol < UVW> or < uvtw > . For instance, < 100> in the cubic system signifies the directions [100], [010] and [001], the X-, y- and z-axes which are crystallographically equivalent. A four-index system [uvtw] known as Weber symbols is sometimes used for directions in the hexagonal and trigonal systems. These symbols can be obtained from the Miller symbols [UVW] from the expressions: 2U - V 2V - U v= t = U+V. w = W. 3 3 3' The reverse conversion (from four- to three-axis zone symbol) can be obtained from: u=

U=u - t; V=v - t; W=w. In this book, both the three- and four-index zone symbols are given for trigonal and hexagonal zone directions. Formulae for the angles between directions in the seven crystal systems can be found in Edington (1975) and may be calculated using many of the computer programs listed in Appendix F. Note that, in the cubic system, a zone axis is parallel to the normal with the same indices. This is not generally true in any other crystal system.

A.4 Zones and the zone law Any two lattice planes intersect in a line that can be described by indices [UVW]. A prism of planes also has a common direction and is known as a

138

Electron Diffraction in the TEM

zone, the common direction being the zone direction. The indices of the zone direction common to two planes hlklll and h2k2l2 can be found from: U = kll2 - k 2l 1; V = llh2 - l2hl; W = hlk2 - h 2k 1.

For a plane (hkl) that lies at the intersection of two zones [U1V1W1] and [U2V 2W 2]: h=V1W 2 - V 2W 1; k=W1U 2 - W 2U 1; l=U1V 2 - U 2V 1.

If you need to know if a plane (hkl) lies in a zone [UVW] the condition is: hU+kV +lW=O.

This is called the zone equation or the Weiss zone law. If the four-axis Weber and Miller-Bravais symbols are used the equation becomes: hu +kv +it +lw = o.

A.5 Software Below are described three interactive software packages that are designed as aids to the understanding of crystallography. Crystallography assumes no prior knowledge of basic crystallography and does not use the stereographic projection. The eight modules are: Introduction, Symmetry I, Symmetry H, Indexing I, Indexing H, Indexing HI, Crystal Systems, Rotations. Available in PC and Macintosh formats from: The Earth Sciences Courseware Consortium, Department of Earth Sciences, University of Manchester, Manchester M13 9PL, V.K. (Tel: 44 (0)161 275 3820; Fax: 44 (0)161 275 3947; e-mail: [email protected]; web-site: www.man.ac.uk/ ~ukescc .html). Introduction to Crystallography also assumes no prior knowledge. The five sections are: Basic crystals, 2-D Crystallography, 3-D Crystal lography, Crystal Structures, Indexing Directions, Planes. Available in PC format from: MATTER Coordinating Office, Department of Materials Science and Engineering, University of Liverpool, Liverpool L69 3BX, U.K. (Tel: 44 (0)151 794 5006; Fax: 44 (0)151 794 4675; e-mail: [email protected]; web-site: http:www.liv.ac.uk/ ~ matterlhome.html). Ca.R.Ine Crystallography (version 3.1) is interactive program for teaching and research that covers real and reciprocal lattices, space groups, stereographic projections, planes and directions. Available in English and French in PC and Macintosh formats from: 17 rue du Moulin du Roy, F-60300 Senlis, France (e-mail: [email protected] or [email protected]).

Appendix A

139

A.6 Further reading Bloss, F.D. (1994) Crystallography and Crystal Symmetry. Mineralogical

Society of America, Washington.

Borchardt-Ott, W. (1995) Crystallography, 2nd Edn. Springer Verlag,

Berlin.

Glusker, J.P., Lewis, M. and Rossi, M. (1994) Crystal Structure

Analysis for Chemists and Biologists. VCR publishers, New York.

Hammond, C. (2001) The Basics ofCrystallography and Diffraction, 2nd

Edn. Oxford University Press, Oxford.

Klein, K. and Hurlbut, Jr., C.S. (1993) Manual of Mineralogy. John

Wiley, New York.

Steadman, R. (1982) Crystallography. Van Nostrand Reinhold, New York.

Appendix B

An introduction to space groups

B.I Screw axes and glide planes In the three-dimensional atomic structure of crystals there are two types of symmetry element that combine a symmetry operation (rotation or reflection) with a translation. A rotation axis with a translation parallel to the axis that is some fraction of the lattice repeat, t, is known as a screw axis, and a mirror reflection with a translation tl2 or tl4 parallel to the reflection plane is known as a glide plane or a glide reflection. The two-, three-, four-, and six-fold rotation axes can be combined with a translation (a one-fold rotation (not shown in Figure B.1) combined with a translation is equivalent to a translation only). Figure B.l and Table B.l show all the possible screw axes, along with their non-translational equivalents. The figure also shows the international graphical and written symbols for the axes, as used in the International Tables for Crystallography (Hahn, 1984). Screw axes are said to be isogonal (from the Greek meaning 'same angle') with the equivalent rotational axes. This means that four-fold screw axes, for example, rotate the motif through 90°, while translating it parallel to the axis. Screw axes are represented by the general symbol N m, where N represents the rotation (two, three, four or six) and m represents the pitch in terms of the fraction of the translation t that is inherent in the operation. For example, the translation involved in the 41 screw axis is Y4t (obtained by dividing the subscript, m, by the main axis symbol, M.There are three four-fold screw axes: 411 42 and 4 3 , with translations of Y4t, Yzt and 3N, respectively. By convention, when mlN is less than Y2, the screw is right handed (a right handed screw is defined as one that advances away from the observer when rotated clockwise). Thus, 41 is a right-handed screw axis with translation Y4t and 43 is a left-handed screw axis, with translation - Y4t = '14; the pair are said to be enantiomorphous. The pairs of screw axes 3 1 and 3 2 , 6 1 and 6 5 , 6 2 and 6 4 are also enantiomorphous. If mlN 141

142

Electron Diffraction in the TEM

Figure B.1. Operation of two- . three- , four- and six fold rotation and screw axes on a single point, represented by a circle. The graphical and written symbols used to describe the axes are shown. The pairs 3,-33 , 4,-43 , 6,-6 5 and 6 r 6 4 are enantiomorphous. Adap ted from Borchardt-Ott W,

Crystallography, 1995,

with the permission of Springer Verlag .

Appendix B

143

Table B.1. Symbols for rotation . rotoinversion and screw axes' Symbol

, 2

Symmetry axis

Graphic symbol

Type of translation (if present)

One-fold rotation

None

None

One-fold rotoinversion Two-fold rotation

--•

None

None

(parallel to paper)

2,

Two-fold screw

•

(parallel to paper)

3

Three-fold rotation

3,

Three-fold screw (right handed)

32

Three-fold screw (left handed)

3

Three-fold rotoinversion

4

Four-fold rotation

4,

Four-fold screw (right handed)

42

Four-fold screw (neutral)

43

Four-fold screw (left handed)

4"

Four-fold rotoinversion

6

Six-fold rotation

6,

Six-fold screw (right handed)

62

Six-fold screw (right handed)

63

Six-fold screw (neutral)

64

Six-fold screw (left handed)

65

Six-fold screw (left handed)

6

Six-fold rotoinversion

.A.

~

~

A

•

•.-•

1/2 c \a or 1/2b None 1/3 c 2/3 c None None 1/4 c 2/4 c 3/4 c

III

None

.-• ••

None

•

*' ~

1 /2 c

\c 2/6 c

1/3 c

3/6 c

1/2 c

4/6 c = 13 c 5/6c None

, All shown normal to the page. unless otherwise indicated.

is equal to Y2 i.e. 21> 42 and 63 , the screw is considered to be neutral in direction. If the translation produced by a glide plane is parallel to the x-axis, it is referred to as an a-glide (translation a/2) and is represented by the symbol a. Similarly, if the translation is parallel to the y- or z-axis, the glide is referred to as b- or c-glide, respectively (Figure B.2 and Table B.2). If the translation is a/2 + b/2, b/2 + c/2 or a/2 + c/2, the operation is known as a diagonal glide plane and is represented by the symbol n. If the translation is a/4 + b/4, b/4 + c/4 or a/4 + c/4, the operation is known as a

144

Electron Diffraction in the TEM

Table B.2. Symbols for reflection planes and glide planes Symbol Symmetry plane

m

Mirror

a, b e n

d

Normal to plane of projection

'l 1-;\ ---------

Axial glide plane

Parallel to plane Nature of glide translation of projection'

I

l

----;.-----

----------

e/ 2 along the z axis a/2 + b/2; a/2 + e/2; b/2 + e/2; or a/ 2 + b/2; + e/ 2 (tetragonal

71

Diagonal glide _._ ._._ ._ . plane Diamond glide plane

a/2 along the x axis or b/ 2 along the y axis

None

......... ..... .. .......

and cubic)

1/71 /"'3/ 8

None

g

a/4 + b/4;b/4 + e/4;a/4 + e/4; or a/4 + b/4 + e/4 (tetragonal and cubic)

'When planes are parallel to the paper, heights other than zero are indicated by writing the vertical coordinate next to the symbol (e.g. 1/ 4 or 3/ 8). The arrows indicate the direction of the glide.

Figure B .2. Glide planes in an orthorhombic crystal whose unit cell is shown shaded. Reproduced from Bloss FD, Crysta/lography and Crystal Chemistry, 1994, with the permission of the Mineralogical Society of America.

diamond glide plane and is represented by the symbol d. Table B.2 gives the standard written and graphical symbols used for glide and mirror planes.

B.2 Space group nomenclature Ifthe 14 Bravais lattices are combined with the symmetry inherent in the 32 point groups (non-translational symmetry), as well as the various glide

Appendix B

145

planes and screw axes, we arrive at the 230 space groups. Each space group is isogonal with one of the 32 point groups. In other words, the point group is derived by replacing the translational symmetry elements in the space group with their non-translational equivalents. As an example, the space group illustrated in Figure 5.5, P4 2/m 21/n 2/m belongs to point group 4/mmm (full symbol 4/m 2/m 2/m), as indicated in the top right-hand corner of Figure 5.5. Another space group that is isogonal with point group 4/m 2/m 2/m is I 4/m 2/c 2/m . There are, in fact, 20 space groups that are isogonal with this point group. Space groups are usually described, as above, by their Hermann Mauguin symbols because they are easy to relate to the corresponding point group, although the International Tables for Crystallography (Hahn, 1984) also gives the Schoenflies symbol for each entry under neath the Hermann-Mauguin symbol (at the top left in Figure 5.5; DM in this case). In the Hermann-Mauguin symbol, the symmetry elements are preceded by the lattice type: P and I, respectively, in the two examples above. One point about the notation for point groups and space groups that may be worth clarifying is the use by crystallographers of what are known as 'abbreviated' symbols. The space group P4 2 /m 21/n 2/m and its isogonal point group 4/m 2/m 2/m are more usually written in the abbreviated forms: P4 2/mnm and 4/mmm, respectively. The reasoning behind the use of the abbreviated symbols is that they show the 'essential' symmetry of the point group or space group; for instance, the intersection of mirror planes every 45° perpendicular to the tetrad (as signified by the second and third m in the point group 4/mmm) dictates that there are also diads at the intersections of these mirror planes. Note that the presence of centres of symmetry is never indicated in point or space group symbols, even in the 'full' versions.

B.3 Space group drawings Each space group is a scaffold-like array of symmetry elements. The International Tables for Crystallography (Hahn, 1984) projects the appearance of each space group onto the x-y plane; that is onto (001). The y-axis is oriented sideways, with the positive direction to the right, the x-axis extends down the page and the z-axis is vertical, towards the reader. The conventional choice of origin is given and is always a centre of symmetry, if one is present. In Figure 5.5 the statement reads: "Origin at centre (mmm)". There are two drawings of each space group. The drawing on the right shows one unit cell with the symmetry elements indicated using the symbols given in Tables B.i and B.2. The second drawing shows the operation of the symmetry elements on an asymmetric motif or group of atoms represented by a small circle. The circle is placed at small fractions x, y, z of the unit cell edges away from the origin, with the height (+)z

146

Electron Diffraction in the TEM

indicated by a + sign. When a symmetry operation such as a reflection plane or centre of symmetry changes the hand of the motif, the circle has a comma inside it. When two motif positions project on top of one another, the circle representing them is split in two by a vertical line, the circle's left side representing one atom and its right side representing the other, as in Figure 5.5. The set of positions generated by the symmetry on the 'starting' position is known as the set of general equivalent positions because the positions do not lie on any of the symmetry elements. The coordinates of these positions are listed below the drawings, together with their total number (16 in Figure 5.5), their Wyckoff letter, k in this case, and the symmetry of the position, 1 (no symmetry). Below the general equivalent positions are listed the special equivalent positions. These are positions whose number is less than the general equivalent positions because they lie on non-translational symmetry elements, i.e. rotation and (roto)inversion axes, mirror planes and centres of symmetry, and the motif is not repeated by these symmetry elements. In Figure 5.5, the number varies from 8 for positions j and i that lie on a single mirror plane, m, to 2 for positions b and a at the intersections of three mirror planes, mmm. (note that this is also where the centres of symmetry are). The right-hand column in Figure 5.5 lists the conditions limiting possible reflections in diffraction patterns, and the first group of entries (headed General) apply to any crystal with this space group. The special conditions listed below the general conditions only apply if all the atoms are in the special positions in the unit cell whose coordinates are listed in the central column. This topic is dealt with in Sections 5.2.1 and 5.2.3 of the main text.

B.4 Further reading Bloss, F.D. (1994) Crystallography and Crystal Symmetry. Mineralogical

Society of America, Washington.

Borchardt-Ott, W. (1995) Crystallography, 2nd Edn. Springer Verlag,

Berlin.

Hahn, T. (1984) International Tables for Crystallography. Volume A,

space group symmetry. Kluwer Academic Publishers, Dordrecht, The

Netherlands.

Hammond C. (2001) The Basics ofCrystallography and Diffraction, 2nd

Edn. Oxford University Press, Oxford.

Klein, K. and Hurlbut, Jr., C.S. (1993) Manual of Mineralogy. John

Wiley, New York.

Appendix C Some useful crystallographic relationships

e.l Interplanar spacings, d hkb and the relationship between direct, a, b, c, a, fJ, r, and reciprocal, a*, b*, c*, ci*, p*, r*, lattice

parameters Orthorhombic:

a* = l/a; b* = lib; e* = lie; a* = [3* = y* = 90° 1

h2

k2

[2

d hkl

a

b

e

-=-+-+ 2 2 2 2 Tetragonal: a = b; cubic: a = b = e Hexagonal and trigonal (hexagonal axes):

a* = b* = 2/(a.j3); e* = lie; a* = f3* = 90°; y* = 60° _1_ 2 d hkl

=i

3

(h2

+ hk + k 2 ) + [2 a2

e2

Trigonal (rhombohedral axes):

a = b = e; a = [3 = y =I 90° a* = b* = e* = (a 2 sin a)/V; cos a* = (cos 2 a- cos a)lsin 2 a where V

= volume of the unit cell = a 3 y'1 -

3 cos 2 a

+ 2 cos3 a 147

148

Electron Diffraction in the TEM

1 d~kl

(h 2 + k 2 + Z2)sin2a + 2(hk + kZ + hZ)(cos2 a - cos a) a 2 (1 - 3 cos2 a + 2 cos3 a)

The rhombohedral lattice can be reduced to the (triple) hexagonal description ai, b':

a' =2a sin (al2),

C'

=a.J3J(1

+ 2 cos a )

Monoclinic:

a* = I/(a sin [3); b* = lib; c* = lI(c sin [3); a* = y* = 90°; [3* = 180 - [3 _1_ = _1_ (h2 + k 2 sin 2 (3 + Z2 _ 2hZ cos (3 ) 2 d hkl sin2(3 a 2 b2 c2 ac Triclinic:

a* = (bc sin a)/V; b* = (ac sin [3)!V; c* = (ab sin y)/V cos a* = (cos [3 cos y-cos a)/(sin [3 sin y); cos [3* = (cos y cos a-cos [3)1 (sin a sin y); cos y* = (cos a cos [3-cos y)!(sin a sin [3) 1 1 2 d2 = V (8 11 h

2 + 8 22k2 + 8 33Z + 2812hk + 2823kZ + 2813hZ)

where V = volume of the unit cell

= abcJl - cos 2 a - cos 2 (3 - cos2 'Y + 2 cos a cos (3 cos 'Y

8 11

= b 2c2 sin2 a

8 12 = abc 2(cos a cos [3-cos y)

8 22

= a 2c2 sin2 [3

8 23 = a 2bc(cos [3 cos y-cos a)

8 33 = a 2 b 2 sin2 y

8 13

= ab 2c(cos

y cos a - cos [3)

C.2

Interplanar angles, p, between planes (h1k111) and (hJl212)

Orlhorhombic:

(h1h2 / a 2) + (k1kdb 2 ) + (hZ2 / C2) cosp = ------r====================== {[(hI/a 2) + (kI/b 2) + (lI/c 2 )][(hVa 2) + (kVb 2) + (ZVc 2)]}

J

Appendix C

Tetragonal: a

149

= b; cubic: a = b = c

Hexagonal and trigonal (hexagonal axes): h1h2 + k1k2 + ~ (h1k2 + h2k1) + (3a 2/ 4c 2)1112 cosp = -----;: -========== ================ {[hi + ki + h1k1 + (3a 2/ 4c2)IiJ[h~ + k~ + h2k2 + (3a 2/ 4c2)1~)]}

!

Trigonal (rhombohedral axes): cos p = (a 4 d 1d 2/y2)[sin 2 r:x(h1h2 + k1k2 + 1112)

+ (cos 2 a - cos a)(k112 + k2lt + 11h2 + 12h1 + h1k2 + h2k1)) Monoclinic: cos p = d 1d 2 [h1h2 sin 2 /3 a 2

+ k1k2 sin2 /3 + 1112 _ b2

c2

(l1 h h

+ 12hI) cos /3 ] ac

Triclinic: cos p

d 1d 2

=- - [Sllh Ih 2 + S22k1k2 + S 331112 + Sza{k112 y2

Sdl1h2 + 12h1) + SdhIk2 + h 2k 1)]

+ k 211 )

150

Electron Diffraction in the TEM

C.3 Angles between planes (or zones) in the cubic system Note that, in the cubic system, a zone axis is parallel to the plane normal with the same indices. This is not generally true in any other crystal system. The indices below represent forms or sets of symmetrically equivalent zones. Therefore, their indices may be permuted, together with their negative counterparts. 100

110

111

210 211

100 110 111 210 211 221 110 111 210 211 221 111 210 211 221 210 211 221 211 221

0.00 45.00 54.74 26.56 35.26 48.19 0.00 35.26 18.43 30.00 19.47 0.00 39.23 19.47 15.79 0.00 24.09 26.56 0.00 17.72

90.00 90.00 63.43 65.90 70.53 60.00 90.00 50.77 54.74 45.00 70.53 75.04 61.87 54.74 36.87 43.09 41.81 33.56 35.26

90.00 90.00 71.56 73.22 76.37

90.00 90.00

90.00 78.90 53.13 56.79 53.40 48.19 47.12

66.42 79.48 63.43 60.00 65.90

78.46 90.00 72.65 70.53 74.21

90.00 90.00 80.40 82.18

Appendix D Relativistic electron wavelengths

Accelerating voltage, V(kV)

Wavelength 1 A (pm)

20 30 40 50 60 70 80 90 100 200 300 400 500 600 700 800 900 1000

8.588 6.978 6.014 5.355 4.865 4.485 4.177 3.919 3.702 2.508 1.968 1.644 1.421 1.256 1.129 1.027 0.942 0.872

pm = 10- 12 m = 10 - 3 nm = 10 - 2 A. Wavelengths were calculated using the equation: 11

A = [hv'2emV] x (1+9.78 x 10 -

7 V) - 1I2

where h (Planck's constant) = 6.626 x 10 - 34 Js; e (charge on the electron) = 1.602 x 10 - 19 C; m (relativistically corrected mass of electron) = mo (1- ~e~2) - 1/2, where mo (rest mass of electron) = 9.110 x 10 - 31 kg and c (the vel~city oflight) = 2.998 x 108 m/s. V is in volts and A is in metres.

151

Appendix E Mathematical definition of the reciprocal lattice

For a simple introduction to vectors and complex numbers and their use in crystallography, see Hammond (2001). a, band c are the unit-cell dimensions of the direct lattice and a*, b* and c* are the dimensions of the reciprocal lattice. These vectors are related by the relations: a*.b = a*.c = b*.c = b*.a=c*.a=c*.b= O. Also: a*.a= b*.b=c*.c= 1 The volume of the direct unit cell Vc is given by a.(b x c) and the volume of the reciprocal unit cell is given by a*.(b* x c*):

a*=~ b*=c~ c*= a x b V'

a=

b* x c*

V

V'

b= c* x a* V

V

c=

a* x b* V

153

Appendix F

Computer programs concerning electron diffraction

There are a number of computer programs available that deal with electron diffraction. Some are designed as teaching aids, but most are designed as aids to the interpretation of diffraction patterns. Below is a list of those known to the author, but it is not guaranteed to be exhaustive! I have only listed the functions relevant to electron diffraction; many of the programs have a number of other functions. It is also worth noting that this field changes very fast! All programs run on PCs unless otherwise stated.

DIFFRACTION (P.J. Goodhew, A. Fretwell, B. Tanovic, I. Jones, A. Green, D. Brook) Free, interactive, on-line educational software from the MATTER team covering an introductory undergraduate course on diffraction (including electron diffraction). Web-site: www.matter.or g.uk/diffraction! ELECTRON DIFFRACTION version 6.8 (J.P. Morniroli.) Simulates spot, ring, Kikuchi and CBED patterns (including large-angle patterns and HOLZ lines). Automatic interpretation of spot patterns from any crystal system other than triclinic. The space group, lattice parameters, atomic species and atomic positions can be input. Crystallographic calculations. e-mail: [email protected]; web-site: www.univ-lillel.frllmpgm IDEALMICROSCOPE (J.M. Zuo, S.H.R. Zhu) for Macintosh. Draws and indexes electron diffraction patterns, including CBED patterns, from crystals of any symmetry. HOLZ and Kikuchi lines can also be plotted. Input data are cell parameters, atomic species and atomic positions. Interactive: changes in patterns can be watched as tilts and other microscope parameters are manipulated. Web-site: www.microscopy online.comNendorslEMLab 155

156

Electron Diffraction in the TEM

JEMS (P. Stadelmann). A Java version of older EMS software suitable for PCs and Macintoshs. Simulates kinematic and dynamical spot diffraction patterns, Kikuchi lines and maps, and CBED (with HOLZ lines). Will index experimental patterns. Input data are cell parameters, space group, atomic species and Wyckoff positions. A version is available free over the Internet. e-mail: [email protected]; web-site: cimewww.epfl.ch WINDOWS CM k·SPACE CONTROL. An on-line program for indexing diffraction patterns and orienting crystals in PhilipsIFEI TEMs. Input data are cell parameters and lattice type. Also shows zone axes and Kikuchi maps, and can instruct TEM stage to tilt to the desired zone axis automatically. Web-site: www.feic.comlsupportlcmks.html MEETINGS AND COURSES. The most comprehensive web-site for information about courses and meetings on electron microscopy all over the world is run by Nestor Zaluzec at Argonne National Laboratory, USA (www.amc.anl.gov). It also has links to microscopy societies world-wide. Another useful source of information on societies and software is the Electron Micoscopy Yellow Pages: cimewww.epfl.ch.emyp/comp.html

Appendix G Answers to exercises

Chapter 2 2.1 The scattering angle et in the equation is equal to 2(}, () being the Bragg angle for the reflection. () is obtained from the equation () ~ }J2d. d 222 =a1J12 (see Appendix C)=0.117 nm, so (}=0.016 radians. This gives a displacement of 98 nm. The Bragg angle at 300 kV is 0.0085 radians and the displacement in the object plane is 5 nm. 2.2 Figure 2.22a is [001] and Figure 2.22b is [011]. The lattice parameter is 0.404 nm. 2.3 The camera constant is 2.9 nm mm. 2.4 The values are a = 0.48 nm and b = 1.02 nm. 2.5 Because the lattice is C-face centred, h + k = 2n, where n is an integer. For the [010] pattern therefore, as k = 0, h = 2n (Figure a.I). The angle f3* is 78°, so f3 = 180 - f3* = 102°. R200 = 5.17 mm, so d 200 = ALIR = 0.46 nm. As d 200 = a sin f3/2, a = 0.94 nm. Similarly doo! = csinf3 and c = 0.53 nm. 2.7 Reflections are absent for a face-centred lattice if h, k and I are not all odd or all even. This leads to the reciprocal unit cell shown in Figure G.2a . For the C-face centred lattice, reflections are absent if h + k i= 2n. This leads to the reciprocal unit cell shown in Figure a.2b.

Chapter 3 3.1 The matrix and precipitate patterns are both from < 110> zones and the 200matrix and 400 ppt spots coincide. Therefore, the orientation relationship is: (l00)o:FJI(100)ppt; [011]o:_FJI[011]ppt. This is the 'cube cube' relationship and could be written in a large number of other 157

158

Electron Diffraction in the TEM

Figure G.1.

Figure G.2.

ways because any two IhkZ} planes and < UVW> directions in the cubic system are parallel. An even simpler way of describing the relationship is: (100)a:_F.//(100)ppt; [010]a:_F.//[010]ppt. As the 200matrix and 400 ppt spots coincide, the d-values for the corresponding planes must be equal and appt = 2a matrix. So the lattice parameter of the precipitate is 0.5732 nm. 3.2 The matrix zone axis is and that of the precipitate is . The matrix 111 and precipitate 110 spots coincide (Figure 0.3).

Appendix G

159

Figure G.3.

Therefore, the orientation relationship is: (111)matrixll(1l0)ppt; [Oll]matnx!/[OOl]ppt. This is known as the Nishiyama-Wassermann relationship.

Chapter 4 4.1 As g2 = (l/d)2 = (h 2 + k 2 + 12)/a 2 , for the (222) planes g = 10.97 nm - 1. (b) The beam is in the symmetry condition with respect to the ± 222 Kikuchi lines, so 8 =g2 ))2=0.223 nm - 1 . (c) From the diffraction patternR=10.5 mm and ~=2.5 mm. 8 =~/R x g2 A=0.10 nm - 1 . 8 is positive, as noted earlier. (d) ~=2 mm and 8=0.08 nm - 1 . 4.2 The pattern shows four-fold symmetry; therefore the zone axis is < 001 >. Because of the extra systematic absences, the spot diffraction pattern will resemble the [001] pattern for diamond cubic (see Figure 2.16) and the shortest g-vectors, and hence the narrowest Kikuchi bands, will be those for the (220} planes. The two narrower Kikuchi bands at approximately 45° to the edges of the page are therefore ± 220, and ± 220 and the wider bands at 45° to the narrow ones are ± 400 and ± 040. The width of the 220 Kikuchi band is 10 mm, which, using the camera constant, gives a value of a = 0.81 nm. You would need to tilt along the ± 400 or ± 040 Kikuchi band to reach the nearest < 110 > zone axis. From [001], the zone would be [011] or [101] as the planes (400) and (040) are parallel to these zones, respectively (Weiss zone law). The angle of tilt would be 45°. 4.3 The d-value for the (200) planes is 0.202 nm, which gives 8200 =0.525°. The width of the 200 Kikuchi band, R 200 , is 8.2 mm. The conversion factor from distance to angle is 28/R =0.128 (see Section 4.4). The values of X and Y in Figure CA are 8.5 and 7 mm, respectively; these values translate to angles of 1.09° about the normal to the (200) planes and 0.90° about the normal to the (022) planes. Using the formula given in Section 4.4, the resultant tilt is 1.4°.

160

Electron Diffraction in the TEM

Figure G.4.

Chapter 5 5.1 (a) An atom related to an atom in a general position X n , Yn, Zn by a screw diad parallel to the y-axis would have the coordinates -Xn, 1I2+Yn> -Zn· (b) The structure factor is: Fhkl

N /2

k

[

]

= ~fn exp21ti(hxn + kYn + lZn) + exp21ti( -hxn + kYn + "2 - lzn) .

If h and I are zero: N /2

[

F OkO = ~fn exp21tikYn

k]

+ exp21ti(kYn + 2") .

If k is odd:

F OkO =

o.

So OkO reflections are absent if k is odd. (c) Physically, by only considering the OkO reflections we are projecting the atoms onto the y-axis, which is effectively halved; so the repeat in reciprocal space is doubled. (d) Absences in the OkO reflections would also occur if there were an n- or a b-glide plane parallel to (001) or (100). However, in both cases there would be other absences in addition to those for OkO reflections. For instance, an n-glide plane parallel to (001) would result in absences for hkO reflections when h + k #- 2n. 5.2 Absences in the [010] pattern for I odd would also occur if the lattice were B-face centred. The two possibilities could be distinguished by

Appendix G

161

tilting the specimen to any other zone, when the general absences in the hkl reflections for the B-face-centred lattice (h + l # 2n) would be apparent.

Chapter 6 6.1 The radius of the FOLZ is 25.5 mm. The formula for the zone-axis repeat, assuming N =1 (P lattice), gives a value of c =1.5 nm, which is the repeat for the 6H polytype. The BF (full) and WP (full) symmetries are both 6mm (the WP (proj) and BF (proj) symmetries are difficult to see). From Table 6.1, the diffraction group is either 6mm1R or 6mm. From Figure 6.8, the possible point groups are 6/mmm or 6mm. 6.2 The radius of the FOLZ is 19.75 mm. The formula for the zone-axis repeat using N = 1 gives a value of b = 0.9 nm. 6.3 The [100], [010] and [001] diffraction patterns are all rectangles or centred rectangles, so the crystal system is orthorhombic. This is confirmed by Figure 6. 13(a) , in which the FOLZ clearly stacks vertically above the ZOLZ. In the [001] pattern the distribution of the reflections in the ZOLZ and the FOLZ is the same. Thus, there is no glide plane parallel to (001). In the [100] pattern the reflections for which k + l # 2n are absent in the ZOLZ, but present in the FOLZ. This behaviour indicates the presence of an n-glide plane parallel to (100). In the [010] pattern the h # 2n reflections are absent in the ZOLZ, but present in the FOLZ. This indicates that there is an a glide plane parallel to (010). The diffraction symbol is therefore Pna-, where the - indicates an undetermined symmetry element: either a mirror plane or a diad. The point group is either mm2 or mmm (see Table A.1). These point groups can be distinguished by the CBED pattern in Figure 6. 13d. The WP (full) symmetry is 2mm. From Table 6.3, point group mm2 shows diffraction group symmetry m1 R along [100], while point group mmm shows diffraction group symmetry 2mm1 R. From Table 6.2, m1 R corresponds to WP (full) symmetry m, while 2mm1R corresponds to WP (full) symmetry 2mm. Thus, the point group is mmm and the space group is Pnam =P2 1/n 21/a 21/m. This is the same space group as olivine (see Figure 6.5), but with the crystal axes specified in a different order. The International Tables for Crystallography (Hahn, 1984) gives tables of the space-group symbols for all the possible settings of the unit cell. 6.4 The WP (full) symmetry is 4mm. From Table 6.2, the possible diffraction groups are 4mm and 4mm1 R. From Figure 6.8, these diffraction groups are consistent with the tetragonal point groups 4/mmm and 4mm, and the cubic point group m3m. Note that other ZAP symmetries at this zone axis would not help to narrow the

162

Electron Diffraction in the TEM

possibilities in this case (see Tables 6.1 and 6.2). Tilting to another zone axis, e.g. [111], would distinguish between them, however. Measurement of the FOLZ ring in Figure 6.2b would give the repeat parallel to the beam and indicate whether the system was cubic or tetragonal (if it is cubic the value must be the same as measured for a and b from the conventional diffraction pattern; if it is tetragonal it would most likely be different). Note that the equality c = a = b is a necessary, but not sufficient, condition for a crystal to belong to the cubic system. The symmetry must conform as well. 6.5 The possible diffraction groups (DG), as deduced from Tables 6.1 and 6.2, are shown in the fourth column of the table below and the hexagonal point groups with which they are consistent are also shown*. The only point group that is consistent with all the ZAPs is 6lmmm . Zone axis WP (proj) WP (full) DG

Possible point group 61m 6mm 6m2 61mmm

[001]

6mm

6mm

*

[110]

2mm

2mm

[111]

2mm

m

6mm or 6mm1 R 2mm or 2mm1 R 2R mmR

* * *

* *

6.6 The BF (proj) symmetry (that of the broad detail) is 6mm and the BF (full) symmetry (that of the fine HOLZ lines) is 3m. Using the other two symmetries given, the diffraction group is 6 RmmR and the two possible point groups are m3m and 3m.

Chapter 7 7.1 Screw axes always result in the systematic absences being confined to a single row in the diffraction pattern and there is therefore always a route for double diffraction to occur. For instance, a screw diad parallel to the y-axis produces absences in OkO reflections when k "# 2n. In a [100] diffraction pattern one route for double diffraction into the 010 reflection is by diffraction by the (011) planes and then re-diffraction by the (001) planes (or vice versa) because 011 + 001 =010. 7.2 The streaking is along z*, so the faults are on the (001) planes. The streaking affects the reflections for which k "# 3n , so the fault vector is bla. As the streaking is continuous, the probability of a fault occurring is about 0.5 or 50%.

Appendix H

References

Azough, F., Champness, P.E. and Freer, R. (1995) Determination of the space group of ceramic BaO.Pr203.4Ti02 by electron diffraction. J. Appl. Cryst. 28: 577-581. Bloss, F.D. (1994) Crystallography and Crystal Symmetry. Mineralogical Society of America, Washington. Borchardt-Ott, W. (1995) Crystallography, 2nd Edn. Springer Verlag, Berlin. Buxton, B.F., Eades, J.A., Steeds, J.W. and Rackham, G.M. (1976) The symmetry of electron diffraction zone axis patterns. Phil. Trans Roy. Soc. 281A: 171-193. Champness, P.E. (1987) Convergent beam electron diffraction. Mineral. Mag. 51: 33-48. Champness, P.E. (1995) Analytical electron microscopy. In: Microprobe Techniques in the Earth Sciences (eds P.J. Potts, J.W.F. Bowles, S.J.B. Reed and M.R. Cave). Chapman and Hall, London, pp. 91-139. Chescoe, D.C. and Goodhew, P.J. (1990) The Operation of the Transmission and Scanning Electron Microscopes, RMS Microscopy Handbook 20. Oxford University Press, Oxford. Cliff, G. and Kenway, P.B. (1982) The effects of spherical aberration in probe-forming lenses on probe size, image resolution and X-ray spatial resolution in scanning transmission electron microscopy. In: Microbe am Analysis-1982 (ed. K.F.J. Heinrich). San Francisco Press Inc, San Francisco, pp. 107-110. Eades, J.A. (1984) Zone-axis diffraction patterns by the "Tanaka" method. J. Electron Microsc. Technique 1: 279-284. Eades, J.A. (1988a) Symmetry determination by convergent-beam diffraction. Proc. 9th European Congress Electron Microscopy, York, 1988. lOP Publishing, Bristol, pp. 3-12. Eades, J.A. (1988b) Glide planes and screw axes in convergent-beam diffraction: the standard procedure. Microbeam Anal. San Francisco Press Inc, San Francisco, pp. 75-80. Eades, J.A. (1992) Coherent-beam diffraction. In: Electron Diffraction Techniques, Vol. 1 (ed. J.M. Cowley). International Union of 163

164

Electron Diffraction in the TEM

Crystallography Monograph 3, Oxford University Press, Oxford, pp. 313-359. Edington, J.W. (1975) Electron Diffraction in the Electron Microscope. Macmillan, London. Gard, A. (1971) The Electron-optical Investigation of Clays. Mineralogical Society Monograph 3, Mineralogical Society London. Gj0nnes, J. and Moodie, A.F. (1965) Extinction conditions in the dynamic theory of electron diffraction. Acta Crystallog. 19: 65-67. Glusker, J.P., Lewis, M. and Rossi, M. (1994) Crystal Structure Analysis for Chemists and Biologists. VCH publishers, New York. Goodhew, P.J. (1984) Specimen Preparation for Transmission Electron Microscopy . Oxford University Press, Oxford. Guinier, A. (1958) Heterogeneities in solid solutions. Sol. State Phys. 9: 293-301. Guinier, A. (1963) X-ray Diffraction in Crystals, Imperfect Crystals and Amorphous Bodies. W.H. Freeman and Co., San Francisco. Hahn, T. (1984) International Tables for Crystallography. Volume A, Space Group Symmetry. Kluwer Academic Publishers, Dordrecht, The Netherlands. Haider, M., Rose, H., Uhlemann, S., Schwan, E., Krabius, B. and Urban, K. (1998) A spherical-aberration corrected 200kV transmission electron microscope. Ultramicroscopy 75: 53-60. Hammond, C. (1993) Stereographic techniques, Module 9.17. In: Procedures for Transmission Electron Microscopy (eds A. Robards and A.J. Wilson). John Wiley and Sons, Chichester. Hammond, C. (2001) The Basics ofCrystallography and Diffraction, 2nd Edn. Oxford University Press, Oxford. Hasan, F., Jahanafrooz, A., Lorimer, G.W. and Ridley, N. (1982) The morphology, crystallography and chemistry of phases of an as-cast nickel-aluminium bronze. Metall. Trans. 13A: 1337-1345. Henry, N.F.M. and Lonsdale, K. (1952) International Tables for X-ray Crystallography. Volume I, Symmetry Groups. Kynoch Press, Birmingham. Hirsch, P.B., Howie, A., Nicholson, R.B. and Pashley, n.w. (1965) Electron Microscopy of Thin Crystals. Butterworths, London. Keyse, R.J., Garratt-Reed, A.J., Goodhew, P.J. and Lorimer GW. (1998) Introduction to STEM. BIOS Scientific Publishers, Oxford. Krivenek, O.L., Delby, N. and Lupini, A.R. (1999) Towards sub-A electron beams. Ultramicroscopy 78: 1-11. Levine, E., Bell, W.L. and Thomas, G. (1966) Further applications of Kikuchi patterns: Kikuchi maps. J. Appl. Phys. 37: 2141-2148. Lewis, M.H. and Billingham, J. (1972) JEOL News 10e(I): 8. Loretto, M.H. (1994) Electron Beam Analysis of Materials. Chapman and Hall, London. Lorimer, G.W. and Champness, P.E. (1974) Mineralogical applications of HVEM. In: High Voltage Electron Microscopy (ed. P .R. Swann). Academic Press, London, pp. 301-311.

Appendix H

165

Lyman, C.E. and Carr, M.J. (1993) Identification of unknowns. In: Electron Diffraction Techniques, Vol. 2 (ed. J.M. Cowley). International Union of Crystallography Monograph 4, Oxford University Press, Oxford, pp. 373-417. MacGillavry, C.H. and Rieck, G.D. (1983) International Tables for Crystallography. Volume D, Physical and Chemical Tables. Kluwer Academic Publishers, Dordrecht, The Netherlands. Misell, D.L. and Brown, E.B. (1987) Electron Diffraction: an Introduc tion for Biologists. Elsevier, Amsterdam. Morniroli, J.P. and Steeds, J.W. (1992) Microdiffraction as a tool for crystal structure determination. Ultramicroscopy 45: 219-239. NIST Crystal Data. Obtainable on CD ROM from NIST Crystal Data Center, NIST, Gaithersburg, MD 20899, USA. O'Keefe, M. and Hyde, B.G. (1996) Crystal Structures. 1. Patterns and Symmetry. Mineralogical Society of America, Washington. Owen, D.C, and McConnell, J.D.C. (1971) Spinodal decomposition in an alkali feldspar. Nature Phys. Sci. 230: 118-120. Pashley, D.W. and Presland, A.E.B. (1959) The observation of anti phase boundaries during the transition from CuAuI to CuAull. J. Inst. Metals 87: 419-428. Pashley, D.W. and Stowell, M.J. (1963) Electron microscopy and diffraction oftwinned structures in evaporated films of gold. Phil. Mag. 8: 1605-1632. Porter, D.A. and Easterling, K.E. (1992) Phase Transformations in Metals and Alloys, 2nd Edn. Chapman and Hall, London. Putnis, A. (1992) Introduction to Mineral Sciences. Cambridge Uni versity Press, Cambridge. Rymer, T.B. (1970) Electron Diffraction. Methuen, London. Sauvage, M. and Parte, E. (1972) Vacancy short-range order in substoichiometric transition metal carbides and nitrides with the NaCI structure. 11. Numerical calculation of vacancy arrangement. Acta Cryst. A28: 607-616. Smith, P.P.K. (1978) Note on the space group of spinel minerals. Phil. Mag. 38: 99-102. Spence, J.C.H. (1992) Accurate structure factor amplitude and phase determination. In: Electron Diffraction Techniques, Vol. 1 (ed. J.M. Cowley). International Union of Crystallography Monograph 3, Oxford University Press, Oxford, pp. 360-438. Spence, J.C.H. and Zuo, J.M. (1992) Electron Microdiffraction. Plenum Press, New York. Steadman, R. (1982) Crystallography. Van Nostrand Reinhold, N ew York. Steeds, J.W. (1979) Convergent beam electron diffraction. In: Introduc tion to Analytical Electron Microscopy (eds. J.J. Hren, J.I. Goldstein and D.C. Joy). Plenum Press, New York, pp. 387-422. Steeds, J.W. (1984) Electron crystallography. In: Quantitative Electron Microscopy. (eds J.N. Chapman and A.J. Craven). Scottish Universities Summer School in Physics, Edinburgh, pp. 49-96.

166

Electron Diffraction in the TEM

Steeds, J.W and the Bristol group (1984) Convergent Beam Electron Diffraction of Alloy Phases (ed. J. Mansfield). Hilger, Bristol. Tanaka, M. and Terauchi, T. (1985) Convergent-beam Electron Diffraction. JEOL Ltd, Tokyo. Tanaka, M., Saito, R., Ueno, X. and Harada, Y. (1980) Large-angle convergent-beam electron diffraction. J . Electron Microsc . 29: 408-412. Thomas, G. and Goringe, M.J. (1979) Transmission Electron Micro scopy of Materials. John Wiley, New York. Unwin, P.N.T. and Henderson, R. (1975) Molecular structure determination by electron microscopy of unstained crystalline speci mens. J. Mol. Bioi. 94: 425-440. Villars, P. and Calvert, L.D. (1985) Pearson's Handbook of Crystal lographic Data for Intermetallic Phases. ASM, Metals Park, Ohio. Wells, A.F. (1984) Structural Inorganic Chemistry, 6th Edn. Oxford University Press, Oxford. Williams, n.B. and Carter, C.B. (1996) Transmission Electron Micro scopy. A Textbook for Materials Science. Plenum Press, New York. Willis, B.T.M. (1958) An optical method of studying the diffraction from imperfect crystals. III Layer structures with stacking faults. Proc. Roy. Soc. A 248: 183-198.

Index

Abbe criterion, 2

Aberration, spherical, 7, 9-10, 15-16,65, 107

constant, 10

error in diffraction pattern from,

9-10

Alignments of instrument, 22-23

Allowed reflections; see Systematic absences

Amorphous materials; see Diffraction, pattern

from amorphous materials Amplitude of diffracted beam; see Structure factor; Wave, amplitude of Angle

Bragg; see Bragg angle

convergence; see Convergence angle

scattering, 10, 81

Antiphase domains, periodic, diffraction from,

121, 126-127

Aperture

condenser 1, 4; see also Spot size

condenser 2, 4, 11-12, 15-16, 21, 22,

98, 106-107; see also Convergence angle

centring of, 16, 21

diffraction, 6-9, 11, 19, 75, 106-107

objective, 4-5, 7, 19-22, 65-66

selected-area; see Aperture,

diffraction

virtual, 6

Astigmatism, 65

in the condenser lens, 16, 21-22

in the diffraction lens, 20, 22-23, 49, 94

correction of, 22-23

Atomic scattering amplitude, 81-82

Beam

coherence, 20

convergence; see Convergent beam

electron diffraction damage, 11, 17-18, 37

displacement, 18

heating, 17

ionisation, 17

knock-on, 18

diffracted, 1-3,9-10, 28-31, 56-57,

71; see also Bragg reflection

amplitude of; see Structure factor

intensity of, 57, 82, 88-89, 114

incident, 11, 30, 70

two-beam conditions; see Two-beam,

conditions

spreading, 16

stop, 20, 65

undeviated, 9, 21, 29-30, 34, 52, 55, 77, 98,

100, 106

Beam-sensitive specimens; see Beam damage

Black cross, 105

Bloch waves, 69

Bragg

angle, 29, 39, 55-56, 65-66,69-70, 73, 105,

106

condition, deviation from; see

Deviation parameter

Law, 28-31, 56

reflection, 28, 56

Bravais lattice; see Lattice, Bravais Bright-field (BF)

disc, 98, 100

image, 65

symmetry; see Symmetry, in CBED

Buxtons tables, 100-104

Camera constant, 31, 42, 48-50, 93

ca libration of, 49-50

Camera length, 7-8, 17, 20,22,23,30,93,102

Coherence; see Beam, coherence

Commensurate modulations, 128; see also

Satellites

Composition plane of twin, 62-64

Condenser lens; see Lens, condenser

Conjugate plane, 1

Constructive interference; see Interference of

waves

Convergence angle, 11-12, 15, 21, 93, 99

Convergent-beam electron diffraction, 11-16,

92-108

patterns, symmetry of, 96-104

spatial resolution of, 14-16

Cooling the specimen, 11, 17,20,94, 131

Cross section, capture, 17

Crystal class; see Point group, crystallographic

Crystal system, 133-134

determination of, 91, 94

lattice; see Lattice, crystal

Damage; see Beam damage Dark-field

image, 65-66,113,117-119

reflections, internal symmetry of, 102

tilt controls, 65, 98

167

168

Electron Diffraction in the TEM

Defects, planar and linear, 128-131; see also Ordered structures; Dislocations, regular arrays; Incommensurate structures Deficit lines; see HOLZ lines

Defocus method; see Tanaka method

Deviation parameter, 59, 71, 73-74

effective, 89

sign of, 59, 73-74

Diamond structure, diffraction from, 45--46

Diffracting plane, 28, 31-35, 56

Diffraction

aperture; see Aperture, diffraction convergent-beam electron (CBED); see Convergent-beam electron diffraction group, 100-105; see also Projection diffraction group pattern, 1, 6-8; see also Reciprocal lattice

centring of, 20

focusing of, 20-21, 23, 49

from amorphous materials, 37

from periodic dislocations, 127-128

from powder specimens, 37, 40

from single crystals, 31-36

inversion of; see Inversion of image

wrt diffraction pattern

micro-micro, 16

Riecke,16

rotation of wrt image; see Rotation

between image and diffraction pattern

selected-area; see Selected-area diffraction

vector, g; see Reciprocal lattice, vector

Diffuse reflections, 119-122, 123-132; see also

Streaking

Diffuse scattering, 69

thermal, 20, 131

Dislocations; regular arrays, 127-128

Double diffraction, 45, 84, 88, 104, 113-119,

127-128

detection of, 116-119

from FOLZ to ZOLZ, 115

offorbidden reflections, 115-116

of precipitate spots and twins, 116

Dynamic absences (GM lines), 104--105

Dynamical theory of electron diffraction, 88-89

EELS (electron energy-loss spectroscopy), 52

Elastic strain, effects of, 121-122

Electron

diffraction; see Diffraction

probe, 11-12, 14--16, 106-107

size, 14--16

gun, 4, 16

field-emission, 16

lanthanum hexaboride, LaB6 , 16

wavelength, 25, 56, 151

Electropolishing, 17

Energy-dispersive X-ray analysis (EDX), 17,52

Equivalent positions in space group

general, 86, 146

special, 45, 88, 146

Error

focusing, 8

excitation; see Deviation parameter

Eucentric plane, 9,19,2123,49,63,65,77,106

Ewald sphere; see Reflecting sphere

Excitation error; see Deviation parameter

Exposure time, 17,20,98

Extinction contour, 18, 89

Extinction distance , 88-89, 98, 99

Extinction symbol, partial, 95-96

Focal length, 1,5,9 Focal plane; see also Lens back, 1,9,11,20,65,70-71 front, 1,5 Focal point, principal, 1,9; see also Lens

Forbidden reflections; see Systematic absences

Form, 62, 64, 136

Fourier

transform, 126

synthesis, 89

Full width at half maximum (FWHM), 14

Full width at tenth maximum (FWTM), 14

g-vector; see Reciprocal lattice, vector

Gaussian intensity, 15

Glide plane, 45, 84, 86, 94--95, 115, 141, 143 144

diagonal, 86, 105, 143-144

diamond, 95, 96-99, 144

GM lines; see Dynamic absences

Goniometer height; see Eucentric plane

GP zones, 64, 120

Gun; see Electron gun

Habit plane, determination of, 62-65, 120

Hermann-Mauguin symbols; see Space group,

nomenclature; Point group, crystallographic

Hexagonal close-packed; see Reciprocal lattice,

for hexagonal close-packed

HOLZ (higher-order Laue zone), 57, 92-95

Kikuchi lines, 99

lines, 98

excess, 99

geometry of, 94--95

ring,99,103

Identification of unknown phases, 52, 99-100

Image

focus of, 8-9, 19, 21, 49

formation of, 5-6, 9, 89-90

inversion of wrt diffraction pattern;

see Inversion of image wrt

diffraction pattern

relation to diffraction pattern, 2, 30-32,

60-66

rotation of wrt diffraction pattern;

see Rotation between image and

diffraction pattern

Incommensurate modulations, 128

Indexing diffraction patterns, 38, 40-49

180 ambiguity in, 35

by computer, 45-49, 155-156

from standard patterns, 40-45

Indices Laue; see Laue indices Miller; see Miller indices Inelastic scattering, 69-71

0

Index Intensity of diffracted beam; see Wave, intensity of; Beam, diffracted, intensity of

Interference of waves, 26-28

International Tables for Crystallography, 86,

89, 141, 145

Inversion of image wrt diffraction pattern, 2,

50-51

Ion thinning, 17

Isogonal, 141, 145

Kikuchi diffraction, 69-78

band, 71, 74-76,

line, 69-74, 98-99; see also HOLZ

Kikuchi lines

maps, 74-77

symmetry, 75

Kinematic conditions for electron diffraction, 88-89,114 Kinematically forbidden reflection; see Systematic absences Knock-on damage; see Beam damage Kossel cones, 71

patterns, 11, 93

Kossel-Mollenstedt patterns; see

Microdiffraction patterns

Lattice

Bravais, 38-41,46, 92,133-134, 144

determination of, 94

crystal (direct), 4, 34-36, 133

plane, 39, 134-136, 218

spacing, 28-31, 49-50, 147-148,

149-150

angles between, 71, 148-150

reciprocal; see Reciprocal lattice

Laue indices, 30

Laue zone

first-order (FOLZ), 57, 92, 94-95

higher order (HOLZ), see HOLZ

second-order (SOLZ), 92

zero-order (ZOLZ), 57, 94-95

Lens

aberrations; see Aberrations

auxiliary, 12-14, 21

condenser 1, 7-8, 12, 20; see also

Spot size

condenser 2, 7-8, 12, 19-21, 65

condenser-objective, 11, 14

diffraction, 6, 8, 20

distortion, effect of on diffraction

pattern, 93

electromagnetic, 4

focusing of electromagnetic, 4-5

formation of image and diffraction

pattern by, 1-2

intermediate, 4

mini, 12,21

objective, 2, 6, 8-9, 11-12, 21, 65, 106

optic axis of, 1-2, 9

polepiece of, 4

prefield, 12, 14

projector, 4, 6, 8, 50

ray diagram for, 2

169

Long-range ordering, see Ordered structures Magnification of diffraction pattern; see Camera length

Magnification of lens, 6

Many-beam theory of electron diffraction, 88 89

Microdiffraction patterns, 11, 94-96, 105

Miller-Bravais indices, 35, 136

Miller indices, 28, 134-135

Mode; see also Bright field; Dark field

micro-probe, 11

nano-probe, 11, 13, 15

TEM, 11, 16, 21

STEM, 11-13, 15, 21-22

Micro-probe mode; see Mode, micro-probe Modulated structures, diffraction from, 125 127; see also Commensurate modulations;

Incommensurate modulations; Satellites

Motif, 39, 133, 145-146

Multiple scattering; see Double diffraction

Nano-probe mode; see Mode, nano-probe Optic axis, 1-2, 9

Ordered structures, diffraction from; see

Commensurate modulations;

Incommensurate modulations; Satellites

long-range, 122-123

short-range, 123-124

Orientation

exact, determination of, 73, 78

relationships, determination of,

60-65

for particles, 60-61

for twins, 61-62

Overfocus, 106; see also Lens Path difference; see Wave, path difference of

Phase difference; see Wave, phase difference of

Point group, crystallographic, 134, 144, 145

determination of, 100-104

two-dimensional, 98, 102

Polytypes, 94

Powder Diffraction File, 46-48

Projection diffraction group, 102

Radiation damage; see Beam, damage

Reciprocal lattice, 4, 25, 31-35, 71, 147-148,

153

for cubic crystals, 40-42, 45-46, 96

for hexagonal close-packed crystals,

42-45, 62-63, 115

for monoclinic crystals, 34-35, 94-95

for orthorhombic crystals, 34

for P hexagonal/trigonal crystals,

35-36

parameters, relation to direct lattice

parameters, 147-148

rod (relrod), 57, 119-122

vector, g, 32, 56, 71

Reflecting sphere, 55-59, 71, 113-115

Reflections from planes

forbidden; see Systematic absences,

170

Electron Diffraction in the TEM

systematically absent; see Systematic absences

Relativistic effect, 26, 151

Relrod; see Reciprocal lattice, rod

Ring pattern; see Diffraction pattern from

powder specimen

Rotation between image and diffraction

pattern, 50-52

Satellites, 120-122, 125-128

Scan coils, 4, 12

Scanning transmission electron microscope,

(STEM), see Mode, STEM Scattering, 1; see also Angle

elastic, 69, 98

inelastic, 69-74, 99

multiple; see Double diffraction

thermal diffuse, 131

Schoenflies symbol; see Space group, nomenclature Screw axis, 86-87, 104--106, 141-143; see also Space group Selected-area diffraction (SAD), 6-8, 19-20

aperture; see Aperture, diffraction

error in, 8-11

Semiangle; see Angle; Bragg angle

Shape effect, 119-121

Short-range ordering; see Ordered structures

Space group, 46, 52, 86-88, 94, 104--105,

141-146

determination of, 104--106

nomenclature, 144--146

Specimen

cooling; see Cooling the specimen

holder, 5,11, 17,98

preparation, 16-17

thickness, 16,45,57,69,88,98,99,

104--105, 107, 116, 119

orientation of, importance of, 64-65

tilting of, 57, 62-63, 65, 71, 73,

76-77,89,91,94,98, 105, 117, 131

Spherical aberration; see Aberration, spherical

Spinel structure, diffraction from , 95, 115

Spinodal decomposition, 121, 125-126, 128

Spot size, 8, 12, 20-21, 98

Stacking faults, streaks from, 128-131

Stacking lattice, 129-130

Staining, negative of biological specimens, 17

Standard patterns

for cubic crystals, 40-42, 45-46

for hexagonal close-packed crystals, 42-45

STEM mode; see mode, STEM

Stereographic projection, 65

Stigma tors, 22

Streaking, 119-122, 128-131

from small particles, 119-123

from stacking faults and twins, 128-131

Structure factor, 81-85, 89-90

Superlattice, reflections from, 122, 126-127

Surface layer, removal of, 17

Symmetry; see also Point group; Space group;

Kikuchi diffraction, symmetry

condition, 74--75

elements, 134--135, 141-144

in CBED

bright-field, 98, 100-102

projection bright-field, 100-101

projection symmetry of whole

pattern, 100-102

whole pattern, 100-102

translational, 84--88, 141-144; see also Glide

planes; Screw axes

zone-axis, 75

Systematic absences, 38-40, 45, 83-84, 115,

117,146; see also Dynamic absences

due to lattice type , 38-40, 83-84, 116

due to translational symmetry, 84--88

due to atoms in special positions, 45, 146

tied conditions, 87

Systematic row of reflections, 117

Tanakamethod,106-108

TEM mode; see Mode, TEM

Tilting the specimen; see Specimen, tilting of

Trace analysis, 64

Twin plane, 62, 64

Twinned crystals, diffraction from, 62-64, 117,

128; see also Orientation, relationships, determination of for twins Two-beam

conditions, 71, 73, 127-128

theory of electron diffraction, 88

Unit cell, 28, 133; see also Lattice

scattering amplitude from; see Structure

factor

volume of, 153

Vacancies, 123

Viewing screen, 4-6, 8, 21-22, 65

Voltage, operating, 11, 18, 26, 81, 94, 104

Wave, 25-28; see also Interference of waves

amplitude of, 25, 81-83

displacement of, 25

intensity of, 25, 82

path difference of, 27, 39, 82

phase difference of, 82, 90

Wavelength; see Electron wavelength

Weber symbol, 137

Weiss Zone Law, 32,138

Whole-pattern symmetry; see Symmetry, in

CBED z control, 9, 19

Zone axis, 31, 41, 75-77,105,136-138; see also

Weber symbol

angles between, 137, 150

high-symmetry, 64-65, 91, 94, 99, 101,

patterns (ZAPs), 75, 94, 96-100, 104

repeat, determination of, 92-94, 103

symmetry, 75

Zone direction; see Zone axis Zone equation; see Weiss Zone Law